Pet Packaging Technology
Pet Packaging Tech text...
PET Packaging Technology
Sheffield Packaging Technology Series Editor: Geoff A. Giles, Global Pack Management, GlaxoSmithKline, London. A series which presents the current state of the art in chosen sectors of the packaging industry. Written at professional and reference level, it is directed at packaging technologists, those involved in the design and development of packaging, users of packaging and those who purchase packaging. The series will also be of interest to manufacturers of packaging machinery. Titles in the series: Design and Technology of Packaging Decoration for the Consumer Market Edited by G.A. Giles Materials and Development of Plastics Packaging for the Consumer Market Edited by G.A. Giles and D.R. Bain Technology of Plastics Packaging for the Consumer Market Edited by G.A. Giles and D.R. Bain Canmaking for Can Fillers T.A. Turner PET Packaging Technology Edited by D.W. Brooks and G.A. Giles
PET Packaging Technology Edited by DAVID W. BROOKS Corporate Technologies Crown Cork & Seal Oxford
and GEOFF A. GILES Global Pack Management Gl axoS mithKline London
Sheffield Academic Press
First published 2002 Copyright © 2002 Sheffield Academic Press Published by Sheffield Academic Press Ltd Mansion House, 19 Kingfield Road Sheffield SI 1 9AS, UK ISBN 1-84127-222-1 Published in the U.S.A. and Canada (only) by CRC Press LLC 2000 Corporate Blvd., N.W. Boca Raton, FL 33431, U.S.A. Orders from the U.S.A. and Canada (only) to CRC Press LLC U.S.A. and Canada only: ISBN 0-8493-9786-3 All rights reserved. No part of this publication may be reproduced, stored in a retrieval system or transmitted in any form or by any means, electronic, mechanical, photocopying or otherwise, without the prior permission of the copyright owner. This book contains information obtained from authentic and highly regarded sources. Reprinted material is quoted with permission, and sources are indicated. Reasonable efforts have been made to publish reliable data and information, but the author and the publisher cannot assume responsibility for the validity of all materials or for the consequences of their use. Trademark Notice: Product or corporate names may be trademarks or registered trademarks, and are used only for identification and explanation, without intent to infringe. Printed on acid-free paper in Great Britain by Antony Rowe Ltd. Chippenham, Wilts British Library Cataloguing-in-Publication Data: A catalogue record for this book is available from the British Library Library of Congress Cataloging-in-Publication Data: A catalog record for this book is available from the Library of Congress
Preface PET is a polymer which is enjoying substantial growth as a packaging material—across global markets and for diverse applications. The growth of PET into packaging, as a replacement for glass, metal and other plastics materials, has been extraordinary. No other rigid plastics packaging sector has experienced the level of growth of PET bottles over the last 20 years. PET is now a commodity polymer competing directly with polyethylene, polypropylene and styrenics in the markets for food and beverage packaging, as well as other products. Its success as a packaging material is due largely to technological developments in the processes used to convert PET into flexible and rigid packs at high outputs, which is crucial for the minimisation of costs. Developments in PET technology in recent years have focused on improvements in gas barrier and heat stability—a process that will continue as new opportunities develop in the food and beverage markets. This volume is designed to inform the reader about PET, about the development of materials and technologies to improve its barrier and heat stability, about the various process technologies for converting it into rigid and flexible packs, and about environmental and recycling issues. It is the first volume to provide a comprehensive source of reference on PET packaging technologies, and it includes the latest developments. The historical development of PET is also covered in an introductory chapter, which brings together many aspects of the early development of PET, with special reference to the 'father' of PET bottles, Nathaniel Wyeth, and his recollection of the first time he ran PET resin to make a bottle. This chapter considers the birth of the polyester industry, with the process of stretching and the uniaxial orientation of polyester fibre, which was a precursor to the biaxial orientation of film and bottles; the demise of Lopac (the Monsanto acrylonitrile copolymer), which gave PET an invaluable lead as the polymer for rigid bottles to replace glass; the development of the preform neck finish, initially based on a glass finish so that plastic closures suitable for carbonated beverage PET bottles could be used; and the further developments in both the materials and the technologies. PET Packaging Technology will be used by packaging technologists, packaging engineers, chemists, materials scientists and engineers, those involved in the design and development of packaging, and those responsible for specifying or purchasing packaging.
The editors have been fortunate to have the support of the most knowledgeable experts in PET technology as authors for this volume. They are busy people, and we are grateful to them for their efforts and contributions. David Brooks Geoff Giles
Contributors Mr Bob Blakeborough
Synventive Molding Solutions Ltd, Unit 1 Silver Birches Business Park, Aston Road, Bromsgrove, Worcestershire B60 3EX, UK
Mr Gordon J. Bockner
Business Development Associates, 4550 Montgomery Avenue, Suite 450 North, Bethesda, MD 20814, USA
Mr David W. Brooks
Corporate Technologies, Crown Cork & Seal Company, Inc., Downsview Road, Wantage, OxonOX129BP, UK
Mr Geoff A. Giles
Global Pack Management, GlaxoSmithKline, London, UK and Holmesdale Cottage, Nuffield, Henley-on-Thames RG9 5SS, UK
Dr Kenneth M. Jones
47 Aspin Lane, Knaresborough, North Yorkshire HG5 SEX, UK
Dr Michael Koch
Ferromatik Milacron Europe, Riegelerstrasse 4, D 79364 Malterdingen, Germany
Dr William A. MacDonald
DuPont Teijin Films UK Ltd, PO Box 2002, Wilton, Middlesborough TS90 8JF, UK
Dr Duncan H. MacKerron
DuPont Teijin Films UK Ltd, PO Box 2002, Wilton, Middlesborough TS90 8JF, UK
Dr Vince Matthews
35 Rossett Beck, Harrogate, North Yorkshire HG2 9NT, UK
Mr Paul Swenson
Kortec Inc., Cummings Center #128Q, Beverly, MA 01915, USA
Dr Bora Tekkanat
Consultant, 1913, Orchardview Drive, Ann Arbor, MI 48108, USA
Mr Mike Wortley
Jomar Europe Ltd, Clarkson, Upper Crabbick Lane, Waterlooville, Hampshire PO76HQ, UK
This page intentionally left blank
DAVID W. BROOKS and GEOFF A. GILES 1.1 Introduction 1.1.1 History 1.1.2 IP—patents 1.2 Market growth and the development of materials ] .2.1 PET fibre and film film 1.2.2 Barrier materials 1.2.3 Competitive materials: PVC, AN/S (Lopac) and AN/MA (Barex) 1.3 Technology 1.3.1 Single-stage ISBM 1.3.2 Two-stage ISBM 1.3.3 Integrated two-stage ISBM 1.3.4 Heat setting 1.4 Packaging 1.4.1 Bottles in the early years 1.4.2 PET cans 1.4.3 Refillable bottles 1.4.4 Preform design, neck design—BPF, vent slots 1.4.5 Beer spheres References
I 1 3 4 7
8 i1 13 14 14 15 15 16 16 18 22 23 24 25
Commercial considerations GEOFF A. GILES and GORDON J. BOCKNER
2.1 2.2 2.3 2.4 2.5
Introduction Container technologies Product processing and filling requirements Packer/filler shelf-life requirements Cost and performance considerations 2.5.1 Material pricing 2.5.2 In-house manufacture of PET containers for packer/fillers 2.6 Recycling issues 2.7 End-use market penetration References
26 28 29 30 31 31 32 33 34 34
PET materials and applications
KENNETH M. JONES 3.1 Introduction 3.2 Polymerisation and manufacturing processes 3.2.1 Manufacturing plants
36 37 40
CONTENTS 3.3 Structures, morphology and orientation 3.3.1 Structures 3.3.2 Morphology 3.3.3 Orientation 3.3.4 Creep 3.4 Properties 3.4.1 Molecular weight and intrinsic viscosity 3.4.2 End group 3.4.3 Thermal properties 3.5 Rheology and melt viscosity 3.5.1 Melt viscosity 3.5.2 Melt flow 3.5.3 Moulding shrinkage 3.6 Moisture uptake and polymer drying 3.6.1 Moisture level 3.6.2 Polymer drying 3.7 Degradation reactions 3.7.1 Thermal and thermal oxidative degradation 3.7.2 Environmental degradation Reheat characteristics Gas barrier properties 3.10 Amorphous polyesters 3.10.1 Homopolymers 3.10.2 Low copolymers 3.10.3 Medium copolymers 3.10.4 High copolymers 3.11 Crystalline polymers 3.12 Polymer blends 3.13 Applications 3.14 Trends 3.15 Global References
44 44 45 48 59 60 61 64 65 70 70 72 75 76 76 77 80 80 81 81 83 87 88 89 91 92 92 93 93 94 94 95
Barrier materials and technology DAVID W. BROOKS
4.1 Introduction 4.2 Polyesters 4.2.1 PEN 4.2.1 Amorphous polyesters 4.2.2 Other polyesters 4.3 Barrier materials 4.3.1 EVOH 4.3.2 PVDC 4.3.3 Polyamides (nylon) 4.3.4 Liquid crystal polymers (LCP) 4.4 Barrier technology 4.4.1 Organic coatings 4.4.2 Inorganic coatings 4.4.3 Scavengers 4.4.4 Nanocomposites
98 98 99 100 101 102 102 104 104 105 106 107 107 109 11 1
Oxygen barrier 4.5.1 Packaging foods and beverages 4.5.2 Packaging oxygen-sensitive foods and beverages 4.6 Carbon dioxide barrier 4.7 Future trends Acknowledgement
xi 1i I 113 1 13 114 1 15 115
PET film and sheet WILLIAM A. MACDONALD, DUNCAN H. MACKERRON and DAVID W. BROOKS
5.1 Introduction 5.2 The film process 5.2.1 Polymer preparation and handling 5.2.2 Extrusion and casting 5.2.3 Drawing 5.2.4 Heat setting 5.2.5 Slitting and winding 5.2.6 Reclaim and recovery 5.3 Polymer, process and properties (3Ps) 5.3.1 Polymer 5.3.2 Process 5.3.3 Properties 5.4 Surface and bulk properties 5.4.1 Film properties 5.4.2 Coating 5.4.3 Co-extrusion 5.4.4 Fillers 5.4.5 Shrinkage 5.4.6 Combination of effects 5.5 PET sheet Extrusion of PET sheet Thermoforming of PET sheet Thermoforming of CPET sheet Materials New developments 5.6 Conclusions—film Acknowledgements References
116 117 117 118 121 130 133 137 137 137 138 138 139 139 142 143 145 146 146 149 149 151 153 153 154 155 155 155
Injection and co-injection preform technologies PAUL SWENSON
Multilayer characteristics Applications 6.2.1 Performance-driven applications 6.2.2 Economics-or legislative-driven applications 6.2.3 Combination applications 6.3 Closure vs bottle permeation 6.4 Container performance 6.4.1 Barrier properties
158 161 161 161 162 162 164 164
6.7 6.8 6.9 6.10 6.11 6.12 6.13 6.14 6.15 6.16
6.4.2 Oxygen barrier 6.4.3 Carbon dioxide barrier 6.4.4 Scavenger property Wall structure Preform and bottle design 6.6.1 Permeation through finish, sidewall and base 6.6.2 Controlled fill Headspace oxygen absorption Oxygen desorption from PET Beer containers Small juice containers Small CSD containers Core layer volumes Recycling Comparison of co-injection technologies Co-injection molding equipment The future
165 166 167 168 169 171 172 174 174 176 178 178 179 180 180 182 183
One-stage injection stretch blow moulding BOB BLAKEBOROUGH
7.1 Introduction 7.2 One-stage machines 7.2.1 One-stage machine construction 7.3 Process stations on a one-stage machine 7.3.1 Injection mould and hot runner 7.3.2 Conditioning station 7.3.3 Blowing station 7.4 'Integrated two-stage'machines 7.5 Drying system 7.5.1 Requirements for a reliable drying system 7.5.2 Drying process monitoring 7.6 Preform design 7.6.1 Neck finish 7.6.2 Preform weight 7.6.3 Cycle time and preform wall thickness 7.6.4 Stretch ratios 7.6.5 Injection mould design and manufacture 7.6.6 Preform design for varying container sizes 7.6.7 Preform weight adjustment 7.6.8 Differences between one- and two-stage preform designs 7.7 Container design 7.8 Hot-fill PET bottles 7.9 Quality control procedures 7.10 Preform examination 7.10.1 Appearance and shape 7.10.2 Preform weight 7.10.3 Neck dimensions 7.10.4 Preform eccentricity 7.10.5 Polarised light inspection 7.10.6 Intrinsic viscosity (IV)
184 189 189 192 192 195 196 197 198 199 200 200 201 202 202 203 205 206 206 206 207 208 208 209 209 210 210 210 211 211
CONTENTS 7,10.7 Acetaldehyde (AA) 7.11 Container examination 7.11.1 Shape and appearance 7.11.2 Dimensions 7.11.3 Capacity 7.11.4 Container wall thickness and material distribution 7.11.5 Top load strength 7.11.6 Impact resistance (drop) test 7.1 1.7 Leakage of liquid (seal integrity) 7.1 .8 Vacuum strength 7.1 .9 Acetaldehyde (AA) 7.1 .10 Oxygen permeation 7.1 .11 Moisture vapour transmission rate 7.1 .12 Product filling temperature 7.1 .13 Container weight 7.12 Bottles for carbonated beverages 7.12.1 Burst pressure 7.12.2 Thermal stability 7.12,3 Carbonation retention 7.13 Additional tests for hot-fill containers 7.14 Additional tests for returnable/refillable PET bottles Appendix: one-stage and integrated PET machine manufacturers
Two-stage injection stretch blow moulding MICHAEL KOCH 8.1 Introduction 8.1.1 The principles of the two-stage process 8.1.2 Technological basics of PET as a stretch blow moulding material 8.1.2 Production concepts and target markets 8.2 Preform injection moulding 8.2.1 Injection machine concepts 8.2.2 Mould design 8.2.3 Productivity parameters 8.3 Stretch blow moulding 8.3.1 Principles of the two-stage stretch blow moulding process 8.3.2 Machinery concepts 8.3.3 Mould technology 8.4 Preform and container design 8.4.1 Container design 8.4.2 Preform design References Abbreviations
Injection blow moulding MIKE WORTLEY 9.1 9.2 9.3 9.4
Basic principles History Process identification Commercial processes
XJii 212 212 212 212 213 214 215 215 215 216 216 217 217 217 217 218 218 218 2I8 2!9 220 220
223 223 223 227 233 238 239 244 247 251 25! 264 268 270 270 274 278 278
280 280 28! 282 283
CONTENTS 9.4.1 Rotary table machines: Jomar, Uniloy and similar Tooling Procrea Materials Applications Machine and process capabilities
283 284 286 286 287 287
10 Hot-fill, heat-set, pasteurization and retort technologies BORA TEKKANAT
9.5 9.6 9.7 9.8 9.9
10.1 The hot-fill process 10.2 The heat-set process 10.3 The pasteurization process 10.4 The retort process 10.5 Concluding remarks References
11 Environmental and recycling considerations VINCE MATTHEWS 11.1 Introduction 11.2 European environmental policy 11.3 EU Packaging and Packaging Waste Directive 11.3.1 Compliance with the Directive's targets 11.3.2 Material identification 11.3.3 CEN standards and the essential requirements 11.3.4 CEN 'umbrella standard' (pren 13427) 11.3.5 Implementation of the Directive in the member countries 11.4 Collection and recovery procedures 11.4.1 Drop-off schemes 11.4.2 Kerbside collection schemes 11.4.3 Reverse vending machines 11.4.4 Other systems 11.4.5 Plastic bottle sorting 11.5 Plastics packaging waste 11.6 Recycling of PET 11.6.1 Principal methods of PET recovery 11.6.2 Contamination issues 11.6.3 Recycling of PET by mechanical methods 11.6.4 R-PET and food-contact quality 11.6.5 Recycling of PET by chemical methods—'solvolysis' 11.7 Environmental benefits of recycling 11.7.1 General principles of recycling 11.7.2 Application of the general principles to the recovery and recycling of PET bottles 11.8 Economic factors affecting PET bottle recycling 11.9 Markets for recovered PET 11.10 PET recycling—the future References
292 293 307 310 313 314
315 315 316 316 318 319 320 320 322 323 324 324 324 325 325 325 328 329 330 330 334 336 342 343 346 355 357 359 362
Introduction David W. Brooks and Geoff A. Giles
Introduction 'The first time we ran the PET resin, our little machine groaned and grunted like it never had before. Our fear was that we not only were going to fail to produce an acceptable bottle again, but that the experiment would damage our test equipment... I remember the mix of expectation and depression I felt when we opened our moulding machine. It was late in the evening, and there was a little cross light hitting the mould. After months of frustration during which we had produced nearly 10,000 bottles by hand, we had grown used to seeing blobs of resin caked on the mould, or crude shapes that looked like anything but a bottle. This time, at first glance, it looked as if the mould was empty. A closer look revealed something else: a crystal clear bottle. Since then I have seen countless truly beautiful PET bottles, but none of them will ever be as memorable as the first' [ 1 ].
These were the words of Nathaniel Wyeth, considered to be the 'father' of PET (polyethylene terephthalate) biaxially oriented bottles, at the Fourth International Conference on biaxially oriented bottles and containers in PET and other engineering and thermoplastic resins, in Diisseldorf in October 1983. His patent, assigned to DuPont, was issued on 15 May 1973. Amoco Container was the first licensee. Other major bottler makers followed; and the rest, as they say, is history. So began the evolution of the PET bottle, which has revolutionised the global bottle market, especially in the carbonated beverage sector. /././
While the events noted by Nathaniel Wyeth stimulated the development of PET resin into the global material that we know today, PET (or polyester, as it is commonly known) developed long before. Although polyester was first discovered in the nineteenth century, it was not until 1941 that J. R. Whinfield and J. T. Dickson of the British company ICI, while searching for a replacement for silk, identified polyester as a fibre-forming polymer. After the Second World War, DuPont was licensed to manufacture the new polyester fibres in the United States, while ICI retained the exploitation rights for the rest of the world. The polyester fibre industry was born when the process of stretching and uniaxially orienting polyester fibre to improve its physical properties was perfected in the 1950s. Demand for this material from
PET PACKAGING TECHNOLOGY
the polyester fibre industry, leading to economies of scale in PET manufacturing plants, resulted in PET becoming more cost-competitive with other materials. In the 1960s, the technology of 'biaxial orientation' was developed— stretching the PET sheet in one direction and then again at right angles to the original stretch. This resulted in a polyester film with enhanced mechanical properties and low gas-permeability that is now widely used for food packaging, film stock, videotapes and computer floppy disks. That side of the business has continued to grow. As PET bottles underwent development for heat stability, so did sheet material, and CPET (crystallised polyethylene terephthalate) was developed for ovenable food trays. Although now levelling out in demand, this development opened up a whole new packaging sector. However, the story should really begin before PET, with bottles made by Monsanto from their Lopac® acrylonitrile (AN/S) resin. This was just one of a range of barrier resins Monsanto had in the late 1960s that had performance bottle potential. They made extrusion blow-moulded (EBM) and injection blowmoulded (IBM) 4 oz and 8 oz Boston Rounds for product testing. Coca Cola® became interested and the first Coke bottle was made in 1969. In 1970, lOoz bottles produced on the Monsanto BDS-8 horizontal EBM wheel were test marketed in New Bedford, MA, US and then Providence, RI, US. They were green, with the traditional Coca Cola® shape. The go-ahead for commercial production came in 1972, for 10, 16 and 32 oz sizes. Coca Cola® were not interested in the family-size segment at that time. The first Monsanto plant started up in Windsor, CT, US in 1975, followed by others in Chicago, IL. US and Havre de Grace, MD, US. By 1976, when one-way bottle production was in full swing, Monsanto also had a refillable bottle ready for production in Chicago. In 1977, the US Food and Drug Administration (FDA) revoked approval for the Coca Cola® 32 oz Cycle-Safe bottle, moulded by Monsanto in Lopac resin. Millions of bottles were sent to the scrap heap; reportedly more than 11 million bottles from one plant alone. The FDA claimed that the Lopac bottle failed to meet the government's new limit of 50ppb (parts per billion) for acrylonitrile extraction. The FDA claimed that this limit was exceeded in a test when a bottle was subjected to a temperature of 48CC (120: F) for 3 months. Monsanto disagreed with this result, suggesting that under normal shelf-life conditions there was no detectable migration of monomer into the contents of the bottle. This move by the FDA, as much as any. started the PET bottle revolution. The first Pepsi-Cola® bottles were in fact also acrylonitrile. In 1968, plastic bottle moulders, DeBell & Richardson, were working with Sohio's Barex (AN/MA), which showed promise, when Pepsi-Cola® approached them to explore plastic bottle possibilities. In 1970, Pepsi-Cola® carried out a test market in Las Vegas, with 250,000 lOoz AN/MA bottles made on a Bekum EBM machine.
DuPont approached Pepsi-Cola® with PET in 1972. Mylar film existed then but no one knew how to make a PET bottle. Pepsi-Cola® were looking for a company that could make a close-tolerance, injection-moulded preform and Broadway Inc. welcomed the challenge. After some initial development they brought along their first preform; for a one litre bottle, the preform was almost as long as the bottle. DuPont, in the meantime, was working with Cincinnati-Milacron on the 'SOM' (slug oriented moulding) approach. An extruded tube was placed in a machine and formed with about 4,000 psi (pounds per square inch) hydraulic pressure. Somehow, without heating, bottles emerged; but the tools were destroyed after about 5-10 cycles. Another idea, namely reheat blow (RHB), was suggested. With Cincinnati, the hand-operated RHB-1 was built. By late 1974, the RHB-3 was ready. The Broadway team had shortened the preform, had an 8-cavity preform injection mould ready, and were making base cups (early bottles had hemispherical bases). The first PET test market was held in New York State during 1975-76, with bottles made by DuPont's Christina Laboratories. Pepsi-Cola® had planned to make their own bottles, but after the test had ended in early 1976, Pepsi helped transfer the technology to others. By late 1976, Amoco Containers' first bottles were ready: 64 oz bottles with a 38 mm neck and weighing 82 g with a snap-on base cup. They were shipped to Michigan, filled and on the market in March 1977. Hoover-Universal's bottles followed a couple of weeks later. One of the best stories arising from recollections of that time was of events that happened in the early 1970s, when Pepsi-Cola® called Goodyear for a sample of polyester resin. They wanted to try to make a bottle but, since the idea seemed far-fetched, they failed to mention this to the Goodyear salesman. He had a choice of five possible grades: three with TiO2, one low-IV (intrinsic viscosity) resin, and one solid-state resin without TiO2. For some reason, he picked the last grade, the only one that had any chance of making a clear preform. It is said that if the salesman had made another choice Pepsi-Cola® might have given up on the whole idea. 7.7.2
In 1973, DuPont issued a series of patents (filed in 1970) assigned to inventors Nathaniel Wyeth and Ronald Roseveare. 'Process and Apparatus for Producing Hollow Biaxially Oriented Articles'. US 3,733,309, 'Biaxially Oriented Poly(ethylene terephthalate) Bottle', and GB 1341845-8, lAn At Least Partly Biaxially Oriented Thermoplastic Bottle' . The main claims of this patent can be summarised as follows: a biaxially oriented bottle of a generally cylindrical section, with a density of about 1.331 to 1.402g-cm3, prepared from polyethylene terephthalate, having an IV of at least about 0.55, has an axial tensile strength of about 5,000-30,000 psi. a
PET PACKAGING TECHNOLOGY
hoop tensile strength of about 20,000-80,000 psi, an axial yield stress of at least 4,000 psi, a hoop yield stress of at least about 7,000 psi, and a deformation constant—equal to the slope of the log (strain rate~') vs strain—of at least about 0.65 at 50°C. The bottle is capable of storing a carbonated liquid with a deformation of less than 5% over lOOh at 50CC, under a pressure of 75 psig (pounds per square inch gauge). The invention can be summarised as follows: it provides a method and apparatus for producing a hollow, biaxially oriented thermoplastic article, which has improved strength properties. The articles are oriented by stretching, typically an average of up to about four times in the axial direction and about 2.5-7 times in the hoop direction. The article has reduced permeability to carbon dioxide, oxygen and water. The bottles produced are useful for storing beverages under pressure, such as carbonated sodas and beer.
1.2 Market growth and the development of materials The number of global PET producers has doubled in the last 10 years, in response to the growing demand for PET for rigid packaging applications. Global demand has seen steady growth through the 1980s and 1990s; in 1985 about 0.5 M tonnes of PET was consumed, in 1990 about 1.5 M tonnes, and this increased to 7 M tonnes in 2000 (see Figure 1.1). PET global capacity has seen a sharp increase in the last three to five years to match the high demand for packaging; from 1990 to 1995 this increased by an average 15% per year, but from 1995 to 2000 the growth was up to 20% per year. The prediction for the next few years is growth of about 10 per cent per annum.
Figure 1.1 Global consumption of polyethylene terephthalate for packaging (M tonne).
Figure 1.2 Regional supply of polyethylene terephthalate for packaging in 2000. Key: D, North America; B. Asia Pacific; IS, Europe; H, South America; •, Middle East/Africa.
The biggest growth has been observed in Asia, where producers have tripled their regional capacities from 1 to 3 M tonnes during 1995 to 1999 (see Figure 1.2). Asia-Pacific now has 37% of global PET capacity. In the period between 1990 and 2000, the regional split for North America has changed from 54% to 34%, for Asia-Pacific from 25% to 37%, and for Europe from 19% to 22%. In this period, the number of PET producers has doubled from about 35 to 75; mostly new companies in Asia-Pacific and South America (see Tables 1.1-1.4). The size of PET plants has also grown in this period; a typical line in 1990 would be about 50 K tonnes, whereas a world scale line is now 200 K tonnes. The major global PET producers have also changed, largely through change of ownership. Eastman has remained the largest global PET producer, with plants in North America, Europe and South America. A consolidation of the market Table 1.1 The major PET suppliers in North America in 2000 PET supplier
Output (K tonnes)
Eastman Chemicals KoSa Wellman M&G Nanya DuPont
836 475 390 360 200 175
North America includes the US and Canada.
Table 1.2 The major PET suppliers in South America in 2000 PET supplier
Output (K tonnes)
Eastman Chemicals Rhodiaster KoSa South America includes Mexico, Brazil and Argentina.
247 177 160
PET PACKAGING TECHNOLOGY Table 13 The major PET suppliers in Europe in 2000 PET supplier Eastman Chemicals Dow DuPont KoSa M&G
Output (K tonnes) 390 280 240 230 220
Table 1.4 The major PET suppliers in Asia-Pacific in 2000 PET supplier Kohap Shin-Kong Tong-Kook Far Eastern
Output (K tonnes) 206 160 140 120
Asia-Pacific includes South Korea and Taiwan.
can be expected in view of the current supply and price situation. Hoechst, the second largest supplier, has steadily dropped out of commodity chemical businesses, and its PET operations are now run by KoSa. DuPont took over Id's PET business, and they have now merged with SASA of Turkey to form DuPontSA. In 1999, Shell decided to exit PET in the course of restructuring of its chemical business, which has led to the sell-off to M&G (Mossi & Ghisolfi Group). Wellman and Dow are the other major PET producers. For a period of time, the PET polymer business has been in oversupply; this is expected to change to a more balanced situation in the next few years. In Europe, demand may well outpace supply beyond about 2005, balanced by excess supply globally because of new capacities being constructed in the Asia-Pacific region. PET is now the most widely used plastic for bottles. The non-return bottle is established around the world; in contrast, returnable bottles have not penetrated to any great extent. The demand for PET bottles has been driven by its use in beverage applications, especially for carbonated soft drinks (CSDs), mineral waters and other beverages, which together account for 80% (while food accounts for 10%) of total PET in packaging (see Figure 1.3). The growth of PET has resulted mainly from the replacement of existing packaging; for CSDs it has replaced glass and to a lesser extent metal cans, and for waters it has replaced PVC and glass. The big question is, will beer in PET progress beyond niche markets? The projected growth for beer in PET bottles is about 10 per cent per annum over the next five years. With technological development, PET has become a suitable packaging material for more diverse end-use applications. Developments involving the use of high gas barrier polymers are progressing with a number of companies.
Figure 1.3 Polyethylene terephthalate packaging applications in Europe in 2000. Key: D, Carbonated soft drinks; ffl. Mineral water; ES. Food; EH, Film/sheet; H, Beer/other beverages; •. Cosmetics; M, Others.
These include ethylene vinyl alcohol copolymer (EVOH), nylons in multilayer structures, coatings with organic materials, the use of polyvinylidene chloride (PVDC), epoxy-amines as external coatings on PET bottles, inorganic coatings including silica and silicon oxide, and plasma coatings of carbon and silicon oxide as both internal and external coatings on PET bottles. These developments will extend the PET market into beverage applications that require high barrier properties, the major target being beers, for which glass and metal cans predominate. There are also many food applications, especially baby food, which is at present largely packaged in glass and metal cans. Newer developments with liquid crystal polymers (LCPs), oxygen scavengers and nanocomposites will extend the barrier potential of PET. The impact of high barrier polyesters, such as polyethylene naphthalate (PEN), as an alternative to PET has so far been insignificant. PEN has better barrier and thermal properties but is more expensive, and its gas barrier properties are not as good as many multilayer and coated PET options. Modification of PET grades by copolymerisation or the incorporation of additives has allowed PET to be processed more rapidly, and thus more economically, by stretch blow moulding with better processing machinery, and can also reduce the formation of acetaldehyde (AA) for sensitive applications such as mineral waters. In hot-fill beverage and food applications, modified PET grades and new process technologies, utilising hot moulds and cryogenic cooling to increase the heat stability, are extending the use of PET. 1.2.1 PET fibre and film
In the 1930s, Carothers and Hill at DuPont produced fibre-forming polyesters that had low melting points and were unsuitable for commercial production. The fibre-forming properties of PET were first discovered in 1941 by Whinfield and Dickson in the laboratories of Calico Printers in the UK. They resulted
PET PACKAGING TECHNOLOGY
in a patent which DuPont acquired in 1948 for the US, and which ICI was granted for the rest of the world. PET fibres became commercial in the US in 1953 and production expanded rapidly in the 1960s and 1970s. The production of textile filament yarn for use in manufacture of garments grew rapidly and. in addition, polyester soon became the principal material for reinforcement of tyres in the US. Growth in the PET fibre market continued worldwide, the enormous expansion being attributed to its great versatility and its importance to the world economy. The discovery of PET's fibre-forming properties soon led to the development of PET films at ICI. Production of polymer films by a drawn orientation process was known for polystyrene (PS) and polyamides (PA). PET was well-suited for biaxial orientation; its properties (molecular weight and melting point) were ideal for producing high-strength films. In the 1950s. the demand for fibres led to rapid expansion in the supply of PET monomers, and the economics of large-scale polymer production became more attractive. PET film manufacture benefited from this rapid growth, and soon chemical companies producing PET fibre were also producing PET films. The key suppliers of films in the US and Europe were DuPont with Mylar, ICI with Melinex and Hoechst with Hostphan, while captive producers, such as Agfa Gevaert, Eastman Kodak. 3M, Fuji and DuPont, were manufacturing for their own internal consumption. In the 1960s, ICI developed the Merolite pack—a sausage pillow-style sachet using flexible, lightweight materials and targeting single-serve carbonated beverages. A thin board sleeve (not unlike a toilet roll inner core) surrounded the body of the 'sausage' for the purposes of decoration. This tube also provided a strengthening feature to hold the container when opening, and also to minimise the risk of squeezing the product out after opening and release of the carbonation gas. The pack was opened by means of a removable tape sealing a small hole through which the product could be dispensed. Sadly, it failed to capture a broad market interest, probably because it was difficult to handle at both the filling and retailing stage, as well as in the hands of the consumer. However, a more widely available system is the CheerPack from Hosokawa Yoko in Japan, or their global licensee, Gualapack, in Italy. Developed during the 1980s, the polyester-laminated pouch has an injection-moulded neck attached, through which the container is filled and consumed. It is very popular for sports drinks because it is practical for use in sports bags, being lightweight and reclosable, and unbreakable in normal use. Again, merchandising issues have limited its market expansion. 7.2.2 Barrier materials 188.8.131.52 OXBAR In the 1980s, Metal Box developed its OXBAR barrier technology, a system designed to provide a chemical barrier within the PET container wall; and specifically to absorb or scavenge oxygen migrating into the pack, preventing
loss of product quality during its shelf-life. Using polymer-based chemistry, OXBAR offers a total oxygen-specific barrier independent of temperature and humidity and has a long but finite lifetime. The components of the system are a blend of PET polymer with an oxidisable polymer (nylon MXD6) at about 5% addition, and a metallic catalyst (cobalt salt >200ppm). The active ingredients are the nylon and the cobalt salt, with cobalt catalysing the reaction of the nylon with oxygen permeating through the pack wall. The OXBAR system consists mostly of PET bottle resin and could be readily converted by standard techniques into preforms and PET barrier bottles and containers. The low levels of active ingredients do not significantly affect the processing of the PET. The important feature of this system is its ability to maintain total barrier properties under elevated temperature and humidity conditions. The OXBAR system provides a total barrier to oxygen ingress for a period of up to about two years. Oxygen transmission data on 1 litre PET bottles produced from a PET blend containing 4% nylon MXD6 and the same blend containing the OXBAR system with added cobalt give an improvement approaching 100-fold. The same bottles were also tested under real storage conditions for two years. The bottles were filled with water, nitrogen-flushed before capping, and the headspace oxygen content was monitored. The control PET blend with nylon MXD6 showed a 10% increase in oxygen into the headspace, while the OXBAR system showed no ingress. The lifetime for the OXBAR system depends on the chemical activity of the cobalt and the level present in the system, and also the thickness of the bottle wall. A further factor is the rate of consumption, which depends on the temperature, wall thickness and the type of PET used. High temperature storage conditions and levels of cobalt below about 200 ppm reduce the lifetime of the OXBAR system. A number of pack tests were carried out with lager beer, orange juice and wine over a 6 month period. In all cases, OXBAR proved superior to PET coated with PVDC, and it was comparable to glass in taste tests. Food contact issues were critical for a novel application involving new chemistry, and extensive extractability tests were carried out by Metal Box chemists on a range of simulants and conditions. At this time, the conclusions were that the levels of cobalt, nylon oligomers and other species were within statutory limits for intended end use. However, the OXBAR system did not become commercial and was shelved in 1990. OXBAR was revisited by Crown Cork & Seal later in the 1990s, and development continues today . 184.108.40.206 PEN In the late 1980s, both Eastman Chemicals and Goodyear developed the first PEN polymers. PET did not have sufficient gas barrier or thermal resistance for oxygen-sensitive foods and beverages, hot-fill foods, juices and sauces. The very limited supply of monomer prevented a major commercial introduction, but sufficient PEN homopolymer was produced to enable trials and testing to be
PET PACKAGING TECHNOLOGY
carried out. Eastman's PEN was called 5XO (five times better oxygen barrier then PET), while Goodyear's PEN was called HP (high performance). Compared to PET, PEN has a high melting point, higher glass transition temperature (Tg) resulting in a higher thermal resistance, and higher gas barrier properties. Bottles could be stretch blown on standard two-stage equipment using high preform temperatures. Bottle tests have confirmed the improved barrier and thermal resistance of PEN bottles compared to PET. However, the projected very high cost, uncertainty about recyclability, and the question of FDA approval prevented PEN becoming commercial. PEN reappeared again some years later. PEN is discussed in more detail in Chapter 4, Section 4.2.1. 220.127.116.11 Barrier developments A number of barrier developments were being progressed in the early 1980s. Mitsubishi Gas Chemical (MGC) was developing nylon MXD6 in Japan, and also using a five-layer, co-injection process to produce 1 litre bottles with PET and nylon MXD6 with tie layers. The bottle had a fourfold better oxygen barrier compared to PET, and was superior to a PVDC-coated PET bottle. In Japan, Unitika together with Nissei were also evaluating a new polymer, polyarylate, called U-polymer, a clear polymer with high temperature resistance and good gas barrier properties (similar to PET). In the US, Eastman developed a high barrier polyester together with tube extrusion processing to produce a three-layer tube and preform, with the polyester having an oxygen gas barrier similar to PVDC. In Japan, Kuraray developed a five-layer co-extrusion line, and used their own EVOH barrier resin in a multilayer co-extrusion structure with PET and adhesive tie resins. Eastman were also co-extruding PET with EVOH in a five-layer structure with tie layers. They developed a new tie layer resin specifically for this application, and they were also producing a range of PET/EVOH blends. Goodyear were developing high barrier polyesters with a threefold better oxygen barrier compared to PET. During 1981, ICI (working with Fibrenyle and Metal Box) developed a PVDC-coated PET bottle, using their Viclan PVDC coating resin. The addition of a PVDC coating improves the oxygen barrier and reduces carbonation loss, thus extending the shelf-life of PET bottles. PVDC can be applied by one of three methods: dip coating, spray coating and flow coating the emulsion onto the external surface of the bottle. Once applied, the coating is cured by drying in a hot-air tunnel at a temperature high enough to form a film, but not so high as to distort the bottle. Metal Box developed a pilot coating line, and a market trial was conducted with coated bottles from the supermarket chain. Finefare, with beer brewed by Watney Mann, which was flash pasteurised and filled by Davenports. The market trial was successful and led to the development of production coating lines by Fibrenyle and Metal Box, and the commercial launch with Jaeger Lager in 1982. Further product launches followed in 1982. with 25 brands in the UK in coated PET bottles. The coated PET bottle achieved
a 4-6 month shelf-life for beers, the limiting factor being oxygen ingress, which over time changes the taste and eventually taints the beer. In the UK, a total of 40 beer brands were packed in coated PET bottles by the end of 1983, with sales of 8 M bottles rising to a predicted 30 M. The coated PET bottle in 2 and 3 litre sizes is still available today from Constar UK (Crown Cork & Seal), who manufacture bottles for breweries in the UK. Wine has been tested and filled in PET bottles and PVDC-coated PET bottles but the penetration has been low. Initial commercial trials were in coated bottles in the US. Shelf-life estimates were about 18 months in coated bottles and 8 months in uncoated bottles. 1.2.3 Competitive materials: PVC, AN/S (Lopac) and AN/MA (Barex) In the 1960s, PVC was being considered for food packaging. In France, edible vegetable oil presented a market opportunity because it was difficult to clean returnable glass bottles. PVC was confirmed to be the best available plastic material because of its transparency, good resistance to oils, low taste, odour and cost. By the end of the 1960s, spring waters were also being packed in PVC in France, once legal approval for packaging waters was completed. Other countries in Europe followed the French example, and PVC remained the main plastic material for packing non-carbonated waters, juices, wine and edible oils for more than 20 years, until challenged by PET. Rigid PVC is an amorphous polymer with good stiffness, clarity and chemical resistance, and good gas barrier properties. Most PVC is processed by extrusion blow moulding and, with the development of high molecular weight polymers, biaxial orientation opened up markets, including packaging of carbonated waters and soft drinks. Monsanto developed Lopac (AN/S), a copolymer of acrylonitrile and styrene (70/30) among a range of barrier polymers in the 1960s. Initially, bottles were extrusion blow moulded and injection blow moulded. Biaxial orientation was also possible; bottles could be stretch blown via a preform, processed on equipment developed by Monsanto. AN/S had excellent gas barrier properties, high stiffness, and excellent clarity and chemical resistance. Monsanto developed the Cycle-Safe oriented bottle in Lopac. The high barrier, tough, refillable bottle was later vindicated with the issue, in 1984, of an FDA regulation allowing the use of the Cycle-Safe bottle for soft drinks, as long as the container met the FDA specifications, which are only achievable using Monsanto's proprietary technology. In Monsanto's Bloomfield, Connecticut Technical Centre, they installed a commercial scale bottle line for production of 64 oz bottles at 125 bottles per minute, with an annual capacity of 50 M containers. The line consisted of an SBC100 stretch blow machine, associated injection moulding, an E-beam facility, material handling and utilities. Monsanto identified refillable soft drinks as a market opportunity for Cycle-Safe bottles because no other plastic material had the toughness and heat resistance to withstand hot caustic washing;.
PET PACKAGING TECHNOLOGY
Monsanto offered licences for Cycle-Safe technology for refillable bottles, and they were investigating the potential for application to beer bottles. Monsanto held a number of patents for Cycle-Safe technology. The key patent  describes packaging materials formed of copolymers of acrylonitrile with a content in the range 55-90% by weight and a high resistance to oxygen and water vapour, providing an improved food packaging material. Other patents describe the use of hydrogen cyanide (HCN) scavengers, such as formaldehyde, which scavenge extractable HCN within the melted copolymer. Also described is the use of lowdosage E-beam radiation to remove residual nitrile monomer from preforms prior to stretch blow moulding, to ensure containers meet the requirements of the FDA and to prevent distortion of the taste of bottle contents, making these containers suitable for packaging foods. Lopac was a polymer which was wellsuited for packaging foods and beverages. It had a lower density than both PVC and PET, ideal for lightweight bottles. It could undergo biaxial orientation, like PVC and PET. It also had high clarity, comparable with PET and better than PVC. Additional advantages were its higher temperature resistance and higher gas barrier properties compared to both PVC and PET. At about the same time, another acrylonitrile copolymer was being developed for food packaging in the US. Barex, a copolymer of rubber modified acrylonitrile and methyl acrylate, was developed by SOHIO (Standard Oil Company - Ohio). Rubber modification is used to enhance its impact properties, otherwise the properties are similar to AN/S copolymers, with excellent clarity, chemical resistance, high stiffness and excellent gas barrier. Barex 210 (AN/MA), a copolymer of acrylonitrile and methyl acrylate (75/25), is easily processable on conventional blow moulding machines used to mould rigid PVC. Biaxial orientation was also possible and, in 1979, 23 and 33 cl bottles were produced on a Sidel machine (Solvay/Sidel BAP) in Barex and Solvay's nitrile copolymer Soltan, for pasteurised 'Fischer' beer in France. Barex was approved for foods by the FDA but not for direct contact with beverages, and was not suitable for hot-fill applications. There follows a consideration of the alternative polymers, PVC and acrylonitrile copolymers with PET, and the key issues for packaging. Both PVC and AN copolymers have a problem with residual monomers: vinyl chloride and acrylonitrile have been shown to have potential harmful effects and must be reduced in the polymer to very low migration levels from the package to the product. In general, residual monomer problems with PET are small and more controllable. The gas barrier properties of AN copolymers are much better than PVC and PET (see Table 1.5). AN copolymers are not as tough as PVC and PET. Orientation enhances the physical and barrier properties and gives sufficient toughness to be acceptable for most packaging applications. All three polymers have relatively low resistance to heat and none can be considered heat resistant. AN copolymers and PVC can be processed by injection, extrusion and extrusion blow moulding. PET is
Table 1.5 Barrier properties of competitive polymers
Lopac AN/S Barex AN/MA PET PVC
1.0 1.1 5.0 10
3.0 4.0 18 30
5.0 6.0 2.5 2.5
Oxygen permeability: cm3 • mil/100 in2 • day • atm. 20 C. Carbon dioxide permeability: cm3 • mil/100 in2 • day • atm. 20; C. Moisture permeability: g • mil/100 in2 • day. 38°C. Abbreviations: PET, polyethylene terephthalate; PVC, polyvinylchloride; AN, acrylonitrile; S, styrene; MA, methylacrylate.
better suited to injection; extrusion blow moulding is only possible with some difficulty, using very high molecular weight grades. All can be stretch blown using biaxial orientation via a preform. PET is very moisture sensitive during processing and will rapidly degrade if the polymer is not correctly dried. PVC and AN copolymers are less moisture sensitive but are more sensitive to heat degradation during processing. Visually, PET is transparent and has good colour and gloss, more so than PVC. AN/S copolymer has good transparency, is hard and, of the alternative polymers, has the visual and tactile perception most like glass. AN/MA copolymers include a rubber component, which decreases the clarity, colour and gloss but improves impact performance. PET has a waterwhite clarity; PVC and both AN copolymers have a yellow tint. PET made the grade, especially for beverages; PVC was acceptable for a time but has now been replaced by PET. AN copolymers did not recover from the early monomer residual issues, and Lopac has disappeared, while Barex is still looking for markets. 1.3
From the early days of the development of PET bottles, two distinct technologies developed: single stage, where the preform is injection and blow moulded in one machine; and two stage, where the preform having been injection moulded is cooled down and taken to a blowing unit to be reheated and blown into the final container. In single stage, there are usually the same number of injection moulds as blow moulds; in two stage, there is no connection between injecting and blowing and so the number of cavities can be optimal. Later chapters cover these technologies in more detail. An alternative technology existed called 'integrated two stage', which moulded the preforms with the optimum number of cavities but then carried them, still hot, to an optimum number of blow moulds all within the same machine.
PET PACKAGING TECHNOLOGY
In two-stage technology, names such as Krupp Corpoplast, Sidel and Cincinatti Milacron were famous. Through company mergers, these names are gradually disappearing. In single-stage technology, Nissei and Aoki have dominated. In the integrated field, Van Doom originated but Sipa have now taken over. 1.3.1 Single-stage ISBM While PET bottle development was proceeding in the US, Mr Katashi Aoki, Chairman of Nissei Plastic Industrial, a large manufacturer of injection moulding machines in Japan, was leading a project to develop a machine to make biaxially oriented PP (polypropylene) containers. He recognised that the prototype machine could be used to produce the new PET bottles and, in December 1975, the One-Stage ASB-150 injection stretch blow moulding machine for making the new biaxially oriented PET bottles was unveiled. All one-stage injection stretch blow moulding machines derived from this original 'Aoki Stretch Blow' design are referred to as classic one-stage machines, as the concept has long since been extended into other PET developments (see Chapter 7). The classic one-stage machine design is extremely versatile in that the same basic machine can be used to make a wide variety of bottles and jars in all shapes and sizes. The ASB-650, which was the standard single-stage machine in the early years, had eight cavities for 1.5 litre bottles. 1.3.2 Two-stage ISBM In the early developments, preforms were made by continuously extruding a PET tube. To make these preforms, Krupp Corpoplast developed a preform manufacturing machine (M120) that took a continuously extruded PET tube, heated and closed one end, and then heated the other and formed a thread finish by blow moulding. This process had a faster output rate, at 12,000 preforms per hour, than the early injection moulding routes of 8 and 16 cavity moulds. Being extruded, the preforms could be multilayered with barrier materials. The Ml20 equipment was installed by such companies as PLM in Sweden, Owens Illinois in the US and Toyo Seikan in Japan. In later years, the Ml20 moved from PLM to Akzo as this preform technology specialised in multilayer. The system was overtaken by injection moulded preforms as the cavitation increased to 32 and beyond. The quality of the injection moulded (IM) neck, adding for example vent slots, made the IM finish preferable. Moreover, IM technology is available from more than one company, giving customers greater technical and commercial choice. Krupp Corpoplast also developed the B40, a 'two-stage' technology machine, with six blow moulds operating at around 4,000 bottles per hour. Subsequent mould and cooling development increased the output to 6.000 bottles per hour.
The B40 became the workhorse for the early two-stage bottle producers (see Chapter 8). 1.3.3 Integrated two-stage ISBM In the United States, companies such as Van Doom developed an integrated twostage approach. Here the preforms were made by more conventional injection moulding routes (with the number of cavities optimised to match the required output) and then, while still hot, were carried to a separate blowing machine with the optimised number of blow moulds to suit the required output. This was the first 'integrated' approach to PET bottle making. Equipment developers such as ASB Nissei in Japan took the 'single-stage' approach. Here the equipment had the same number of injection cavities as blowing moulds. This was a more compact approach and proved ideal for smaller batch output (ca 6 million bottles per year), with excellent glossy surfaces. 1.3.4 Heat setting The first mention of heat setting appears in the patents of Wyeth and Roseveare of DuPont [ 1 ] and Siggel et al. of Glanzstoff . The Wyeth patents describe the fundamental aspects of PET stretch blow moulding and methods and apparatus for producing biaxially oriented PET bottles, with general ranges of preferred process conditions and bottle properties. None of the claims in these patents refer to heat setting, although there is a section which discusses the advantages of its use for bottles intended for hot beverages and when subjected to high temperatures and pressures in a pasteurisation process. Heat treatment can be carried out at 140-220°C for a short time, sufficient to increase the material crystallinity of the finished bottle to at least 30% and up to 50%. Good results were obtained when the heat setting was carried out for 0.1-600 s. It may not be coincidental that the values quoted by Wyeth are almost identical to those given by Siggel et al. Siggel's patent pre-dates Wyeth, but refers specifically to vacuum deep drawing of PET sheet, with additional heat treatment of the shaped sheet to increase the degree of crystallinity. The sheet initially has 5-25% crystallinity and is shaped while at a temperature of 85-200°C. Further heat treatment of the sheet, for a period of 30-600 s while the mould surface is at 140-220°C, is designed to increase crystallinity above 25%. In the 1970s, a patent of key significance to heat setting technology was issued by AS Haustrup Plastic . It describes how a blown PET bottle is transferred to a heated mould and then reblown, while the temperature of the heated mould is maintained above 140°C. Stretch blow moulding can take place into a heated mould, or the blown bottle can be reblown into a heated mould at a later date, on a separate machine. Collins at ICI  describes stretch blow moulding PET
PET PACKAGING TECHNOLOGY
into a heated mould maintained at 130-220°C, cooling the container while maintaining pressure in the mould, and then removing the container. Sabatier of Carnaud Total Interplastic  describes a process for reducing residual stress in PET bottles by filling with hot liquid under pressure, or by increasing the temperature of the walls of the mould to 180-200°C. Many patents, assigned to Owens, Illinois , PLM , Monsanto , Yoshino  and Rhone Poulenc , were issued in the 1970s. These patents extend the scope of heat setting of PET. To summarise , the patents describe in broad terms heat setting of bottles using heated mould systems. Heat setting can be extended to include the bottle sidewalls, neck and base. Mould temperatures of 70-250CC are quoted, with setting times of up to 8 min. A differentially heated mould can be used to heat specific sections of the bottle and neck, and oil or water can supply the mould. The bottle can be blown with high-temperature compressed air and stretched with an internally heated rod. Subsequently, the bottle can be cooled inside or out of the mould and can be held under pressure while cooling. Heat setting can increase the crystallinity of the bottle wall to 25-60%, and the bottle can be designed to resist deformation when hot filled and cooled. 1.4
1.4.1 Bottles in the early years The total estimated PET bottle grade capacity in Europe in 1979, when PET bottles were first manufactured in the UK, was about 25 K tonnes. The total installed bottle production capacity in the UK by the end of 1979 was 150M bottles in 1.5 and 2 litre sizes, and the total PET resin demand was about 7 K tonnes. There were six companies manufacturing bottles, three using singlestage Nissei ASB 650 machines, two using Husky Injection/Krupp Corpoplast two-stage machines, and Carnaud GPG using equipment that they had developed themselves. PET bottle grades in Europe were available in a range of viscosities (IV 0.75-0.98) and were based on germanium or antimony catalyst. The high IV grade produced by Akzo was used by PLM for their Strongpac PET bottle, which was converted from extruded tube into preforms and then stretch blown into bottles. As the technology of making plastic bottles for pressurised, carbonated products was in its infancy, bottle shapes had to rely on known pressure vessel profiles, so the early bottles had hemispherical shoulders and bases. In order to allow the bottles to stand up, a base cup had to be attached. These were generally made in black, high-density polyethylene for durability when chilled. Moreover, black could contain a certain amount of recycled material to reduce costs (Figure 1.4). Attempts were made to have the base cups clipped onto the bottles to ease removal. However, they soon came off as the bottles expanded and so cups had to be glued on. These were not efficient to apply and during
Figure 1.4a PET beer bottles with HOPE base cup.
Figure 1.4b PET soft drinks bottles with HOPE base cup.
very hot periods of storage or distribution the hot melt adhesive would soften and the bottles then took on a lean like the tower of Pisa!! Some attempts were also made to have thermoformed base cups. These had the advantage of being nestable and made in PET, which meant they could be welded to the bottles. Being tapered, the base standing diameter was reduced and the sharp corner at the base made the bottles more difficult to pass along conveyors and dead plates. They also had a tendency to be brittle if a filled bottle was dropped, particularly if chilled in a fridge. In the 1980s, developments for one-piece bottles entered the marketplace. As interest gained ground for in-plant operations, having to purchase and glue base
PET PACKAGING TECHNOLOGY
cups onto bottles just added to the complexity of carrying out this work in-line. A one-piece bottle was ready for filling post blow moulding without secondary operations. The product developed became known as the 'petaloid' base, as it looked petal-like and had five 'feet'. A number of companies developed alternatives to avoid patents and early problems of bases cracking. Today, onepiece, footed base bottles are commonplace. In the early 1980s, Metal Box aimed to develop a single serve (250 ml) PET bottle to service an energy drink market, where the PET bottle could increase the market beyond that achieved by glass. In order to achieve the greatest possible shelf-life, the body had to have maximum stretch all over (including the base). The neck was designed to be plastic closure only and lightweight. To enable the bottle to stand up, the base was blown to a hemisphere, giving maximum stretch, and then inverted. To prevent the inverted base from reverting when under carbonation pressure, a special PET ring was spin-welded onto the base rim. This bottle was known as the welded ring inverted base (WRIB) bottle. To provide additional shelf-life, the bottle was coated with PVDC. The shelf-life was spectacular for a 250 ml bottle in the 1980s. Even today, its performance would exceed most 250 ml PET bottles. However, it failed due to the overall cost and problems with the security of the base rim weld over time as the PET crystallised. 1.4.2 PET cans 18.104.22.168 STEPCAN Metal Box developed STEPCAN in the 1980s at its R&D Centre, Wantage, UK. STEP is an acronym for the stretch tube extrusion process, developed to convert extruded PET tube into can bodies via a novel stretching process. Extruded PET tube was produced by Akzo Chemicals, and later also by Metal Box, using high molecular weight PET (IV ~ 1.0). The STEP process involves reheating amorphous PET tube, and stretch blow moulding and biaxial orientation to produce a 2 m long blown tube. This tube is then constrained, heat set at a high temperature to produce a highly crystalline, thermally stable, biaxially oriented blown tube, which converts into 18 standard size (83 x 97mm) can bodies. The process maximises the mechanical and barrier properties of PET and, by varying the hoop-to-axial orientation balance, can eliminate any tendency to split or delaminate in subsequent operations. Each of the processes was protected by a patent application in a number of countries. The two key process stages are as follows. First, simultaneous biaxial orientation gives 20% strain-induced crystallisation, natural strain hardening and very uniform material distribution, both around and along the tube. There is high mechanical strength and small crystallite size, which ensures high clarity and gloss. The second stage involves controlled heat-setting of this blown tube, giving fast, high crystallisation (40%) and stabilisation of network chains. High clarity and high gloss are maintained and gas barrier properties are enhanced.
The blown stabilised tube can then be cut into can bodies, which can be flanged at both ends. This allows the can body to be subsequently double seamed, with standard metal can ends for high integrity, suitable for packaging processable foods, pasteurisable beverages and hot-fill products without distortion. It is worth considering the background to the development of STEP. PET was developed in the 1970s to produce a high molecular weight polymer suitable for conversion into oriented bottles by stretch blow moulding. The injection stretch blow moulding process was developed to first produce a preform, which is then biaxially stretched into a bottle. The bottle has an injection moulded neck, which is not heated or stretched and remains amorphous. The bottle may also have sections which do not have uniform thickness, do not have uniform material distribution, do not have uniform gas barrier performance, do not have uniform mechanical properties. In the 1970s, PET bottles had a hemispherical base, which helped to improve their orientation and properties. PET bottles are satisfactory for the use for which they are designed, especially for packaging carbonated beverages, but not for processed foods and other products that require high temperature treatment. Developments at Metal Box have also involved investigation of free blowing of PET tube, initially without a mould, to determine the natural stretch ratios in the hoop and axial directions at different stretching temperatures and blow pressures. This development provided the basis for designing the tube needed to be converted into the 2 m length blown tubes. Further developments involved free blowing with additional rod stretching to control bubble propagation during the biaxial process . Thermal crystallisation of amorphous PET is an alternative process to heatset, strain-induced, crystallised PET material for generating heat stable containers. However, this process results in loss of clarity and poor impact performance. It is commercially used for manufacture of ovenable trays and for crystallising necks on some hot-fill bottles. Further thermal crystallisation of already crystallised, strain-induced oriented PET, achieved in the novel heat setting process of STEP, retains the high clarity, improves the gas barrier and mechanical performance, and maintains impact resistance. STEPCAN could be processed successfully in commercial filling processes of high quality fruit and acidified vegetables at pasteurisation temperatures of 93-104°C. Double seam integrity was confirmed by a range of physical and biological leakage tests (biotesting) on unprocessed and processed filled cans. The ultimate test was the successful seaming of STEPCAN under the commercial conditions achieved in various countries in the world. The next stage was to extend STEPCAN for low acid foods that required sterilisation temperatures of 121 °C, to achieve a specification for a can that could be sterilised in steam without overpressure, to allow processing on standard canners' equipment. STEPCAN was introduced commercially in the UK by Marks & Spencer, with a range of high quality fruit packs (Figure 1.5). The STEPCAN also had
PET PACKAGING TECHNOLOGY
Figure 1.5 STEPCAN processable PET food can.
the new Carnaud (before the merger with Metal Box) easy-open, full aperture metal end (HOLE). STEPCAN was a unique packaging concept, offering the market a glass-clear, seamless PET can body alternative to a metal can, suitable for conventional food processing systems. The limitations in the can production output and the requirements for a higher barrier for packaging foods prevented commercial success. At the time of termination, development of a multilayer can and a continuous drawn tube route were progressing. The production facility at Perrywood, UK, and development at the R&D centre in Wantage, UK, were closed in 1990 . 22.214.171.124 Arnican While STEPCAN was being developed by Metal Box, Akzo Plastics was developing a similar PET can, called Arnican. This can was manufactured from a biaxially drawn PET tube. Akzo produced the extruded PET tube and blew the can bodies. Akzo had Thomassen & Drijver Verblifa as development partners. Can bodies were double seamed with metal ends, and limited filling trials were carried out. Akzo were also developing a multilayer version to improve the barrier properties of the can. Because Akzo were also close partners with Metal Box, supplying them with extruded tube for the STEPCAN development, they did not progress any further. This, as much as any other reason, prevented further commercial development of Arnican. 126.96.36.199 Thermoformed can In 1979, Plastona in the UK made a 33 cl PET can, called Plastocan, on its own thermoforming lines, and these cans were available for commercial use in the UK in 1980. At about this time, the global market for 22-33 cl metal cans was increasing, and attention turned to the possibility of making a PET can in
these sizes for beverages. At the same time, Thermoforming S.p.a in Italy was developing a thermoformed PET can, called Thermocan. They were carrying out R&D on the whole process, involving the production of PET sheet, modifications and improvements of thermoforming equipment, and optimisation of PET properties for can manufacture. These involved biaxial orientation in the sidewalls of the can to obtain greater strength and improved barrier properties, also can design, sheet treatment to optimise thickness distribution, and techniques to control flange thickness for seaming metal ends on to the can. The possibility of improving the gas barrier properties of cans was investigated, using co-extruded multilayer sheet, with PVDC as the gas barrier layer, PE as the internal layer and PET as the external layer. The advantages stated for Thermocan included: cost reduction compared to aluminium cans, small scale production capability, local manufacture, lightness, easy handling, high mechanical performance, suitability for packing CSDs, and a shelf-life of at least 6 months. Patents were filed, which extended to the US and other countries. The thermoformed can could not hold high-carbonated pressures, as it deformed and distorted, but it was satisfactory for still and some low-carbonated products . 188.8.131.52 Petainer In 1983, PLM AB in Sweden and Metal Box in the UK formed a joint venture company, Petainer SA. The ambition of this venture was to further develop the Petainer technology, which PLM invented and patented. At this time, a machinery agreement was signed with Krupp Corpoplast, which included them in a three-way technology development of a new packaging system. Coca Cola® joined this development, having initially tested the first prototype cans made by Petainer. To further develop Petainer into the US, a US partner was sought, to contribute experience with market know how. Sewell Plastics joined forces with PLM and Metal Box, and Petainer Development Company was formed in 1984. The purpose of this company was to take the process from laboratory to full-scale production. In 1985, a site for the first plant was selected in Atlanta, US and equipment was in place later that year. The scope of the venture was to completely develop the package, and would require a major investment of resources and technology. In order to be commercially viable, it was necessary to put together a total system, including production, handling, filling, closing, packing, transportation, distribution, vending, collecting and recycling. The background to the development of Petainer starts with the PLM joint venture with Akzo Chemicals, a major producer of PET polymers. They developed a tube technology for PET bottles, together with Krupp Corpoplast, and manufactured the first preform machine. This machine could take an openended, extruded, amorphous PET tube and convert it into preforms for a 1.5 litre bottle. The PLM company, Strongpac, used this machine to produce bottles from extruded tube, which had improved mechanical performance and was
PET PACKAGING TECHNOLOGY
lightweight. This work provided the background to a new technology, the Retainer lightweight neck technology, which allows the neck finish to be oriented, and also reduces material and increases thermal stability in the neck and shoulder of the bottle. PLM developed a novel stretching and heat stabilising technology for PET, to provide an alternative pack for beverages and foods. The technology consists of three key process stages, which utilise either extruded tube, injection-moulded or thermoformed preforms, and involves: • • •
preform stretching to maximise uniaxial orientation and crystallinity heat shrinking the stretched preform to provide heat stability forming containers
Each of the processes was protected by a patent application in a number of countries. The process stages involve the injection moulding of preforms in amorphous PET. The preform is then heated to about the Tg (75 C), is wallironed by uniaxial orientation, and a dome base is formed. The stretched preform is trimmed to provide the correct length and is then flanged and reformed into a can body. The open top can body is now trimmed to a precise length in preparation to neck-in and flange to the correct diameter to take a seamed metal end (209 diameter). The finished can is a 12 oz oriented PET necked-in beverage can with a draw wall ironed (DWI) base. The first commercial scale production lines using modules produced by Krupp Corpoplast were installed in the Petainer plant in Atlanta, US, and the first Petainer cans were produced in 1986. Direct comparisons with an aluminium beverage can in terms of cost, barrier and recyclability were always going to be a major challenge, which eventually prevented commercial success. The equipment was subsequently sold to Yamoro Glass in Japan . 1.4.3 Refillable bottles In a number of European (and some South American) countries, the major beverage container market was for returnable/refillable glass bottles. The only way for PET to gain a foothold was to also have a returnable/refillable bottle. Therefore, a 1.5 litre, 109 g bottle was developed in the 1980s to be heat stable enough to withstand the hot wash and caustic solutions used to ensure the bottles were cleaned. As PET could absorb certain chemicals and odours, special equipment had to be developed to 'smell' inside the bottles. If the 'sniffer' could not detect the smell of the original product, the bottle was rejected. Also, as the bottles would have a tendency to experience continued minor shrinkage at each washing, care had to be taken to record on each bottle the number of trips it had made. Given the continued growth of one-trip PET bottles, some markets have now found it better, and cheaper, to have returnable, one-trip PET bottles, with the deposit built into the purchase price of the filled bottle. As the returnable/refillable bottle market is static or even declining. Chapter 10. in this
volume, 'Hot-fill, heat-set, pasteurization and retort technologies', focuses on the higher performance containers and new markets. 1.4.4 Preform design, neck design - BPF, vent slots The neck finishes in the bottles test marketed in Europe in the mid 1970s were based on the finish from the 1 litre returnable glass bottle as used by Coca Cola®, who led the PET bottle evaluation in Europe at that time. This was a 28 mm finish that could accept a metal roll-on pilfer-proof (ROPP) closure. (It should be noted here that ROPP is an industry-recognised definition of this type of closure; no packaging should be deemed to be 'pilfer-proof but should be tamper evident, and the packaging should carry information for the consumer to be aware of how to recognise signs of tamper evidence.) As the test market moved into country and area launch, the neck finish became established. As, indeed, did the 1.5 litre PET bottle having the same diameter and height as the 1 litre glass returnable bottle (because it was easier to test market a new bottle which fitted the same filling line change parts and distribution system). These dimensions exist to the present day. As the UK came into the PET bottle era in 1979 (Able Developments, part of Wells Soft Drinks, were one of the first and went in-plant with Krupp Corpoplast B40 two-stage machines), more attention was given to the neck finish. The 28 mm ROPP finish was essentially the MCA 2 neck finish and PET bottles had to accept the metal ROPP closure. Problems arose as the PET finish was so accurately made (certainly more concentric and tighter toleranced than the glass equivalent) that the closures could be removed from the bottle faster than the gas inside the bottle (containing carbonated soft drinks) could be released to atmospheric pressure. On certain rare occasions, this caused the cap to 'missile' off the bottle, which could cause injuries; such an event was referred to by the wonderful term 'tail end blow off or TEBO. Another factor was that the rolled-on thread finish on the cap could vary, subject to the condition of the capping chuck. If the threads were not rolled into the neck finish sufficiently, then the cap could also disengage from the bottle, which was referred to as "premature release' and could cause injuries (several court cases occurred in the UK). In the late 1970s and early 1980s, the UK bottle and closure industry put a great deal of effort into resolving these issues. The British Plastics Federation (BPF) and the Metal Closures Association (MCA) worked together to overcome these problems. Companies like Metal Box (now Crown Cork & Seal), who had the resources of PET bottle production, both metal and plastic closure manufacture, and capping machine supply and service as well as extensive R&D capabilities, were well qualified to participate on both the BPF and MCA bodies as well as to test and evaluate the resultant proposals. Before this time, the assessment of TEBO was rather subjective; as a result, a number of devices were constructed to ensure that consistent and repeatable testing could take place, and
PET PACKAGING TECHNOLOGY
industrial standards were set. The outcome was the BPF C neck finish, which has remained in production on preforms and bottles for many years and is only now being superseded by the PCO (plastic closures only) neck finishes. PCO neck finishes are lighter weight finishes made possible as the industry has largely moved away from metal closures on carbonated beverage bottles. The BPF C finish superseded the A and B variants. It had vent slots that were more like channels instead of the early 'vee' slots, and had a special thread profile more suited to the manufacture of the neck 'splits' needed to mould the finish. By spark eroding the start of the thread, it was possible to increase the effective thread length and make the cap engage with the neck for more turns. The new profile of vent slots increased the rate of gas pressure release and, linked to the increased turns of thread, reduced the incidence of TEBO. Incidences of 'premature release' were reduced by better understanding of the maintenance of well-defined thread definition on RO (roll on) and ROPP caps. The launch of plastic prethreaded caps in the early 1980s also meant that consistent thread engagement and closure performance was assured. 1.4.5 Beer spheres In the late 1970s, Johnson Enterprises of Rockford, Illinois, US developed a large PET container made in the shape of a sphere for the take-home beer market, giving rise to the registered name of 'beer sphere' (Figure 1.6). This was a 20 litre container weighing 280 g. Made on a Cincinnati Milacron RHB IX, the preform was heated by radio frequency because of its very thick sidewalls (7 mm). This container was used by a number of regional breweries, who still
Figure 1.6 Beer sphere PET beer container.
had access to the old cask-filling machinery. By 1982, Metal Box Company took a licence for European production and distribution into Europe. In response to the UK demand, they developed a 30 litre container, in conjunction with Johnson Enterprises, utilising the Metal Box PET knowledge and the 280 g preform. This larger container was used by several UK breweries for draft beer in small UK outlets and for export to the Far East, Australia and the US. Returnable, refillable kegs are expensive for such long-haul business. Some customers developed the market opportunity into draft wine and cider. Developments in the dispense equipment added to the market opportunity for this novel container. Johnson Enterprises continue to produce the beer sphere and in the UK the licence has been taken up by Green Sphere. Several of the larger US breweries are producing 20 litre beer spheres. To the best of the authors' knowledge the 30 litre beer sphere remains the world's largest PET container for carbonated beverages. References 1. Bakker, M. (1994) Bottlemaking Technology and Market News, 3, 1994. 2. UK Patents 1341845-8. Wyeth and Roseveare, DuPont. 3. Folland, R. The OXBAR Super Barrier System: a Total Oxygen Barrier System for PET Packaging. CMB Technology, Europak, 1989. 4. US Patent 3451538. The Monsanto patent for acrylonite copolymers: packaging films with improved properties. Expired in 1986. 5. US Patent 3496143. Siggel et al., GlanzstotT. 6. UK Patent 1523146. AS Haustrup Plastic. 7. UK Patent 1474044. Collins, ICI. 8. UK Patent 1530305. Sabatier, Carnaud Total Interplastic. 9. US Patents 4154920, 4233022 and 4439394. Owens, Illinois. 10. US Patents 4264558 and 4387815. Jacobsen, PLM. 1 1 . US Patent 4318882. Agrawal, Monsanto. 12. US Patents 4164298 and 4375442 and Japan Patents 54066967, 54068384/5 and 56080428/9. Yoshino. 13. EP Patents F2389478 and BE866692. Bonnebat, Rhone Poulenc. 14. Brooks, D.W. Heat Setting PET Bottles Patents Review. Metal Box internal technical record, 1985. 15. UK Patent GB 2,145,027. Tubular Articles of Biaxially Oriented Polymers. D.W. Brooks, Metal Box. 16. Dick, D.A. STEPCAN: the choice is clear for a long-life, processed food PET container. CMB Technology, Europak, 1989. 17. Bocchi, L. Experience and developments in thermoformed PET containers for carbonated beverages. Thermoforming S.p.a. Fourth International Conference on Bi-axial Oriented Bottles and Containers and other Engineering and Plastic Resins. Dusseldorf, 1983. 18. Emilson, L, (PLM) and Folland, R. (Metal Box). Petainer PET Can Technology. BevPack, 1986.
Commercial considerations Geoff A. Giles and Gordon J. Bockner
There is little question that the growth of PET packaging has been the big story in packaging in the 1990s. It now appears that this story will continue to dominate our attention well into the future. PET packaging has demonstrated an unusually strong connection with consumers. For whatever reasons— portability, lightweight, convenience, safety—PET packaging is helping brand owners to sell product. However, because PET packaging is used in a wide range of market categories, it is important at the outset of this section to make a basic distinction between these markets. Commercial considerations will also be viewed from several angles: the converter (making the container), the packer/filler and the brand owner (who may not actually handle packing and filling). This gives rise to a complex matrix of considerations when assessing the benefits of PET packaging. The world of PET packaging can be divided into two parts. The larger part— represented, for example, by nearly 25 billion containers in the US—is the huge but maturing and increasingly commodity-driven world of carbonated soft drinks (CSDs), where merchant suppliers are (to be kind) profit-challenged. The soft drink giants keep a tight rein on pricing. Coca-Cola® self manufactures nearly 90% of its containers through its bottler cooperatives in the US. Having grown significantly over the last 20 years, the future CSD market will be driven by more customised packs which will add consumer value. The second part, the so-called 'custom' segment of PET container consumption, represented mainly by beverage products, water, juices, teas and, to a lesser extent, a host of other food products, is often lumped together under the 'new age' label. It is younger and smaller but faster growing. The overall custom market is projected to grow from approximately 11 billion containers in 1998 to approaching 20 billion by the early 2000s. A fairly large portion of this market, especially that represented by water, which converted to PET many years ago. also provides smaller returns for container manufacturers. This will drive the 'custom' segment to seek new opportunities beyond beverages and water. In recent years, it has been emphasised that some demanding food and beverage products cannot be packed in PET until improved performance containers are available. Furthermore, the commercialisation of such containers is dependent upon the development of cost-effective, performance-enhancing, container technologies to manufacture them. Whilst we appear to be waiting
for these technologies, we read in the trade press about new food and beverage products moving into PET. This is a result of shelf-life criteria being changed to accommodate PET and of efforts to optimise the performance characteristics of 'standard' PET packaging. These are often food or beverage products that are switching from other existing packaging materials. This is not to say that these alternative materials will be totally replaced by PET. Some products will remain in glass, cans or other plastic containers for some time to come. In most instances, however, the growth of PET will come at the expense of these other packaging materials. In some cases, these will be other polymers, such as polyvinyl chloride (PVC), which are still used to some extent in Europe for water and edible oil, or multilayer, olefin-based plastics. However, the material that will be impacted most by the ongoing development of PET packaging will be glass, used in its traditional markets of food and beverages. There are many considerations for a packer to make when selecting a particular package for their product. Three primary considerations are: • • •
functionality or package performance cost market preference
There are also a series of secondary considerations affecting decisions on package selection. Some of these considerations could include: • • • •
availability of the package distribution requirements environmental or recycling issues traditional packaging formats already used
When viewed from the perspective of the package supplier, packer/filler or brand owner, the factors to be considered when determining package functionality or performance can be either 'internal' or 'external'. Internal factors are those within the control of the particular business making the considerations (i.e. converter, packer/filler or brand owner), including material and process and product developments, utilisation of equipment innovations, and economies of scale. In other words, factors which the particular businesses themselves can sponsor or implement over time, given the development and commercialisation of new technologies and products, and availability of capital. The PET packaging industry continues to benefit from a multitude of 'internal' developments. Conversely, the glass industry does not benefit to the same extent as it is a 'mature' technology. External factors are those that are beyond the direct control of a particular business, although it may be able to influence their impact. Some of these external factors which can, for example, impact the converter, include new food or beverage processing techniques, introduction of a new beverage or food product, modified shelf-life requirements or distribution channels, changing consumer preferences or habits, and environmental issues. Even international
PET PACKAGING TECHNOLOGY
competition from drinks cartons is an external factor. Resin price and price instability are also factors that can impact development and conversion to PET. An external factor to the converter, but internal to the packer/filler, is the acceptance of the PET shelf-life. Packer/fillers who have traditionally accepted and ultimately demanded the total oxygen barrier, infinite shelf-life and product neutrality of glass have gradually considered and implemented alternative processing and marketing methods which have enabled them to convert to PET packaging. The net influence of these internal and external factors, across the supply chain, has been to create an effective parity and competitive equivalence between glass and PET for an increasing number of end-use markets. Products to be packed fall into three categories: • • •
products which are 'safe' for PET products which are 'safe' for glass or other traditional packaging products which are converting from one to the other
Generally, the 'safe' PET markets are growing in their own right, while the 'safe' glass and traditional markets are declining, and the trend for the 'converting' products appears to be in favour of PET. There will be 'blips' along the way, for example: raw material price increases based on temporary supply/demand imbalance may delay change and even induce significant structural changes to the industry; short-term equipment or container supply shortages may distort trend lines; introduction of new products will continue to favour glass at first but will ultimately yield to consumer preference. The critical question does not appear to be whether PET will grow at the expense of traditional packaging but how soon and in which end-use markets. Container manufacturing technology is not the only driver of new PET product introductions. In fact, four drivers must be considered: • • • •
container technologies product processing andfillingrequirements packer/filler shelf-life requirements cost/performance characteristics
These drivers are considered in the following sections of this chapter. 2.2
In the last decade we saw the first significant conversions of hard-to-pack foods and beverages switching into PET containers. These included, in particular, oxygen-sensitive products such as tomato ketchup being filled into narrow-necked containers, and the launch of single-serve beer bottles. These
conversions were the result of two trends which, it is thought, will govern the growth of standard and customised PET container markets over the next several years. The first trend is the growing market's readiness to accept plastic containers, reducing or modifying their shelf-life requirements, introducing innovative food processing techniques, and the improving cost/performance characteristics of customised PET containers. The second trend is the development of the following two distinctive approaches to technological development: •
The aggressive and creative utilisation of 'existing' manufacturing and material technologies with continued R&D initiatives. This has resulted in a commitment among producers and end users of PET containers to optimise the performance of existing PET container manufacturing concepts. The continued development of 'innovative' container process and product technologies in order to provide food and beverage packers with custom containers with significantly improved performance characteristics on a competitive basis. Product processing and filling requirements
In general, there are three main product groups: •
Carbonated soft drinks (CSDs), which are carbonated to around four volumes of carbonation and supplied originally in 2,1.5 and 1 litre multiserve sizes. However, use of the smaller, single-serve, sizes is increasing. In the US, the fastest growing market is for the 20 oz size (approx 63 cl). Internationally, the 50 cl size has been developing a strong market and is currently the smallest suitable size produced from standard PET technology. Hot-filled (85°C/185°F), single-serve containers (typically 500 ml), with thermal stability and improved gas barrier, have the fastest growing market for beverage PET containers. In the US, the 16oz glass juice bottle market has succumbed to PET. Hot-fill ready-to-drink tea is next. Finally, a range of food products require hot fill at >90°C/194°F and demand gas barrier properties at least 3-4 times greater than that which is generally characteristic of commercially available, standard oriented PET containers. These include tomato-based products, spaghetti sauces, jams, preserves and pickles. The successful development of these markets will depend on the availability and commercialisation of new filling technologies, closures and improved container barriers over the next few years. Current hot-fill containers are available in the larger multiserve
PET PACKAGING TECHNOLOGY
(family) sizes with better surface-to-volume ratios and are more suited to the cash-and-carry and club warehouse markets. The smaller sized, single-serve containers will require the extra barrier to deal with their higher surface-to-volume ratios. A fourth product group is developing comprising future food products with process and shelf-life requirements even more rigorous than those noted above. These are the retorted and/or pasteurised products, which are either extremely oxygen sensitive or require the higher barrier to deal with the higher surface-tovolume ratio prevalent in the smaller sized containers. This category includes baby foods, pet foods, meats and beer (which is a growing category for the PET bottle market). It should be noted that work is underway to develop appropriate PET bottles for tunnel pasteurising beer by combining manufacturing technologies for heat stability and barrier. Today, beer is almost always cold filled into PET containers. 2.4
Packer/filler shelf-life requirements
Packer/fillers (and brand owners) are examining their current practices in order to move more products into PET to increase market share. While there may be little flexibility in processing or product formulation for some food and beverage products, it is believed there is significant flexibility regarding shelflife requirements when converting to PET. A range of factors can impact the shelf-life performance of the food or beverage product, in particular gas permeation through the sidewalls and closure, and UV light penetration through the sidewalls. Frequently the first introductory packs produced when switching to PET have to match the shelf-life requirements (and process and filling conditions) of the 'old' package (usually glass or metal). This requires a high performance specification from the PET container. Once the launch has proved successful, ongoing development of the food or beverage product being packed, as well as the processing and filling conditions, usually leads to a reduction in the performance required from the pack and the packed costs. This is a commercial consideration worth making when starting development of a new food or beverage product. Priority is often given as to how these developments can be commercialised with minimum additional capital either at the container manufacturer or packer/filler stage. An assessment of the real, commercial, shelf-life requirements might allow some developments to be brought forward and implemented to avoid any re-tooling later on (e.g. lightweighting, or some might say 'right' weighting!). This is also important if capital is required to produce an extended shelf-life package, which is subsequently not required before the capital has been depreciated.
Oxygen scavengers are being developed which will mop up oxygen (contained in the headspace, entrained in the product, or having entered the container by sidewall permeability) to extend the shelf-life. These can overcome the need to develop special high-performance, costly PET containers. When carbon dioxide loss is an issue, it is important to consider the mechanisms that lead to loss. First of all, a pressurised PET container will relax immediately after filling and capping. Then there is 'sorption', when the COi migrates into the sidewalls of the container before reaching the outside and when steady state permeation occurs. Careful container design and 'right' weighting can help to reduce these losses. The permeation rate can be increased if the container is stored at elevated temperatures. The shelf-life can be halved for every 10°C/50°F above 25°C/77°F. This is an important consideration if carbonated products are to be shipped in regions of continuously elevated temperatures or warehoused in high ambient temperatures. Another factor to consider is the impact of UV light. As the beer sector for PET bottles grows, it will be mainly in the single-serve market and UV will play a major part on the resultant shelf-life. This will require developments in UV light barriers (in the 350-450 nm wavelength band), therefore we see mainly amber coloured PET bottles for beer. In Japan, however, all coloured PET will be eliminated from I April 2002! Thus, we will see developments in the area of increasing UV barrier for clear PET containers in the coming years. 2.5 2.5. /
Cost and performance considerations Material pricing
For the packer/filler or brand owner switching to PET, a key concern is the potential for container price fluctuation due to variable resin prices. When resin availability decreases prices are raised; generally, this is a cyclic phenomenon. When new resin capacity comes on stream the additional capacity generally weakens or, at best, holds prices. As the volume of the PET container market grows, there comes a point when container demand matches resin capacity. Beyond this point the resin prices tighten until new capacity is brought on stream and the whole cycle repeats itself. Being a polyester, there are valuable end-use markets for PET resin other than just bottle grade, namely, fibre grade. After a poor cotton crop in a major producing country, there is increased demand for polyester fibre grade resin, thereby squeezing out some capacity from the bottle grade resin, and so increasing pressure on bottle grade prices. It is this swing between different PET resin markets which can have a greater effect on bottle grade price stability than pure oil pricing, which impacts all of the resin industry. This is a point worth bearing in mind when considering long-term price forecasting.
PET PACKAGING TECHNOLOGY
In-house manufacture of PET containers for packer/fillers
A further consideration for a packer/filler, from a cost and performance perspective is whether to go in-house with container production. The economic entry barriers for the manufacture of PET containers are much lower than for glass containers, particularly for the reheat, two-stage, stretch blow moulding systems, thereby making self manufacture of PET containers a reasonable possibility. This fact is unlikely to be a significant driver at the time of converting from, say, glass to PET. However, it will be an opportunity to be evaluated once conversion has taken place and the volume of bottles being used is sufficient to justify the investment in equipment, and will typically be carried out as part of a cost-reduction initiative. Direct container cost comparisons almost always favour glass, but an expanded systems cost analysis, including distribution and handling costs (inbound and outbound), will reduce or eliminate this differential. When analysing the cost benefits for making a change in container materials (e.g. when switching from glass to PET) and outsource container supply to inhouse supply, a number of cost factors, in addition to base container cost, must be included. These are called system costs and include such as factors as: • • • •
inbound container freight warehousing costs of thefinishedproduct outbound freight elimination of glass breakages
Some of these factors lend themselves to fairly straightforward quantitative analysis (e.g. outbound freight), while others are very difficult to quantify and might be deemed 'soft' benefits, such as ease of handling lightweight, unbreakable containers, and reduction in noise when handling on a packing/filling line. 184.108.40.206 Inbound container freight Inbound container freight of (outsourced) empty containers is unlikely to play a significant part, as the weight consideration will probably not reduce the vehicle movements. However, this factor will become significant when considering inhouse container production, where the incoming freight would then be carrying preforms instead of full-sized containers. 220.127.116.11 Finished product warehousing costs This is an area where it is difficult to be quantitative. The top load resistance for PET containers filled with a still product is lower than that for glass and can lead to higher warehousing costs, depending on how high the finished product is stacked. Most modern warehouses are equipped with racking; if this is not the case through the complete supply chain, then the system cost will generally favour glass or cans.
However, PET stack strength for cold-filled bottles can be (and is) increased by liquid nitrogen dosing just before capping. This assumes that the bottle design can take pressure without significant distortion. 18.104.22.168 Outbound freight Outbound freight costs of filled containers are likely to show a significant improvement with use of PET compared to glass. Based on the weight of filled PET containers, which are less 'bulky' than glass, it is possible to show that the total vehicle movements can be 25-30% less than the equivalent glass containers, producing a significant cost reduction. That is, trucks carrying filled PET containers 'cube-out' before they 'weigh-out'. Reduced weight loads also permit use of trucks with lower cost specification. 22.214.171.124 Breakages in-plant Breakages in-plant have improved considerably over recent years as manufacturers have developed methods to handle containers more gently. However, past studies have shown that in-plant breakage costs can amount to 1 % of filling and packing costs, excluding the cost of the lost product. 126.96.36.199 Breakages in distribution Breakages in distribution have been shown to be capable of running at 0.5% or higher. This is variable subject to the distribution infrastructure. The more handling and trade channels serviced, the higher the potential breakage levels. Operator and consumer safety may also be a point to be considered. 2.6
When considering the impact of recycling on the selection of alternative forms of packaging and, in particular, on the specific recyclability of alternative materials, one must consider distinguishing between what can be done, what is in fact being done, and the public perception of what is being done. Glass, aluminium cans and PET are all recyclable. That is, if collected, sorted, cleaned and appropriately handled, these materials can be reused in a manner that extends their respective life cycles, conserves material and avoids consigning containers to a landfill. However, plastic (and specifically PET) and glass each present distinct issues, particularly when considering 'closed loop' bottle-to-bottle recycling, and each has a different public perception barrier to overcome. Other, more added value, end-use opportunities need to be developed beyond 'bottle-to-bottle' recycling, as raising the recyclate quality to food grade is costly. Recycling is discussed in more detail in Chapter 11 of this volume.
PET PACKAGING TECHNOLOGY
End-use market penetration
Precise unit volume numbers for individual categories of beverage and food products are very difficult to obtain. Food and beverage companies guard their own product volumes very closely, while industry trade associations and government agencies, which used to track industry-wide numbers, have increasingly cut back on these activities. While current market data may be difficult to find, the trends in the contest between PET and glass containers are very clear. In recent years, the use of PET CSD bottles has continued to grow strongly, while use of glass has decreased by a corresponding amount. In the US, CSD glass containers have virtually disappeared, except for a few small restaurant sizes. PET has now established a strong base in a number of non-hot-fill food applications (i.e. edible oil, some ketchups, peanut butter, pourable dressings). Further market penetration has been achieved in hot-fill juice, teas and isotonics, as well as applications beyond food packaging in the personal care, household and do-it-yourself markets. As is always the case with new packaging materials, the obvious and easy applications are achieved first. Then, building on these successes and given a high level of consumer acceptance (which PET has), packaged goods companies look for other areas where the new material will fit and increase their market share. PET has moved into this phase. The new applications will require higher thermal stability and improved barrier to gas and UV light. The resin, equipment and container manufacturers are all improving their products to satisfy new market expansion opportunities. The hot-fill market for PET containers continues to grow. Multilayer and coated, high-barrier bottles continue to be developed for single-serve size PET bottles requiring improved shelf-life due to the increased surface-to-volume ratio or for packaging more oxygen-sensitive products. The opportunity to manufacture clean bottles, to keep them clean and clean fill soon after bottle manufacture, will lead to new market developments, including cold aseptic filling. This will further increase the switch from glass and metal cans. The perceived quality of products packed in glass compared to those packed in PET has narrowed, and in some markets PET has overtaken glass. This will further facilitate the conversion to PET and will be worth serious consideration when assessing future packaging needs for packer/fillers and brand owners. PET has become the material of choice for so many markets that it will continue to go from strength to strength for many years to come. References The following reports are produced by Business Development Associates. Inc.. Bethesda. MA. USA. 1. Technology, Markets and Prospects: PET Packaging in Foods and Beverages in the US. 1994. 2. High Performance Polyester Packaging for Foods and Beverages. 1996.
3. Improved Gas Barrier and Thermal Properties for PET-based Containers: Polyester Packaging, The Critical Path Ahead, May 1997. 4. Custom PET Markets—and the Technologies Which Will Drive Them—PET Strategies, 1998. 5. Custom PET Packaging for Foods and Beverages, 1998. 6. Beer in PET (parts 1-3), 1999-2000.
PET materials and applications Kenneth M. Jones
This chapter describes polyethylene terephthalate materials specifically designed and made for the packaging industry, including their manufacture, properties and performance. The development and properties of copolymers produced to meet specific processing needs and/or end-use requirements is considered, including injection stretch blow moulding, extrusion and forming, film manufacture, and materials with improved gas barrier and environmental stress crack performance. Over the past 25 years, synthetic polymeric materials have played a significant role in enhancing the ability to package materials— especially foodstuffs—in a safe and convenient manner that is appreciated by both the retailer and the consumer. PET polymers have played a major role in this area, with significant developments obtained in high-barrier containers for carbonated soft drinks (CSDs), high strength films, excellent gas barrier packaging for sensitive foodstuffs, and materials of high clarity. PET-based polymers have shown great versatility in their applications from the time they were first developed in the early 1940s by Whinfield and Dickson [1, 2]. In those early days, the polymer was used specifically in synthetic fibre applications—this is still one of its major uses [3,4]. These products were based on the uniaxial orientation of the polymer chain. Several polyester polymer variants have now been developed to meet this sophisticated end-use market. During the latter part of the 1950s, both ICI and Dupont led in the development of second-generation products based on the biaxial orientation of extruded amorphous film. These developments produced highly oriented film products, to compete initially against the cellulose-based products in applications such as X-ray films, insulating films, audiotapes and food-packaging films. A highly intricate drawing and heat setting process technology was developed and is used to produce a quality film of high integrity to meet these highly demanding market applications. Over the past quarter century, several new film products have been developed by various polyester film producers to meet many challenging new markets. In the mid 1970s, Dupont technical group developed and patented technology that led to the production of third generation materials that had a three-dimensional oriented structure. The work, led by Wyeth  at the Dupont experimental station, demonstrated that bottles and containers produced by this new technique of
PET MATERIALS AND APPLICATIONS
injection stretch blow moulding (ISBM) had exceptional strength and excellent gas barrier properties. This development again revolutionised the polyester industry and allowed the polymer to be used as a replacement for glass in bottle manufacture. In all three developments, the major polymer backbone component is PET, which is the resin originally developed by Whinfield and Dickson. This is a polycondensation polymer based on the reaction of terephthalic acid and monoethylene glycol. The polymerisation reaction is represented in simple form by the following equation: n HOOCC6H4COOH + (n + 1)HOCH2CH2OH = HOCH2CH2O(OCC6H4COOCH2CH2O),7H
The initial polyester produced by Whinfield and Dickson was made using the precursors dimethyl terephthalate and monoethylene glycol, respectively; however, the majority of today's newer polymer production plants use pure grade terephthalic acid (PTA) and monoethylene glycol as the raw materials. To meet more stringent downstream processing requirements and product end-use properties, the majority of today's polyester polymers used in the packaging industry are based on novel copolymers. 3.2
Polymerisation and manufacturing processes
PET is produced by a polycondensation reaction, using one of the following series of initial chemical reactions: the ester interchange of dimethyl terephthalate with monoethylene glycol, the direct esterification of terephthalic acid with monoethylene glycol, or the reaction of ethylene oxide with terephthalic acid to form, initially, the monomeric and low molecular weight oligomeric precursors with various monoethylene glycol to acid ratios depending upon the route used. In the former two processes, the oligomeric mixture is polymerised without further purification, while in the latter process the monomeric species, bis hydroxyethylene terephthalate (BHET), is extracted and purified from the resulting reaction products. The need for this additional purification stage has made this process uneconomical and it is not used in practice. The ester interchange reaction is carried out in the presence of a catalyst, usually a salt of a transition metal, such as manganese, cobalt or zinc, or an alkaline earth metal, such as calcium. The reaction is allowed to proceed until more than 99% of methanol is released, using a high mole ratio (2:1) of monoethylene glycol to ester and a rising temperature profile, starting at a temperature of around 160°C and rising to around 230°C to allow the reaction to proceed to completion. The ester interchange catalyst systems are potential degradants at high temperatures, and phosphorus-based stabilisers, such as
PET PACKAGING TECHNOLOGY
phosphoric acid, are added prior to polycondensation. The reaction equation is shown below: 2HOCH2CH2OH + C 2CH3OH
The direct esterification reaction is usually carried out in the absence of a catalyst, although metal alkoxide compounds of titanium, tin and antimony are known to catalyse the reaction. The solubility of terephthalic acid in monoethylene glycol is very low and the reaction is carried out at temperatures in excess of 240°C and usually in the range 260-290°C, using a mole ratio of monoethylene glycol to acid of around 1 .2 to 1 . This gives acceptable reaction rates allowing the process to be completed (degree of esterification of around 93%) within acceptable times: 1.2HOCH2CH2OH + HOOCC6H4COOH = HOCH2CH2O(OCC6H4COOCH2CH2O),, OCC6H4COOH + 2 H 2 O
where, n is the average degree of polymerisation for the oligomeric reaction product and is usually in the range 3-10. The high acidity of the terephthalic acid catalyses the formation of diethylene glycol and this must be controlled at an acceptable level to give consistent polymer properties. Both alkali and alkaline earth metals as well as quaternary ammonium compounds can be used to bring about a significant reduction in the level of diethylene glycol formed. This can be formulated as follows: HOCH2CH2OH + HOCH2CH2OH = HOCH 2 CH 2 OCH 2 CH 2 OH + H 2 O
Polycondensation reactions are equilibrium reactions; therefore, to allow the polymerisation reaction to proceed, the level of free monoethylene glycol and water must be reduced quite significantly. The equilibrium constant for this reaction favours the low molecular weight oligomeric species, and thus, in the most conventional manufacturing plants, the reaction takes place in the melt phase at relatively high temperatures under vacuum. The use of a polymerisation catalyst is essential to allow the reaction to proceed to acceptable molecular weights. The most common catalysts in current use are: antimony compounds, such as antimony triacetate, antimony glycoloxide and antimony trioxide; germanium compounds, such as amorphous germanium dioxide and germanium glycoloxide; and titanium compounds, such as titanium alkoxides. High acid ended oligomeric product from the reaction of monoethylene glycol and terephthalic acid can be polymerised to moderate molecular weights without
PET MATERIALS AND APPLICATIONS
the use of a catalyst; however, the reaction time is quite long. It is also usual to add small quantities of melt stabilisers—such as compounds based on phosphorus, including phosphoric acid and its esters—to reduce thermal degradation and colour formation. Typical conditions in current use on a continuous manufacturing plant are: melt temperatures in the range 270-300°C and a pressure of less than 5 millibars in the final reactor. In a batch process, it is essential to achieve lower final reactor pressures to obtain adequate molecular weight build up. In this case, the final pressure should be less than 2 millibars. Polymers can be produced to various molecular weights using either the continuous or the batch process. In practice, the molecular weight will be targeted to end-product requirements. The reaction is represented by the following equation: HOCH2CH2O(OCC6H4COOCH2CH2O),7H = HOCH2CH2O(OCC6H4COOCH2CH2O),M H + HOCH2CH2OH
where, m is the average degree of polymerisation for the polymer species. However, in the melt process a small quantity (less than 50 ppm) of acetaldehyde is produced from the degradation of the monoethylene glycol entity. This can give rise to taint of some sensitive foodstuffs, such as mineral water and CSDs, and must be reduced or removed prior to use in the packaging of these materials. For this reason, polymer used in these applications is produced in the solid state at significantly lower processing temperatures. In the solid-state polymerisation (SSP) method, the low molecular weight polymer precursor is produced by the melt phase process, as described previously [7-9]. Pellets of the amorphous polymer, with a number averaged molecular weight (Mn) in the range 15,000-25,000, which are produced by the melt phase process, are first heated at temperatures of around 160°C using good agitation under a positive dry gas stream, usually nitrogen, to develop primary crystallinity. The pellets are then gradually heated with good agitation and under a positive stream of dry nitrogen gas (dew point less than —40°C) to around 210°C to anneal and develop a higher level of crystallinity (around 48%). Good agitation is critical during these two stages to eliminate the tendency for the amorphous and the nonannealed crystalline pellets to stick and sinter together. The crystalline pellets are held at this or slightly higher temperatures under a positive stream of dry nitrogen gas (dew point less than —60°C) to allow the polycondensation reaction to proceed to the required molecular weight. The solid-state polycondensation reaction can yield a very pure grade of PET with very low levels of acetaldehyde (less than 2 ppm). For conventional injection stretch blow moulding and sheet extrusion applications, polymer is produced to Mn in the range 25,000-33,000. The reaction can also produce polymer to a significantly higher molecular weight than the melt phase process, which is suitable for extrusion blow moulding applications. For this type of application polymer with Mn greater than 35,000 is required. On achieving the required Mn, the pellets are cooled to temperatures
PET PACKAGING TECHNOLOGY
below 100°C under a positive stream of dry nitrogen gas to minimise hydrolysis and degradation. The polymerisation reaction can be summarised by the following equation: HOCH2CH2O(OCC6H4COOCH2CH2O),nH = HOCH2CH2O(OCC6H4COOCH2CH2O)/,H + HOCH2CH2OH
where, p is the degree of polymerisation of the SSP polymer. Recently, Dupont have developed an improved process for the production of PET for packaging applications [ 10]. In this patented process, the low molecular weight oligomeric compound produced by the reaction of terephthalic acid and monoethylene glycol is pelletised on a heated rotoformer (temperature around 1503C) and allowed to develop a highly crystalline structure. This structure is highly robust in character and allows the pellets to be fed directly to a solidstate reactor at temperatures in excess of 200CC without the risk of sintering. The polyester products arising from this process have similar properties and characteristics to conventional solid-state polyester products. 3.2.1 Manufacturing plants As indicated in Section 3.1, the monomer can be produced from pure dimethyl terephthalate (DMT) or pure terephthalic acid (PTA); however, for most packaging applications, polymers based on terephthalic acid are preferred. Most manufacturing plants today use highly sophisticated continuous processing routes to produce PET polymer for the packaging industry. A typical modern continuous plant will have a three or four vessel reactor, depending upon the technology used . In a typical four-vessel plant , the first vessel is a primary esterifier operating under atmospheric or slight positive pressure (1 -2 bar) and temperatures in the range 260-280CC. A slurry mixture of monoethylene glycol and terephthalic acid at a mole ratio of around 1.2 to 1 is fed into this vessel continuously. The reactor is designed as a stirred tank and steady state conditions are controlled to give a degree of esterification of around 90%. The reaction product is fed from the primary esterifier to a second vessel that is again designed as a stirred tank to give complete mixing. The product is reacted at temperatures in the range 270-290CC under atmospheric or slightly reduced pressures (600 millibars), and steady state conditions are controlled to give a degree of esterification greater than 94%. The product from the second vessel is then fed to a third vessel, whose primary function is to take off excess monoethylene glycol and to allow the initial polymerisation reaction to occur. The conditions in this vessel are set to maximise the build-up in molecular weight without excessive carry-over of solids with the liberated monoethylene glycol. Most production plants operate at temperatures around 280 C and pressures in the range 15-30 millibars. Steady
PET MATERIALS AND APPLICATIONS
state conditions are controlled to give a degree of polymerisation of around 30% and a molecular weight of around 6,000. The fourth reactor is referred to as the high polymeriser and is designed to give the polymer maximum surface area to allow the release of monoethylene glycol and other volatiles to occur readily. There are several patented reactor designs in use consisting of a horizontal cylindrical vessel with a purpose designed horizontal agitator that moves the polymer in a plug flow with some localised back mixing through the unit. This design allows the molecular weight to build up gradually across the vessel. The polymerisation reaction is carried out at temperatures in the range 275-290°C and pressures of less than 5 millibars. The molecular weight is controlled at around 15,000-20,000 depending on end-use requirements. Higher molecular weight products can be produced, up to around 33,000, at lower throughputs or using purpose-designed plants. Polycondensation catalysts and other additives (such as stabilisers) are added to the transfer line between vessel one and two or between vessels two and three. In a typical three vessel plant patented by Dupont , the first esterification vessel consists of a unique design that allows the monomer to circulate at high rates without mechanical agitation, using differential pressures from the initial high gas release at the feed end to siphon the product round the unit. A slurry mixture of monoethylene glycol and terephthalic acid at a mole ratio of around 2.0 to 1 is fed directly into the vessel immediately below the heating calandria. Both water from the esterification reaction and excess monoethylene glycol are vaporised and the relative density is reduced to force circulation within the unit. The reaction conditions are controlled at atmospheric pressure and temperatures in the range 270-290°C to give a steady state product with a degree of esterification of about 90%. The second vessel is referred to as the 'up-flow pre-polymeriser' (UFPP) unit and is designed to take the excess monoethylene glycol and volatiles off efficiently without too much solid carry-over, while allowing good molecular weight build-up to occur. The reaction product from the esterifier is treated with additional monoethylene glycol and preheated to a temperature of about 280°C prior to entry. The pressure at the top of the reactor is reduced to around 20 millibars to enhance the removal of excess monoethylene glycol, water and other volatiles and to allow molecular weight build-up to occur. The product exiting the reactor has a degree of polymerisation of around 30 and a molecular weight of about 6000. Again, the reaction product is fed to a horizontal polymerisation vessel, as described above. However, in the Dupont finisher, the horizontal agitator has extra wiper blades that smear the surface wall. This gives additional surface area to enhance molecular weight buildup and eliminates the accumulation of degradation by-products on the reactor wall. Again, the polymerisation reaction is carried out at temperatures of around 280-290°C and pressures of less than 5 millibars, and the molecular weight is controlled at around 15,000-20,000 depending upon end-product requirements,
PET PACKAGING TECHNOLOGY
Higher molecular weight products can be made at lower throughputs or in a designated purpose-built plant. Catalysts, stabilisers and other additives are added with the raw materials or into the transfer line between the esterifier and the UFPP reactor. On all continuous plants, patented melt viscosity measurement devices are placed in the extrusion manifold to measure and control the molecular weight to the required specification. Copolymers using other diacids, such as isophthalic acid or 2,6 naphthalene dicarboxylic acid, other glycols, such as diethylene glycol or cyclohexane dimethanol (CHDM), or a mixture of both acids and glycols can be produced on continuous plants. These additives can be added as separate slurries or as a mixture with the terephthalic acid and monoethylene glycol. They would normally be added to the esterifier but can be added later, in smaller quantities, to the transfer line prior to the secondary esterifier or the UFPP vessel. Batch reactors are currently only favoured for the production of speciality polyesters containing high additive levels, copolymers which have low sales volume or which are difficult to handle on continuous plants, and the highly branched polyesters. A batch plant will usually consist of two reaction vessels: an agitated esterification pressure kettle that can handle both dimethyl terephthalate and terephthalic acid as the raw materials, and a polymerisation pressure vessel that can hold vacuum down to pressures less than 1 millibar. Additives and copolymer components can be added with the raw materials or separately to either vessel in the transfer line between the esterifier kettle and the polymeriser. The polymerisation is carried out in the temperature range 270-300 C and a final reactor pressure less than 2 millibars (and preferably less than 1 millibar). The molecular weight build-up is controlled to the required level by measurement of the torque applied to the agitator. A typical modern, continuous, solid-state polymerisation manufacturing plant will have four major reaction vessels . The polyester amorphous pellets produced on a melt phase process are fed continuously into a fluidised bed reactor or a highly mechanically agitated horizontal reactor. Here they are heated, by a positive flow of dry gas or a combination of gas and surface heaters, to a temperature around 160°C, in order to initiate primary crystallisation. The residence time (around 10-15 min) is controlled to ensure that the pellets are completely crystallised, so reducing the tendency to stick. The crystalline pellets are subsequently fed to a second reactor that can be designed either as a purpose-built column reactor, such as is used in the Buhler process, or a mechanically agitated horizontal reactor, as developed by Zimmer and Bepex. In both cases, the pellets undergo gradual heating in a positive flow of dry nitrogen gas to temperatures around 210CC. They are treated at this temperature for a period, usually around 30 min residence time, to anneal and develop a more robust crystalline structure. Differential scanning calorimetry (DSC) monitors the changes that occur in the polyester morphology at this stage in the process. Typical changes are shown in Figure 3.1.
PET MATERIALS AND APPLICATIONS Heating rate 20°C/min
200 220 Temperature (°C)
Figure 3.1 Use of DSC information to control SSP column temperatures. Heating rate 20 C/min. Abbreviations; Tc, crystallisation peak; Tf, secondary melting exotherm; Tm, primary melting point; SSP, solid-state polymerisation; DSC, differential scanning calorimetry.
The melting characteristics of the secondary crystals that are formed on annealing are closely monitored through measurement of the melting exotherm (Tf). The SSP process conditions are chosen such that Tf is always a few degrees above the temperature of the pellets. The highly crystalline pellets are transferred continuously to a vertical column reactor, heated with a positive counter current of hot dry nitrogen gas (dew point — 60°C) to temperatures around 210°C to allow the polymerisation reaction to proceed. The temperature of the pellets and the gas in the column must be accurately controlled to within one degree Celsius, and kept a minimum of 5°C below the annealing temperature to eliminate any tendency to sinter. The pellets will have residence times of several hours within the reactor, depending upon molecular weight requirement and copolymer content. As indicated in Section 3.2.1, the solid-state process is highly versatile in terms of molecular weight build-up and can produce a product to a range of molecular weights ranging from 20,000 to over 80,000 by changing residence times and reaction temperatures within the column. However, it is important that the gas flow is not hindered or allowed to channel through the pellet bed, otherwise a product of non-uniform molecular weight is obtained. In all plants, trickle samples are taken from the bottom of the column for testing in order to control the molecular weight within the required specification. The pellets are transferred from the reactor to a cooling unit that has a positive
PET PACKAGING TECHNOLOGY
feed of cold dry nitrogen gas (dew point less than — 40CC) to reduce tendency for moisture uptake and to prevent hydrolysis taking place. This unit can be designed as an extension to the column reactor, a separate fluid bed, or an additional horizontal vessel with mechanical agitation, such as a thermoscrew. In addition to the vessels mentioned, these plants contain sophisticated gas cleaning and purification units. The gas cleaning systems are also used to clean the pellets, removing fine dust and powder that is formed from the attrition occurring within the handling system. High levels of crystalline dust can have a deleterious influence on most downstream processing.
Structures, morphology and orientation
3.3.1 Structures The structure of PET is based on the multiple build-up of the repeat unit monooxyethyleneterephthalate (—OCH2CH2OOCC6H4CO—) that is derived from the esterification of the terephthalic acid and monoethylene glycol entities. The combination of both the aromatic terephthaloyl and aliphatic ethylene glycol units closely defines its unique properties. In considering the physical structure of this polymer, it is best to start with the single chain and then examine the arrangement of a number of chains with respect to each other. The arrangement of a single chain is governed by the various alternative conformations of the molecule due to rotation of the many single bonds in the structure. When many molecules come together, they may form amorphous or semi-crystalline structures depending on the nature of the molecule and the thermal history to which the sample is subjected. PET exists in both amorphous and semicrystalline forms. Part of the polyester molecule is shown in Figure 3.2, where the repeat unit is shown between the dotted lines. The aromatic ring (paraphenylene unit) is planar and, together with the associated —CH2CH2— on either side of the ring, it forms a single rigid structure. Rotational movements within the chain are limited to the other single bonds in the structure (—C—O— and —C—C— bonds). The chain repeat distance, as determined by X-ray diffraction studies, is 10.75 A, which is slightly less than that of a fully extended, linear, zigzag chain. The average length of the molecular chains in polyester polymer used in the packaging industry lies typically between about 0.1 and 0.2 um. However, for extrusion blow moulding polyester grades the chain length is more likely to be as high as 0.3 um. The aromatic terephthaloyl unit in combination with contribution from some hydrogen bonding between the carbonyl oxygen and the ethylene hydrogen groupings gives the PET molecule good rigidity and high modulus. The carboxyl grouping on the ethylene —C—C— bonds can take a gauche or trans conformation. In
PET MATERIALS AND APPLICATIONS
Figure 3.2 Polyethylene terephthalate: chemical repeat unit.
the amorphous state, the molecules are mainly in the gauche form; however, on crystallisation the molecule transforms to a trans configuration. The polyester molecule can also take the trans configuration when it is oriented.
Early X-ray diffraction work indicated that highly ordered or crystalline entities with highly structured shapes (micelles) of around 100-200 A in size were present in the polymer. However, since the molecules are significantly longer than the micelles it was concluded that the individual chains pass through a number of the highly ordered or crystalline regions, alternating with segments in the amorphous or disordered regions to give integrity to the system. The amorphous phase is assumed to form the matrix. These characteristics were the basis of the fringed-micelle model that was proposed in 1930 [15-17]. The model explains many of the characteristics associated with polyester polymer, including strength, durability, cohesion, gas barrier properties and heat setting, that are associated with crystalline regions. The non-crystalline regions are mainly responsible for extensibility, recovery, toughness and diffusion. The structural basis for the fringed-micelle model is that, on coming together, the favoured arrangement that the molecules take is one in which the free energy is at a minimum. The free energy state at high temperature, when the molecular mobility is too high for intermolecular bonding to be effective, is the random state. At lower temperatures, the molecules become less mobile and local
PET PACKAGING TECHNOLOGY
Figure 3.3 Molecular structure: modified fringed-micelle model showing crystalline/ordered domains with the chain molecule linking both amorphous and crystalline regions.
alignment of neighbouring areas of various molecules can take place to minimise free energy. Further work, especially using single crystals [18,191, has allowed the theory to be developed. In the late 1950s, direct evidence for folded chains was provided by electron diffraction studies on single crystals. Subsequently, folded chain structures were shown to be present in melt grown crystals. To accommodate for this observation, the fringed-micelle model was modified to show that a single molecule could fold back and forth within the micelle, as shown in Figure 3.3, as well as passing through both crystalline and amorphous regions. Although extended chain crystals have the lowest free energy, the chains prefer to crystallise by folding, since this allows the crystallisation to proceed rapidly. This indicates that the considerations are kinetic in nature and are not in the steady state of equilibrium. Consequently, the lamellar crystals are not in their most stable form and will always be liable to change when suitable conditions prevail, such as on subsequent heating. This is of fundamental importance to understanding the changes that can occur in PET on heating and is a prime cause for the changes observed in the pellet morphology during SSP. It is also important to the understanding of the mechanism as applied to heat setting (as discussed in detail in Chapter 10). In the latter case, the final structure of the article is a function of its entire thermomechanical history. However, the alternative paracrystallinity model proposed by Houseman , which assumes the amorphous regions to be small defects in the crystalline structure, best describes properties such as creep and barrier. This model shows the presence of voids and motions due to the dislocations.
PET MATERIALS AND APPLICATIONS
Injection-moulded articles (such as preforms) and extruded sheet are essentially amorphous in character and various models have been proposed for their structure. All these models recognise the presence of an entangled molecular network. However, some researchers believe that the structure is not homogeneous, and that in addition to the network some crystal nuclei or extended chain molecules are present. There is evidence from work carried out by Windle and co-workers at Cambridge University, Cambridge, UK (personal communication) that some alignment occurs in the amorphous state prior to crystallisation in PET cast film, and especially in the presence of the more rigid naphthalene 2,6 dicarboxylate copolymer entity. These structures can have a significant influence on the performance of the amorphous article in any subsequent stretching process. If one considers how the network responds to stretching in various industrial processes where the drawing stresses are relatively high, it is clear that the entanglements will hinder the movement of molecules during the stretching process, and as the stretch ratio increases the ease of movement becomes more difficult. The influence and benefit of these entanglements are clearly shown in the load-extension curves shown in Figure 3.4 for PET. In the initial stages, the system obeys the normal laws of physics, with the stress increasing sharply with strain and the polymer matrix acting as an elastic; however, as the stress
120 - -
Figure 3.4 Load-extension curves for PET.
PET PACKAGING TECHNOLOGY
is increased beyond a critical level (the yield point) the polymer yields and the stress falls back slightly. At higher strain levels, the stress is again observed to increase sharply as the entanglements restrain movement and strain hardening sets in prior to rupture. As the stress increases, the molecules develop significant levels of orientation along the stretch direction, which contribute to high strength products in industrial processing. At the higher stretch ratios, the chain movement contributes to localised heating and some additional crystallisation occurs. These crystals can give some degree of thermal stability to the system and will influence the level of shrinkage occurring at higher temperatures; however, the level of crystallisation is not sufficient to give dimensional stability above the glass transition temperature (Tg). 3.3.3 Orientation In practice, the stretching performance of PET is dependent on: temperature, molecular weight, strain rate, crystallisation, moisture, and copolymer type and composition [21-29]. The influence of temperature is shown by the stress/strain curves in Figures 3.4 and 3.5. At low temperatures, the stress increases sharply up to the yield point, and then falls back as the polyester molecules yield. Under these conditions, the work involved in straining the molecules generates heat and a rise in temperature of several degrees is observed at the yield point. Invariably, necking occurs under these conditions leading to a localised thinning and nonuniform stretch. As the temperature is increased to around the Tg. a much Homo polymer
Sheet IV 0.75
Figure 3.5 Uniaxial stretch of PET sheet at various temperatures. Abbreviation: IV. intrinsic viscosity.
PET MATERIALS AND APPLICATIONS
Table 3.1 Properties of uniaxially stretched sheet Draw ratio 4.5 4.5
Draw temp. C
% Shrinkage (BW)
Tensile strength MPa
Extension at break %
1.99 0.5 1
Homopolymer: IV 0.78. Abbreviations: IV, intrinsic viscosity; BW, boiling water.
more uniform and controlled yield is obtained. At higher strain levels, the stress increases sharply again as strain hardening sets in prior to rupture. To produce both strength and rigidity (modulus), as are required for both films and bottles, it is necessary to develop a degree of hardening (high orientation) at the stretching stage. As the resin temperature is increased to above 110°C, the molecules flow more readily and a much higher stretch is required to achieve strain hardening. Test results (see Table 3.1) indicate that the level of orientation attained at the higher stretch under these conditions is less than that obtained at the same stretch ratio at the lower temperature. This is reflected in a lower tensile strength, higher extensibility at break and lower shrinkage. The optimum processing conditions for homopolyester are seen to be 85-105°C. These conditions will change if the Tg is affected by copolymerisation. Molecular weight also has a significant influence on the stretching characteristics of PET. The molecular entanglement associated with the higher molecular weight resin has a more restraining influence on the molecules. In this case, the higher molecular weight polymer (see Figure 3.6) has a higher stress yield point, whilst the strain hardening occurs at a lower stretch ratio. For good process control it is important, therefore, to control the molecular weight within a tight specification. As anticipated from the entanglement theory, strain rate can also have a significant influence on the properties of the final product. At high strain rates, there is considerable molecular resistance to chain disentanglement and movement. The stress/strain curves (see Figures 3.7 and 3.8) show a significant increase in the stress yield point, and strain hardening occurs at a lower stretch ratio as the strain rate is increased. At very high strain rates, one sees a significant increase in temperatures at strain hardening and a higher level of crystallinity is obtained in the product . The influence of crystallinity is to contribute towards the resistance in the molecular movement during the stretching process. As the level of crystallinity increases, the stress level to yield increases (higher modulus) as the product has become more rigid and brittle. Similarly, the stretch ratios show a decrease with increased crystallinity (see Figure 3.9). It is important, therefore, in both film and injection moulding processes to minimise the level of crystallinity build-up during sheet casting and moulding, as well as at the product reheating stage prior to stretching.
PET PACKAGING TECHNOLOGY Sheet temperature: 95°C
Figure 3.6 Uniaxial stretch of PET sheet: influence of IV Abbreviation: IV. intrinsic viscosity.
3.0 Stretch ratio
Figure 3.7 Uniaxial stretch: influence of strain rate.
PET MATERIALS AND APPLICATIONS Simultaneous stretch: 3 x 2
51 IV 0.60
' 90°C -80100°C
Log strain rate (1/s)
Figure 3.8 Variation of yield stress with strain rate. Abbreviation: IV, intrinsic viscosity.
Water is a good plasticiser for PET and as such it can lower the Tg quite effectively . At high relative humidities (RH greater than 90%), the Tg is reduced by several degrees Celsius (see Figure 3.10). The level of moisture in the amorphous products prior to stretching can therefore have a pronounced influence on the film or container properties. The resultant effect is similar to stretching at higher temperatures: the molecules will be more mobile at lower temperature and the resin will flow rather than strain harden at the designed stretch ratio. Most polyesters used today in the packaging industry are copolymers, and even the homopolymers that are available on the market are not true homopolymers, since they all contain some generated or added diethylene glycol moieties. The influence of copolymerisation is dependent on the type of additive and on the level added. Aliphatic, longer chain glycols or aliphatic diacids tend to reduce the Tg and will therefore act in a very similar manner to plasticisers, such as water. In this case, as described above for water, the molecules are more mobile at lower temperatures and the resin will flow rather than strain harden under the standard homopolymer stretching conditions. When an aromatic copolymer additive is used in copolymer manufacture, its influence will be dependent upon its molecular structure. Molecules such as naphthalene 2,6 dicarboxylic acid will
PET PACKAGING TECHNOLOGY Temperature: 90°C
Figure 3.9 Influence of crystallisation on natural stretch ratio. Abbreviation: IV. intrinsic viscosity.
0.4 0.5 06 Equilibrium moisture content (%)
Figure 3.10 Influence of moisture on glass transition temperature (Tg).
53 increase the rigidity within the molecular chain, which will increase the apparent Tg and contribute towards reducing the mobility within the polymer matrix. In this case, higher temperatures are required to give satisfactory stretching. For molecules such as isophthalic acid, which act as chain disrupters, it is most likely that the overall crystallisation reaction occurring during the latter stages of stretching is hindered and thus the molecules have a greater freedom to flow. In these cases, it is found that strain hardening is delayed and that higher stretch ratios are required to obtain good physical properties. In the more complex processes used to manufacture film or bottles , it is possible to have sequential biaxial stretching, simultaneous biaxial stretching, or an intermediate situation as in preform blowing. Although the same principles apply, there is a significant difference in the mode of application. In this case, the polymer is more restrained in each direction during the draw down. This can have a bearing on the stresses involved; that is, higher stresses are observed during stretching. This effect is more pronounced under simultaneous biaxial stretching as well as for the sequential sideways draw. Typical stress/strain curves obtained under both sequential and simultaneous stretching of PET polymer are shown in Figures 3.11-3.14.
Forward stretch (x2)
Sheet IV 0.75
Figure 3.11 Sequential stretch of PET sheet. Abbreviation: IV, intrinsic viscosity.
Forward stretch (x2.5)
Sheet IV 0 75
Figure 3.12 Sequential stretch of PET sheet. Abbreviation: IV, intrinsic viscosity. Forward stretch (x3)
Sheet IV 0.75
30 Stretch ratio
Figure 3.13 Sequential sideways stretch of PET sheet. Abbreviation: IV. intrinsic viscosity.
PET MATERIALS AND APPLICATIONS Sheet IV 0.75
Figure 3.14 Simultaneous stretch of PET sheet. Abbreviation: IV, intrinsic viscosity.
As mentioned previously in this section, stretching the polyester beyond its natural draw can induce a degree of crystallisation in the polymer [28, 29]. This can have a significant influence on both the secondary draw in a sequential stretch process and the degree of setting achieved. The magnitude of the stress in the secondary draw is dependent upon the level of crystallisation developed during the forward draw, and therefore, to some extent, on the time delay between the forward draw and the start of the sideways draw. In the bottle blowing process, the delay is very short—less than 0.1 s—and thus the influence may not be as pronounced as that observed in the film process. However, the behaviour of the material in the sideways draw will be dependent upon the extent to which the polymer is oriented in the forward draw process. With a forward stretch ratio of 2.0 or less, a pronounced plateau is seen in the stress/strain characteristics of the sideways draw (see Figure 3.11). As the draw ratio is increased to 2.5 in the forward draw, the yield stress increases and the plateau disappears for stretch temperatures below 100°C (see Figure 3.12). At an initial stretch ratio of 3.0, higher stresses are observed for the sideways draw and the plateau is absent at temperatures below 110°C (see Figure 3.13). These results (see Table 3.2) again show that the effect of increasing the temperature is to reduce the level of orientation obtained for a given stretch ratio, increase the density and thus the degree of crystallisation, and reduce the shrinkage.
PET PACKAGING TECHNOLOGY
Table 3.2 Properties of biaxially stretched sheet (ratio 2.0 x 3.5) Shrinkage
Tensile strength (MPa)
Extension at break
14.4 17.4 21.6 26.7
20.4 12.0 6.0 1.6
20.4 9.7 4.4 0.9
Draw temperature =C
80 90 100 110
1352.3 1355.9 1360.9 1367.0
Homopolymer: IV 0.78. Abbreviations: IV. intrinsic viscosity: F. forward result: S. sideways result. Table 33 Properties of biaxially stretched sheet Tensile strength (MPa) Draw ratio Sequential stretch 2.6 x 4.0 Simultaneous stretch 2.6 x 4.0
Extension at break (^ )
Homopolymer: IV 0.78. Stretch temperature: 90 C. Abbreviations: IV. intrinsic viscosity: F. forward result: S. sideways result.
In the simultaneous stretching of the polyester polymer in both directions (see Figure 3.14), the stress rises more slowly than in the secondary sideways draw and a yield point is observed in the stress/strain curves at all temperatures. The curves are of similar character to those observed in the sequential process at low initial forward stretch ratio (less than 2.0). For a given draw, the sideways stretch needs to be greater to avoid uneven stretching than is the case with sequential stretching. For similar stretch ratios, the tensile properties of sheet are lower than those achieved by sequential stretching (see Table 3.3). The influence of molecular weight on both sequential and simultaneous draw is as anticipated. The higher molecular weight samples require a greater stress to stretch and reach the strain harden regime at a lower extension than lower molecular weight material. In the sequential sideways draw, it can be seen that the higher molecular weight sample draws at a slightly lower stress (see Figure 3.15). This is because a lower level of crystallinity is formed during the forward draw. In practice, the influence that molecular weight can have on the uniformity of stretching can be summarised using area expansion product (X L Xj) of the natural stretch ratios in the longitudinal and transverse direction against molecular weight—in this case represented by intrinsic viscosity (IV) (see Figure 3.16). The influence of moisture, crystallisation and strain rate are also as anticipated and mentioned previously in this section. However, the effect of copolymerisation will be dependent upon the influence that the copolymer component has on the level of crystallisation occurring during strain hardening. If the additive retards the crystallisation, then the sideways draw will require less stress to
PET MATERIALS AND APPLICATIONS
Figure 3.15 Sequential stretch: influence of molecular weight. Abbreviation: IV, intrinsic viscosity.
075 0.8 Intrinsic viscosity
Figure 3.16 Influence of intrinsic viscosity (IV) on area expansion draw
PET PACKAGING TECHNOLOGY
stretch; however, if the additive enhances crystallisation, then the sideways draw will require higher stress and the product is likely to show brittle failure at high stress levels. In addition to ensuring that good tensile properties are achieved, an understanding of the morphology of the polymer is important in ensuring that the integrity of the manufactured articles meets the customers' requirements. This is true of cast sheet, heat set film, injection-moulded preforms and containers, and blow-moulded bottles. If one considers and applies the fringed-micelle type model to these various applications, it is possible to envisage possible problem areas and probable remedies. In injection moulding, the temperature difference between the cold mould wall and the hot molten resin can give rise to different stress levels within the injection moulded article, which will cause the molecular chain to be stretched and become more oriented. In practice, these are observed as highly ordered laminar layers that in thick preform moulding can lead to stress crystallisation occurring within the preform (see Figure 3.17). A similar effect is also observed in cast sheet and especially in thick sheet, where the temperature difference between the calendering rolls and the hot
Oriented structure trapped at pressurisation stage.
Gradual reduction of orientation towards the centre of the mould as stress levels are lower and the cooling rate is slower and that allows more time for the orientation to relax.
Xi v/ l|l|'lt
Areas prone to stress crystallise during IM Figure 3.17 A) Influence of shear on injection moulding.
PET MATERIALS AND APPLICATIONS
Position across mould Figure 3.17 B) Shear rate profile across the mould.
extruded polymer can build up different stress levels across the sheet. In both cases, higher haze levels are observed within the samples and, on subsequent stretching, the product can delaminate. In the manufacture of bottles by ISBM, the heated preform is blown into a cold mould. If the preform has high crystallinity levels in the base or the molecular weight is not uniform, overstretching can occur in the petaloid base area leading to uniaxial orientation in critical stress areas of the container when under pressure (see Figure 3.18). In practice, this can enhance the susceptibility of the base to environmental stress cracking. All of these problems can be readily overcome by choosing the correct resin and tight process control. The morphology of the final product is also important in obtaining good gas barrier properties, in reducing creep, and in establishing hot-fill properties in the final product. These are discussed later under the appropriate headings.
Creep is another important characteristic of polymers. This is particularly true of polymers under continuous stress or strain in use, as is the case for pressurised containers. In the CSD bottle, the stress levels are high and are applied for an extended period of time. As shown by Bonnebat et al. , oriented PET is quite resistant to creep at low temperatures; however, at temperatures approaching
PET PACKAGING TECHNOLOGY
Figure 3.18 PET bottle: petaloid base. Potential areas of high stress that have partially uniaxial oriented structures are shown. These areas are likely to be prone to stress cracking in use.
Tg the creep compliance (elongation/tensile stress) increases sharply as the modulus falls and the molecules have more freedom to move. Creep is associated with movement of the molecules in the amorphous phase, and an increase in crystallisation level and/or orientation can reduce the level quite significantly. The mechanism is similar to stretching at very slow speeds, where there is a lower tendency to strain harden and therefore no resistance to chain movement. The polymer will show an increase in creep as the stress levels approach the yield point. 3.4 Properties The properties of PET and its copolymers are determined basically by their chemical composition and molecular structures. The combination of both the aromatic terephthaloyl entity and the flexible monoethylene glycol gives PET its unique characteristics, first recognised by Whinfield and Dickson. It is a strong, tough, flexible thermoplastic that readily crystallises and can be oriented into highly ordered structures. The oriented structures can also be heat set to give increased dimensional stability at high temperatures (above 80 C C). The polyesters have been used in a variety of applications because of their versatility and excellent physical properties. Their main characteristics are summarised as follows: •
General characteristics—cooled to give clear amorphous state, crystallisable, high melting temperature, melt processable, moderate softening point (amorphous Tg ca 80°C), worldwide food approval, excellent clarity, colourless, excellent strength, good creep resistance especially when crystallised, good barrier properties, and excellent chemical resistance. Characteristics of stretched products (oriented)—excellent strength and stiffness (high modulus), good creep resistance, excellent clarity.
PET MATERIALS AND APPLICATIONS
colourless, good water vapour barrier, adequate CC>2 barrier, low taint, outstanding impact resistance, excellent chemical resistance, worldwide food approval, and favourable environmental impact. 3.4.1 Molecular weight and intrinsic viscosity Molecular weight and molecular weight distribution are fundamental properties that determine end-use applications. The polymers are produced to various molecular weights and are available in amorphous, semi-crystalline or highly crystalline states. In the polyester industry, molecular weights have been characterised by IV measurements in dilute solutions. However, PET is not soluble in the common solvents and, over the years, resin manufacturers have used several different highly polar solvents to characterise the polymer. In more recent times, the production and use of highly crystalline solid-state materials, which are more difficult to dissolve, have exacerbated the situation. The solvents most commonly in use are the following: ortho-chlorophenol, hexafluoroisopropanol, 60:40 part mixture of phenol and tetrachloroethane, meta-cresol, trichloroacetic acid, trifluoroacetic acid, and 25:75 part mixture of ortho-chlorophenol and chloroform. The technique is based on the concept that the hydrodynamic volume of a linear polymer is related to its molecular size and, therefore, to particular solution viscosity properties. However, each solvent will have different solvation effects on the polymer molecules and this can have a significant influence on the apparent molecule size in that solvent. For these reasons, all the solvents measure slightly different IVs for identical molecular weight materials. The difference observed is greatest with higher molecular weight products and when hexafluoroisopropanol is used as the solvent. Within the industry, both manufacturers and end users have attempted to normalise the measurements by adjusting the Huggins constants. This works well over a short molecular weight range but is not to be recommended in practice. In general, the ASTMIV testing procedure using the solvent mixture of 60:40 phenol and tetrachloroethane is used as standard for the industry. In addition to the solution techniques, ICI has developed a modified melt flow index (MFI) testing procedure that measures the melt viscosity of the polymer at low shear rates and converts the values to IV. This instrument is manufactured and sold by Lloyds Instrument under the name Daventest melt viscometer. This test procedure is employed extensively to measure the IV of highly crystalline polymers that are used in injection moulding and sheet extrusion. For linear polymers, the IV measurement is correlated to molecular weight by the wellknown empirical expression first proposed by Mark [311 and Houwink : [ri] = K*Ma where, r) is the IV, M is the molecular weight, and K and a are constants.
PET PACKAGING TECHNOLOGY
The values of the constants, A" and a, are solvent dependent and, as expected, there are several different relationships established and published in the literature for PET. The value of the molecular weight can be expressed as Mn, Mw and Mv, which are the number average molecular weight, weight average molecular weight and the viscosity average molecular weight, respectively, depending on how the correlations are established. Although there is no preferred relationship, the ones most used by the author are as follows: (a)
= 1.7* l(T 4 *Mw 083
which was established by Ravens and Ward  using end group analysis. IV was measured in ortho-chlorophenol at 25°C. [T]]= 1.47* l(T 4 *A/vv 0768
which was established using gel permeation chromatography (GPC) data for molecular weights determined in ortho-chlorophenol, and holds for polydispersity (Pd) of less than 3. With Pd above 3, the polyester shows severe branching or abnormal molecular weight distributions, such as observed in high molecular weight SSP (IV > 1.5) products. (b)
[rj] = 4.68 * 1(T4 * Mn>, on the other hand, the permeability shows a dependence on the gas pressure and the more complex 'dual mode' sorption mechanism must be applied [84, 85]. The influence of crystallinity and orientation is to reduce the level of amorphous material available for diffusion; in both cases, the highly ordered structures in these regions obstruct the movement of the molecules and increase the average length of the paths the gas has to travel . In general, it is assumed that the crystalline domain is a complete barrier to the flow of gas, and as a first approximation the following relationship can be used:
where, Da is the diffusivity in the amorphous polymer and x( the degree of crystallinity. A similar effect is also seen on the solubility, with the highly ordered crystalline type structures reducing the solubility by a similar factor. The solubility function can be represented as follows: S = Sa(\-Xc) where, Sa is the solubility in the amorphous polymer.
PET PACKAGING TECHNOLOGY
The permeability in both crystalline and oriented structures is therefore represented by the following expression: Psc = Pad ~ Xcf
where, Psc and Pa are the permeability in the semi-crystalline/oriented and the amorphous samples, respectively. In addition to morphological contributions, the barrier properties are also influenced by the chemical structure, and to additives that can create more tortuosity in the flow path through the polymer matrix. Copolymer additives that can increase the cohesive energy between the molecule chains, such as the chloroterephthalic acids and hydroxyterephthalic acids, improve the gas barrier properties, whilst additives such as cyclohexane dimethanol give poorer barrier properties. Additives, such as isophthalic acid, that can influence the freedom of molecular movement around the aromatic paraphenylene entity, as well as molecules, such as naphthalene 2,6 dicarboxylic acid, that give increased chain rigidity, show positive benefits [87, 89] (also, L. Monnerie, Laboratoire de Physicochimie et Macromoleculaire associe au CNRS, ESPCI, Paris, personal communication). The incorporation of additives that can have an influence on the molecular chain mobility, such as plasticisers  and antiplasticisers  (also, L. Monnerie, personal communication), will also produce a positive or negative effect on the barrier properties depending on their influence on the chain molecules. In most cases, the addition of plasticising agents will have a negative effect, especially at high concentrations. Interestingly, it has been shown that the addition of small quantities of moisture will initially improve the barrier property, presumably through an increase in the cohesive bondage between the chain molecules. On the other hand, the addition of antiplasticisers, such as tetrachlorophthalic dimethyl ester, dimethyl naphthalate and dimethyl terephthalate, can have a very positive effect. In all cases, the additives are suppressing the (3 transition as measured by dynamic mechanical analysis. Interestingly, in dielectric relaxation measurements, the |3 transitions are not suppressed. Monnerie and co-workers  have used these two techniques in conjunction with solid state nuclear magnetic resonance (NMR) spectroscopy to resolve which chain motions are involved. They conclude that these additives hinder the rotational movement of the aromatic phenylene units, and therefore the overall freedom of the molecular chain. The results show that the effect is to reduce the diffusivity of the gas through the matrix. Yang and Jean  have shown a correlation between the free-volume hole size as measured by positron annihilation lifetime (PAL) technique, which supports the proposed theories on gas transport in various polyester matrixes. Other methods of improving the barrier properties include the addition of other high barrier resins, such as MXD.6. polyesteramides and modified
PET MATERIALS AND APPLICATIONS
Table 3.7 Gas barrier properties of PET and copolymers Gas barrier properties at 30° C
02 cc • mil/100 inch2 • 24 h • Atmos
CO2* cc • mil/100 inch2 • 24 h • Atmos
N2 cc • mil/100 inch2 • 24 h • Atmos
H2O g - mil/1 00 i n 2 24 h - Atmos
9 5 4
54 40 33
4 2.5 2
8 8.2 6.5 8
40 53 35 47.5
PET homo/low copolymer Amorphous Oriented Crystalline PET medium copolymer Amorphous !0%IPA 10% PETN 20% IPA 20% PETN PET high copolymer Amorphous PETG 50% IPA 50% PETN 100% IPA 100% PEN
19 4 6.3 2.3 3
109 16 39 6 18
Note: *Values for CO2 permeation are dependent on gas pressure: the values quoted are for low pressure (Ptending —* 0). Abbreviations: PET, polyethylene terephthalate; IPA, isophthalic acid; PETN, polyethylene terephthalate naphthalene 2,6 dicarboxylate copolymer; PETG, polyethylene terephthalate cyclohexane dimethanol copolymer; PEN, polyethylene naphthalene 2,6 dicarboxylate.
polyvinyl alcohol, the addition of platelets such as clay and liquid crystal polymer types, and the use of specific scavengers, especially for oxygen. A summary of the more relevant data is presented in Table 3.7. 3.10
Several different polyester resin types are available in the marketplace for use in the packaging industry. Each resin type will have been developed for specific injection moulding and/or extrusion applications, including their downstream use. The resin types are usually classed as homo, low, medium and high copolymer, and within this classification there will be other types, including branched polymers and blends.
PET PACKAGING TECHNOLOGY
The term homopolymer is a misnomer for this classification, since all the polymers will contain generated and possibly added diethylene glycol (DEG) at significant levels, and should therefore be classed as copolymers. Homopolymer is the major formulation used for fibre applications and, as such, was the original formulation used for packaging applications. Polymer types with molecular weight up to 20,000 and DEG levels up to 2.5% wt/wt are still being used to make standard film products. Various formulations containing generated DEG have worldwide food approval; however, polyester made with the addition of DEG is currently undergoing the FDA approval procedures. During the development of the ISBM process in the late 1970s, both film and fibre formulations were solid-state polymerised to an IV of around 0.75. and used successfully to produce two-piece CSD bottles. The containers had excellent tensile properties as well as a good barrier to COi, and were used successfully to bottle CSDs. Although this formulation has been superseded by copolymer formulations for use in the production of one-piece bottles, polymers are still being used successfully to make custom containers, such as peanut butter jars. In this application, clarity and the ability to hold container integrity during vacuum filling is critical. The resin is also used to make IM mould articles, including flat plate, as used for car number plates. However, for successful use in these applications, the molecular weight must be matched to the mould flow characteristics, as defined in the spiral mould test. Resin manufactures have developed an understanding of cleaner catalyst systems that do not cause stress crystallisation, and these are used to produce polymer grades that give good integrity and high clarity in the containers. Homopolymer is used successfully in sheet extrusion, which can be formed into thin-walled containers, display packaging and clear boxes. In the latter application, the resin has a clear advantage over competitive material in that it does not show stress whitening in the fold region. The sheet is usually co-extruded, with a copolymer layer on both surfaces containing surface modifying agents to reduce friction and improve de-nesting, as well as to improve adhesion and printing characteristics. Homopolymers are also the most favoured resin types for heat setting and use in hot-fill applications . In this case, the choice is governed by the thickness of the initial moulding. However, for mould thicknesses greater than about 4 mm, the use of copolymer is recommended to reduce the tendency for stress crystallisation to occur in the mouldings. High molecular weight (IV > 1) homopolymers, including some that are slightly branched, are used successfully in extrusion blow moulding (EBM) applications. The melt viscosity of these resins is highly sensitive to shear rate, and this enables the use of mild extrusion conditions (high shear) and high melt strength post-die (low shear). For successful use in this application area, it is essential to maintain the IV above 1.0 to reduce excessive sag in the parison prior to moulding.
PET MATERIALS AND APPLICATIONS
3.10.2 Lo w copolymers The low copolymer is the biggest market segment for PET polymer technology, and includes both the ISBM CSD and mineral water bottle applications. The move to low copolymer became essential when the market demanded onepiece bottles that have improved both bottle aesthetics and ease of recycling. To accommodate this shift in bottle design, a bottle base had to be created that could hold high pressures, in addition to keeping its shape and integrity under pressure for long periods. In this case, the standard champagne base could not hold the normal CSD bottle pressures without the use of excessive resin weight in its structure. The bottle base was redesigned into a petaloid shape that usually has five lobes and five crevasses. This base shape has areas of high stress that can give a catastrophic blow-out during manufacture, especially if the IV is low, and can lead to stress cracking during use [92-95]. To produce bottles with good base integrity, it is essential that the injection moulding and blow moulding operations be controlled to produce stress-free preforms and bottles. During this development, the machinery manufacturers produced bigger and faster machines to handle the increased demand. To satisfy these new requirements, the resin manufacturers moved to copolymers that are more forgiving in both the injection moulding and bottle blowing operations. The level of copolymer used is 1 -2.5% wt/wt, depending on the copolymer additive and overall formulation as designed specifically by the resin manufacturer to meet customers' requirements. The favoured copolymer additive is cyclohexane dimethanol or isophthalic acid. All resins for these applications are solid-state polymerised to standard IVs of 0.82 or 0.84. The higher IV resin is used to maintain molecular weight when the environmental conditions are unfavourable, such as the very warm and humid conditions that prevail in many countries during the summer months. During the reheat operation prior to blow moulding, the preforms are heated by quartz infrared heaters to temperatures around 10°C above Tg. It is crucial to have a uniform temperature profile across the wall to ensure that even stretching occurs during blowing in order to give maximum orientation and low creep properties in the wall [961; also that the resin flows uniformly to the base without causing high stress areas in the crevasses. To enhance the rate of heating and to achieve improved temperature uniformity, resin manufacturers, such as Dupont, now add specific near infrared absorbers to their resin formulation . These absorbers allow thicker wall preforms (greater than 4 mm) to be used more readily in bottle manufacture, as well as giving more freedom in bottle design. The preferred absorbers are fine metallic particles and/or carbon black, and these are used at the ppm level. All the resins used satisfy worldwide food regulations. Low acetaldehyde resins are required for the manufacture of bottles for sensitive foodstuffs, such as mineral water. These resins are produced under conditions that remove the vinyl end precursor during the solid-state operation, and may also contain additional
PET PACKAGING TECHNOLOGY
stabilisers. However, as described previously, to obtain low aldehyde levels in the bottle it is important that good drying and mild extrusion conditions are used. It is also important to give attention to the temperature profile and flow characteristics in the hot runner system, since they can both contribute to the variance seen in the acetaldehyde levels in the preforms. The use of a static mixer in the IM manifold can reduce the degree of variability. The addition of copolymer additive can have a significant influence on the stretching characteristics of the polyester polymer and blowing conditions should be adjusted accordingly. Typical data are presented in Figure 3.34. To produce thick-walled containers, as required for the refillable CSD bottles, much thicker walled preforms are needed. To meet these requirements, a resin with a higher copolymer level is used. For this application, the copolymer additive is used at a level of around 2.3-3.0% wt/wt, depending upon the additive being used and the overall manufacturers' formulation. Again the most favoured copolymer additives are CHDM and isophthalic acid. The resin formulation must also produce bottles that are robust to the subsequent caustic wash cycle at 60CC, and must survive at least 20 trips. To survive the wash cycle without loss in integrity and especially without enhancing any subsequent environmental stress cracking, it is critical that, in the manufacture of the preform and bottle, conditions are chosen to give an adequate wall thickness to the base and not to create excessively high stress areas. To minimise stress levels in the champagne base, it is important that its design ensures that all potentially sharp angles are
Sheet temperature 90°C
3 4 5 Copolymer level (moles%IPA)
Figure 3.34 Influence of copolymer level on stretch ratio. Abbreviation: IPA. isophthalic acid.
PET MATERIALS AND APPLICATION S
curved. To maintain integrity in use, it is important that the IV is retained at 0.80 and that the level of carboxyl ends is kept low. To achieve this, it is essential that drying conditions are set to achieve a moisture content below lOppm and that mild conditions are used on both the extruder and the manifold/hot-runner system. For applications that need higher wash temperatures (around 70CC), such as containers for mineral water, a higher level of heat setting is required or additives, such as naphthalene 2,6 dicarboxylic acid, are used to enhance the Tg. Standard grade and refillable bottle grade resins are both used for sheet extrusion, and are especially recommended for thick sheet applications. As is the case with IM, the thicker sheet is more prone to crystallise during casting and calendering. The use of copolymer reduces the rate of crystallisation during cooling and allows the production of thick sheet (up to 5 mm). Again, the IV should be maintained at 0.80 to give melt strength and adequate support during extrusion and casting. Copolymer resins can be used successfully in many IM applications. As has been described previously, it is crucial for these applications that polymer with the optimum melt viscosity for both melt flow and product integrity, including clarity and strength, is chosen. Copolymers made to various IVs from 0.5 upwards are available for use. The spiral test data in combination with mould dimension and injection route will give a good indication of suitability for use. 3.10.3 Medium copolymer's Several PET copolymers with additive levels in the range 4.5-13%wt/wt are available as speciality resins. These polymers have a much lower tendency to crystallise and are more difficult to solid-state polymerise, as well as drying from the amorphous state. However, they do have specific benefits over standard resins, depending on the copolymer additive used. Their main benefits are seen in the following areas: improving gas barrier properties, increasing or decreasing Tg as may be required for particular end use, retarding crystallisation, increasing shear sensitivity and producing high clarity thick-walled products. Both isophthalic acid and naphthalene 2,6 dicarboxylic acid copolymers show positive improvements in gas barrier property, while naphthalene 2,6 dicarboxylic acid copolymers also show an increase in Tg. On the other hand, the use of diethylene glycol, polyethylene glycols and aliphatic diacids, such as adipic acid, will give a lower Tg and poorer gas barrier properties. While most of the copolymer additives will retard crystallisation, the most effective are CHDM and isophthalic acid. Again, isophthalic acid and CHDM are very effective in increasing the shear sensitivity, especially at low IV, and are used as polymer modifiers for IM applications. Various copolymer types are available for this use and, as has been mentioned previously, the polymers can be matched to end-use requirements through knowledge of the spiral test data, IM conditions, including mould dimension and injection route, and end-use characteristics. High clarity
PET PACKAGING TECHNOLOGY
polymers containing very low catalyst residues are also available to produce thick-walled containers. These same copolymers can be used in extrusion to produce high clarity sheet. The situation as regards food contact is not as clear-cut as that for a low level copolymer. In this case, it is recommended that each formulation be reviewed with relevant expertise to obtain opinion and guidance on the way forward. 3.10.4
The most well-known high copolymers are based on CHDM, and are referred to as PETG. These are made by Eastman and are used in both IM and extrusion applications. They are amorphous copolyesters, containing about 35% wt/wt of copolymer component. However, because of their amorphous nature, they need to be carefully dried at low temperatures (around 90C C) for long periods (around 24 h), under vacuum or in the presence of dehumidified gas. They are made to a range of molecular weights and are renowned for high clarity. Copolyesters based on other additives, such as naphthalene 2,6 dicarboxylic acid, isophthalic acid and cyclohexane dicarboxylic acid, are available for more specific end uses, including improved gas barrier, increased Tg and high rigidity. The high copolyester grades are used as the surface layer in co-extrusion with both homopolymer and low copolymer. to give improved melt-adhesion and printing. 3.11
High crystallinity is required in polyester products to give dimensional stability and rigidity at high temperatures. To obtain satisfactory rates of crystallisation in the mould or after forming, a suitable nucleating agent must be incorporated into the polymer. The type of additive and level must be matched to the downstream process requirements. In both extrusion and injection moulding processes, it is important that the nucleant does not cause problems during the initial melt cooling process. In both the injection and casting processes, this can affect the product integrity, with localised shear crystallisation occurring in the mould and the formation of poor quality, partially crystalline sheet during casting. As a consequence, poor impact performance is obtained as well as misshaped articles. To obtain adequate crystallinity and good product integrity, it is therefore essential to match the level of nucleant, and so the crystallisation rate, to the needs of the downstream process. The type of nucleant will depend upon when the crystallisation should occur, such as on cooling as in the injection moulding process, or on reheating as in the forming process. For the former, the type of nucleant is usually of a paniculate kind, such as talc, or a cation, such as the sodium ion . In both cases, a critical mass of additive is required to produce sufficient nuclei to give a beneficial effect on the rate of crystallisation, as well as efficiency in the
PET MATERIALS AND APPLICATIONS
dispersion of the participate to its optimum size (around 1 um). For injection moulding applications, the optimum level is found to be around SOOpprn of sodium and around 0.2% of talc. However, these levels will vary depending on the polymer formulation and also on the level of branching that is present. To achieve the required level of crystallisation, the moulding is held for a finite time (about 20s), in a hot mould at around 140°C. Care must be taken during cooling post-mould, to ensure that no stress areas are frozen in, which could lead to the article distorting in use. On the other hand, for extrusion into sheet form for thermoforming, it is best to use nucleating agents that are less effective in the cooling mode but very effective on heating. This type of nucleation is best achieved using a stress-induced mechanism, as is obtained when low melting point crystalline polymers, such as polyethylene and polypropylene, are finely dispersed at a level of 1-3% wt/wt into the polymer matrix. On reheating the sheet, the crystalline polymer will remelt, inducing highly localised finite stress areas, which induces crystallisation in the polyester. This is a very effective method for inducing crystallisation into thermoformed polyester trays, which are used for microwave applications. In the thermoforming process, the sheet is heated in an infrared oven to a temperature where nucleation and crystallisation are imminent, and formed as crystallisation is occurring. Again, the formed article is held in the mould for a finite time to develop maximum crystallinity (around 10 s). Care must be taken during cooling to ensure that all the moulds are cooled evenly and without build-up of localised stress areas that could affect the integrity in use. The molecular weight of the polymer has a strong influence on the rate of crystallisation, and the level of additives must be optimised for each IV. 3.12
Polymer blends can give beneficial effects that are not otherwise readily achieved. The addition of low melting point polymers enhances crystallisation from the glassy state; however, it is also observed that this creates voids and some localised orientation in the polyester, which can enhance its impact properties. The use of an elastic/rubbery polymer type, such as modified acrylic resins, as additive within the blend, at levels greater than 5% wt/wt, causes significant improvement in impact performance. Blends made with superior barrier polymers, such as poly vinyl alcohol copolymers and MXD.6, can give enhanced gas barrier properties. Some of these benefits are discussed in detail in Chapter 4, 3.13
The properties of PET that have been described have established it as an ideal polymer for use in packaging applications. It is already established as the
PET PACKAGING TECHNOLOGY
preferred polymer for many applications, such as pressurised containers for CSD and mixer drinks, custom containers for many food and non-food applications, high quality injection-moulded containers for outlets such as cosmetic and perfumery, and sheet extrusion for use in both clear and crystalline containers, as well as in clear display packaging. PET will continue to build a market share in these areas at the expense of existing materials. It also has strength in many thin film applications, which are described in detail in Chapter 5. New and innovative developments that are currently being worked on across the whole manufacturing and processing chain, such as improved barrier and cast foam products, will allow newer end-use applications to be identified. 3.14
The interest in polyester polymers will continue across all current market sectors for the foreseeable future. The major growth and opportunities will be in the packaging sector, where it is now recognised as the preferred material for several food and non-food applications. The use of plastic materials such as PET is now acceptable to the younger generation, and it is envisaged that attempts will be made to replace more of the conventional packaging materials, such as steel, aluminium and glass, over the next 10 years. To achieve this potential growth, intrinsic properties, such as gas barrier and hot fill, must be improved. Work within the industry is focused towards achieving these goals. There is much interest in bottling beer in plastic containers, such as PET bottles. Several different routes to achieve high barrier are under investigation. Plastic bottles and containers that can retain their integrity at high temperatures are also in demand for use in hot-fill and oven pasteurisation applications. Interest in non-packaging applications, such as engineering plastics, foam and cast sheet, will allow further developments to occur, such as in blends, nucleation, filled grades, impact modified, high clarity and UV stability, to meet the end-use requirements. These developments will increase the opportunities for use in packaging applications. The consumer will expect all plastic material to be more environmentally friendly both during manufacture and in use. Although PET is acknowledged to be recyclable, a very high proportion is still not reused. This is discussed in more detail in Chapter 11. New, cleaner manufacturing processes are being developed and used, making the whole process more cost effective and more acceptable to the environment. 3.15
The versatility of PET makes it a highly acceptable packaging material worldwide. The presence of polyester fibre plants and technology across all continents has allowed the material to be produced and used in newer plastic end-use
PET MATERIALS AND APPLICATIONS
applications without significant initial investment. Growth in the US and Western Europe will gradually slow down as the CSD market sector reaches maturity. However, significant growth will continue in the Eastern Bloc Countries, China and South America. Newer markets, such as the beer market, will open further opportunities worldwide and especially in the US and Western Europe.
References 1. 2. 3. 4. 5. 6. 7. 8. 9. 10. 11. 12. 13. 14. 15. 16.
17. 18. 19. 20. 21. 22. 23. 24. 25. 26. 27. 28. 29. 30. 31. 32.
Whinfield. R. and Dickson, J.T. UK Patent 578,079. Whinfield, R. (1946) Nature. Ludewig, H. (1971) Polyester Fibres Chemistry and Technology, Wiley Interscience, New York. Polyester: 50 Years Achievement. The Textile Institute, Manchester, M3 SDR, UK. Wyeth, N.C. and Roseveare, R.N., N.C. UK Patent 1341845-48. Monsanto Corp., USA. UK Patent 1,226,154, US Patent 3,551,386. Shuya Chang, Ming-Fu Sheu and Shu-May Chen (1983) /. Appl. Polymer Sci., 28, 3289. Wu Rongrui, Huang Guanbao, Zhang Dashu and Li Yanli. Proceedings of the 2nd International Conference on Man-Made Fibres, Beijing, China, 26 November, 1987. Jabarin, S. A. and Lofgren, E.A. (1986) / Appl. Polymer Sci., 32, 5315. Dupont Polyester Presentation. Polyester '99 World Congress, Zurich, Switzerland, December 1999. Technical Presentations. Polyester '97 World Congress, Zurich, Switzerland, November 1997. Technical Literature, Zimmer AG, Germany; Inventa AG, Germany. Technical Literature, Dupont Polyester, Wilmington, Del., USA. Technical Literature, Sinco Eng. SpA, Italy; Buhler Ag, Switzerland; Zimmer AG, Germany; Hosokawa Bepex Corp., USA. Herman, K., Gerngross, O. and Abitz, W. (1930) Z. physik. Chem., BIO, 371. van Krevelan, D.W. (1976) Properties of Polymers and the Estimation and Correlation with Chemical Structures. 1 st Edition, Elsevier Scientific Publishing, Oxford, New York and Amsterdam, p. i6. Hearle, J.W.S. and Greer, R.E.J. (1970) Text. Progress, 2, 4. Keller, A. (1957) Phil. Mag., 8 (2), 1171. Schlesinger, W. and Leeper, H.M. (1953) J. Polymer Sci., 11, 203. Houseman, R. (1950) Physik, 128 (1), 465. Jones, K.M. (1992) 'Plastic South Africa' Presentation given to the Plastic Institute, South Africa, 18. Bonnebat, C., Roullet, G. and de Vries, A.J. (1979) SPE 37th Annual Conference, New Orleans, 273. Jabarin, S.A. (1984) Polymer Eng. Sci., 24, 376. Thompson, A.B. and Marshall, I. (1954) J. Appl. Chem., 4, 145. Heffelfinger, C.J. and Schmidt, P.O. (1965) J. Appl, Polymer Sci., 9, 2661. Bonnebat, C., Beautemps, J. and de Vries, A.J. (1977)./. Polymer Sci., 58, 109. Jabarin, S.A. and Lofgren, E.A. (1986) Polymer Eng. Sci, 26, 620. Le Bournelle, G., Monnerie, L. and Jarry, J.P. (1986) Polymer, 27, 856. Fuller, W., Mahendrasingen, A., Martin, C., et al. (2000) Polymer, 40 (20), 5553. See also Polymer, 41 (3), 1217; Polymer, 41 (21), 7793 and Polymer, 41 (21), 7803. Leiger, P.P. (1985) Plastic Eng., 47. Mark, H. 'Derfesl Korpef (ed. R. Sanger), Hirzel, Leipzig, Germany. Houwink, R. (1940) J. prakt. Chem.. 15, 157.
PET PACKAGING TECHNOLOGY
33. Ravens, D.A.S. and Ward, I.M. (1961) Trans. Fara. Soc.. 57. 150. 34. Moore, Jr., L.D. (1960) Cleveland ACS, Meeting 4, Vol. 1. 35. Jabarin, S.A. PET Technology: Properties and Processing. Polymer Institute. University of Toledo. Toledo, 111., USA, Chapter 4, p. 16. 36. Jabarin, S.A. and Balduff, D.C. (1982) J. Liq. Chromatogr.. 5. 1825. 37. Jabarin, S.A. PET Technology: Properties and Processing. Polymer Institute. University of Toledo. 111., USA, Chapter 4, p. 19. 38. Cooper, D.R. and Semlyen, J.A. (1975) Polymer. 14, 185. 39. Pebbles, J.R.. Huffman, M.W. and Ableh, C.T. (1969) J. Polymer Sci.. 7. 479. 40. Goodman, I. and Nesbitt, B.F. (1960) J. Polymer Sci.. 48. 423. 41. Mifume, A., Ishida, S., Kobayashi, A. and Sakajiri. S. (1962) 7. Chem. Soc. Japan (Ind. Chem. Sec. >. 65. 992. 42. Groenickx, G.. Reynaers, H.. Berghams. H. and Smets, G. (1980) 7. Polymer Sci. Polymer Physics Ed.. IS, 1311. 43. Groenickx, G. and Reynaers, H. (1980) 7. Polymer Sci. Polymer Physics Ed.. 18. 1325. 44. Alfonso. G.O., Pedemonte, E. and Ponzetti. L. (1979) Polymer. 20. 104. 45. Chixing Zhou and Clough, S.B. (1988) Polymer Eng. Sci.. 28. 65. 46. Sweet. G.E. and Bell, J.P. (1972) 7. Polymer Sci.. (Pt A-2) 10, 1273. 47. Ward. I.M., Monnerie, L. and Maxwell A.S. (1998) Polymer. 39 (26). 6851. 48. Davies, G.R. and Ward, I.M. (1972) 7. Polymer Sci., 10. 1153. 49. Lawton. E.L. (1985) Polymer Eng. Sci.. 25. 348. 50. Lin, C.C. (1983) Polymer Eng. Sci., 23. 113. 51. Pearson, G.H. and Garfield, L.J. (1978) Polymer Eng. Sci.. 18. 583. 52. Axtell. F.H. (1987) A Study of the Flow Properties and Processability of Thermoplastic Polyester. Thesis. Loughborough University, Loughborough. UK. 53. White. J.L. and Yamane. H. (1985) Pure Appl. Chem.. 57. 1441. 54. Ferry. J.D. (1942) 7. Am. Chem. Soc.. 64. 1330. 55. Lee, Y. Wang. T. and Chang, S. (1983) 7. Chinese Inst. Chem. Eng.. 14. 347. 56. van Krevelan. D.W. (1976) Properties of Polymers and the Estimation and Correlation with Chemical Structures. 1 st Edition. Elsevier Scientific Publishing. Oxford. New York and Amsterdam, p. 491. 57. Holmes. D.B.. Esselink, B.P. and Beek. W.S. (1966) Processing polymers to products. Proc. Intern. Congress Amsterdam, 't Raedthuys. Utrecht. 1967, p. 167. 58. Yasuda. H. and Stannett. Y. (1962) 7. Polymer Sci.. 57. 907. 59. Mclntyre. J.E. (1985) Fibre Chemistry, (eds. M. Lewin and M. Pearce). Chapter 1. Marcell Dekker. New York. 60. McMahon. W. (1959) 7. Chem. Eng. Data., 4. 57. 61. PETG Technical Literature, Eastman Chemicals Corp.. Kingsport. Tn. USA. 62. Goodings. E.P. (1961) Soc. Chem. Ind.. (London) Monograph. 13. 211. 63. Buxbaum. L.H. (1968) Angew. Chem. Int. Ed., 7. 182. 64. Allan, R.J.P.. lengar, H.V. and Ritchie, P.O. (1957)7. Chem. Soc.. (London) p. 2107. 65. Marshall. I. and Todd. A. (1953) Trans. Fara. Soc.. 49. 67. 66. Villain. F, Condane. J. and Vert, M. (1994) Polymer Deg. Stability. 43. 431. 67. Jabarin. S.A. and Lofgren. E.A. (1984) Polymer Eng. Sci.. 24. 1056. 68. Zimmerman. H. and Kim. NT. (1980) Polymer Eng. Sci.. 20. 680. 69. Aalbers. J.G.M. and van Houwelingen. G.D.B. (1983) Fresinus Z. Anal. Chem.. 314. 472. 70. Khemani. K.C. (2000) Polym. Degrad. Stab.. 67 (1). 91. 71. Yoda, K.. Tsuboi. A.. Wada. N.T. and Yamadera. R. (1970) J. App. Sci.. 14. 2357. 72. Nealy. D.L. and Adams, L.J. (1971) 7. Polymer Sci.. 9. 2063. 73. Zimmerman. H. and Becker, D. (1973) Faserforshung u. Textii. 24. 479. 74. Allen. N.S.. Edee. M.. Mohammadian. M. and Jones. K.M. (1991) Eur. Pol\. J.. 27. 1373.
PET MATERIALS AND APPLICATIONS
75. Allen, N.S., Edge, M., Mohammadian, M. and Jones, K.M. (1991) Textile Res. J., 61, 690. 76. Allen, N.S., Edge, M., Mohammadian, M. and Jones, K.M. (1994) Poly. Deg. Stability, 43, 229. 77. Rosato, Donald V. and Rosato, Dominick V. (eds.). Blow Moulding Handbook, J. Wiley and Sons. London, UK, 1989. 78. Technical Literature, Sidel Corp., Le Havre, France. 79. Kim, S.L. Effect of Equilibrium Time on the Properties of Reheat Blown 21 PET Bottles, SPE ANTEC Conference, Boston, USA, 1983, pp. 804-908. Technical Literature 'Laser++', Dupont Polyester, Wilton, Middlesbrough, UK. van Krevelan, D.W. (1976) Properties of Polymers and the Estimation and Correlation with Chemical Structures. \ st Edition, Elsevier Scientific Publishing, Oxford, New York and Amsterdam, p. 403. 82. Michaels, A.S., Vieth, W.R. and Barrie, J.A. (1963) J. Appl. Physics, 34, 13. 83. Vieth, W.R., Alcalay, W.R. and Frabetti, A.J. (1964) /. Appl. Polymer Sci., 8, 2125 84. Koros, W.J. and Paul, D.R. (1978) J. Polymer Sci., 16, 2171. 85. Brolly, J.B., Bower, D.I. and Ward, I.M. (1996) J. Polymer Sci., 34, 769. 86. Perkins, W. (1988) Polymer Bull., 19, 397. 87. Light, R.R. and Seymour, R.W. (1982) Polymer Eng. Sci., 22, 857. 88. Weinhold, S. Technical Presentation, Polyester '97 World Congress, Zurich, Switzerland. November 1997, Figure 1, p. 3. 89. Monnerie, L., Maxwell, A.S., Laupretre, F. and Ward, I.M. (1998) Polymer, 39 (26), 6835. 90. Yang, H.E. and Jean, Y.C. (1998) Medical Plastic and Biornaterials, January. 91. Maruhashi, Y. and Asda, T. (1992) Polymer Eng. Sci., 32, 481. 92. Tekkanat, B., McKinney, B.L. and Behin, D. (1992) Polymer Eng. Sci., 32, 393. 93. Jabarin, S.A., Lofgren, E.A. and Mukherjie, S. (1994) ANTEC conference, 3271. 94. Jabarin, S.A. and Lofgren, E.A. (1992) Polymer Eng. Sci., 32, 146. 95. Moskala, E.J. (1996) Bev-Pak Americas '96 Conference, Florida, USA, 8-1. 96. Gray, F.P. (1996) PET Oriented Containers; Creep Behaviour, presented at Bev-Pak Americas '96. Florida, USA. 97. Aharoni, S.M., Sharma, R.K., Szobota, J.S. and Vernick, D.A. (1983) J. Appl. Polymer Sci., 28, 2177.
Barrier materials and technology David W. Brooks
PET is now a commodity polymer for packaging markets—in particular for beverages and foods. It has competed successfully with traditional materials like glass and metal for containers and bottles, and is now the major material, in terms of volume, for the manufacture of bottles. PET has good gas barrier properties but, when packaging oxygen-sensitive materials and highly carbonated products, PET does not have a good enough barrier to oxygen, carbon dioxide and moisture. This is the case for products such as beers, baby foods and wine, when packed in small containers and when a long shelf-life is required. The present chapter briefly describes the different types of polyester, in particular polyethylene naphthalate (PEN), which is a high barrier polyester, and amorphous polyesters, which are clear like glass in thick mouldings, making them ideal for high value packaging. Polymers which have better barrier properties than PET have been utilised in multilayer structures—using co-extrusion and co-injection technologies—to enhance the barrier properties of PET without detracting from its other beneficial properties. Barrier improvements can also be achieved with coatings, both internally and externally applied to bottles and containers. Now 'active' systems, such as oxygen scavengers, are being explored and, more recently, nanocomposites are being developed for use in packaging. Liquid crystal polymers (LCPs) have the highest barrier properties currently available and will be further developed for use in packaging. Whether plastics will somehow eventually merge with glass, to form plastic glass, only time will tell. 4.2
PET bottles produced by the stretch blow moulding process are particularly suitable for packaging products that require high clarity and gloss, a barrier against gases, resistance to creep under pressure, and toughness and impact strength. PET is a condensation polymer polymerised from two monomers, pure terephthalic acid (PTA) and a di-alcohol or diol, ethylene glycol (EG). Replacing PTA or EG with other monomers produces different polyesters, for example, isophthalic acid (IPA), which at low additions can improve the barrier properties of PET. Another widely used monomer is 1.4 cyclohexane dimethanol
BARRIER MATERIALS AND TECHNOLOGY
(CHDM), supplied by Eastman Chemicals, which substitutes for EG in PET to produce polyethylene terephthalate glycol modified polyester (PETG) and other amorphous copolyesters. Another option is to replace EG with diethylene glycol (DEG), which doubles the EG content. It is also possible to include more than one acid or diol in the structure, to produce various copolyesters. PET copolymers used for stretch blown bottles may contain small amounts of either 1PA or CHDM, which help to broaden the processing window, increase line speeds, slows crystallisation speed and reduce stress in the bottle. Extrusion blow mouldable PET was developed some time ago but did not progress commercially because of cost and processing difficulties. This PET has a much higher molecular weight (intrinsic viscosity (IV) about 1.05) than standard, bottle-grade PET (IV about 0.8), and this increases the melt strength to help control the formation and stability of the extruded parison. In the 1980s, Eastman Chemicals and Goodyear Tyre Co. developed a high barrier polyester called polyethylene naphthalate. PEN has a better gas barrier (five times better than PET), better UV barrier, improved temperature stability and greater stiffness than PET, but is more expensive to produce, so that it costs more than PET. PEN is being targeted at high-performance packaging but so far with limited penetration. The high price and limited availability of the monomers have restricted PEN's introduction into high volume commercial packaging applications. 4.2.1 PEN
PEN is polymerised using 2,6-dimethyl naphthalenedicarboxylate (NDC) with EG, and is being developed or studied by most polyester producers. It is a semicrystalline polymer similar to PET, but with a double ring structure, which makes it more rigid and improves its barrier and mechanical properties. It has a high molecular weight and can be converted by injection, extrusion and biaxially stretch blow moulded into containers and bottles via injection moulded preforms. PEN is a higher melting polymer than PET, otherwise the processability is similar. The properties of PEN make it an ideal material for high-performance packaging, with the potential to replace glass in some market segments. PEN has a gas barrier (oxygen, CC>2) about five times better than PET, moisture barrier about four times better than PET, stiffness 50% greater than PET, and a higher glass transition temperature (Tg) at 121°C compared to 75°C for PET (see Table 4.1). Following initial objections to the use of PEN for bottles that could end up in the recycle stream mixed with PET, technology was developed to separate the two polyesters. As a result of this PEN homopolymer, PEN/PET copolymers and blends are now accepted by the Food and Drug Administration (FDA) for food contact applications. The monomers used to produce PEN are on the European
PET PACKAGING TECHNOLOGY Table 4.1 Properties of polyethylene terephthalate (PET) and polyethylene naphthalate (PEN)
Tensile modulus (MPa) Tensile strength (MPa) Melting point (TM)( C) Glass transition (Tg) ( C) Thermal shrinkage ( 1 50 C.7c ) Oxygen permeability CO2 permeability Moisture permeability
1200 45 257 75 1.5 1.5 9 1.2
1800 60 270 121 0.9 0.3 1.7 0.28
Oxygen and CO? permeability: (cm 3 • mm m ' • d a y " 1 - a i m ' ) 23 C/50-chlorophenol, and is attacked by
PET PACKAGING TECHNOLOGY
Table 5.3 Thermal properties of 23 ^.m Mylar® film Property
ASTM D34 18-82
Shrinkage (150 C. 30min) MD TD
Coefficient of thermal expansion at 30-50 C Heat scalability Specific heat (25 C) Thermal conductivity
1.7 x 10~5 Cm/cm/ C
None unless coated or treated 1.32J/g/ C 0.15 W/m K
Abbreviations: MD. machine direction: TD. transverse direction.
Table 5.4 Mechanical properties of 23 pim Mylar® film Property
Tensile strength (MD)at25 C Tensile modulus (MD)at25 C Elongation (MD)at25 C Stress to produce 5c/i elongation (MD) at 25 C Density at 25 C Folding endurance 1 kg loading, at 25 C Tear strength Initial (Graves) at 25 C Propagating (Elmendorf) at 25 C Coefficient of friction (kinetic) at 25 C Refractive index ( A B 8 E a t 2 5 C) Coefficient of hygroscopic expansion
29 000 psi 200 MPa 565 500 psi 3 900 MPa 1 309J-
ASTM D882-80 ASTM D882-80 ASTM D882-80
15 200 psi 105 MPa 1 395 g/cm3 100 000 cycles
ASTM D 1004-66
ASTMD 1505-66 ASTM D2 176-63
1.0 x 10"5 mm/mm 7r RH
Abbreviations: MD. machine direction; RH. relative humiditv.
35% nitric acid, 10% ammonium hydroxide and «-propylamine. PET film also has very low moisture permeability and overall resistance to staining by various chemicals and food products. Gas and vapour barrier properties can be significantly improved by coating with a barrier coating, such as polyvinylidene chloride, or by vacuum metallisation.
PET FILM AND SHEET Table 5.5 Chemical properties of 23 |im Mylar® film Property
Moisture absorption (immersion for 24h at 23 C)
Less than 0.8%
16cc/(100 in 2 ) (24h) fatm)/(mil) 6cc/(m 2 ) (24h) (atm)/(mm)
Hydrogen at 25 C
]00cc/(100 in 2 ) (24 h) (atm)/(mil) 39cc/(m 2 ) (24h) (atm)/(mm)
Nitrogen at 25 C
1 cc/(100 in 2 ) (24h) (atm)/(mil) 0.4cc/(m 2 ) (24 h) (atm)/(mm)
Oxygen at 25 C
6cc/(100 in 2 ) (24h) (atm)/(mil) 2.3 cc/(m 2 ) (24 h) (atm)/(mm)
2.22 g/( 100 in 2 ) (24 h)/ (mil) 0.87g/(m 2 )(24h)/(mm)
Mod. ASTM E96-80
Benzene at 25 "C
0.36g/(100in 2 )(24h)/(mil) 0.14g/(m 2 )(24h)/(mm)
Mod. ASTM E96-80
Carbon tetrachloride at 40" C
0.08g/(lOOin 2 )(24h)/(mil) 0.03g/(m 2 )(24h)/(mm)
Mod. ASTM E96-80
Ethyl acetate at 40" C
0.08g/(100in 2 )(24h)/(mil) 0.03g/(m 2 )(24h)/(mm)
Mod. ASTM E96-80
Hexane at 40 C
0.12g/(IOOin 2 )(24h)/(mil) 0.05g/(nr)(24h)/(mm)
Mod. ASTM E96-80
Water at 37. 8 C
1.80g/(lOOin 2 )(24h)/(mil) 0.70g/(rrr)(24h)/(nim)
Mod. ASTM E96-80
Permeability to gases Carbon dioxide at 25' C
Permeability to vapours* Acetone at 40 : C
*Vapour permeabilities at the partial pressure of the vapour at the temperature of the test.
Table 5.6 Chemical resistance properties of 23 jxm Mylar® film
Property Chemical resistance to: Acetic acid, glacial* Hydrochloric acid (10%)* Sodium hydroxide (2%)* Ammonium hydroxide (10%)* Trichloroethylene* Hydrocarbon oil (immersion for 500 hat 100°C) Ethanol* C
* Immersion for 31 days at 23 C.
Tensile strength % retained
Elongation % retained
Tear strength % retained
100 100 100 0 100 92
100 100 100 0 100 88
100 100 70 0 100 87
PET PACKAGING TECHNOLOGY Table 5.7 Electrical properties of 23 M-rn Mylar® film Property
Dielectric strength 25 C. 50 Hz, 50 mm electrode Dielectric constant 25 C, 1 kHz Dissipation factor 25 C. 1 kHz Volume resistivity 25 C Surface resistivity 25 C. 30% relative humidity Corona resistance 1000 volts
1018 ohm cm 1016 ohm square
ASTM D257-78 ASTM D257-78
PET film has excellent electrical insulating properties, as shown in Table 5.7. Because of its excellent thermal, insulating and moisture resistant properties, PET film is used in a wide variety of electrical applications. However, for many specialty applications further modification of either the surface or bulk properties are required, as illustrated in the sections below. 5.4.2 Coating PET is a fairly inert polymer and for many applications the surface of the film is altered by coating or adhesive lamination to other materials, for example, film for packaging will be lacquered to accept inks or adhesives, and film for photographic applications will be primed to accept photosensitive overcoats. An untreated film would require treatment with aggressive chemicals to modify the surface sufficiently to allow such coatings to adhere to it. Coatings are also applied to achieve other surface effects, such as antistatic properties, barrier (to water, oxygen, carbon dioxide, flavour), release and frictional characteristics. The chemistry and colloid science of these formulations is vast and complex and outside the scope of the present article. However, it can be said that coatings often contain a 'primary effect' material, key to obtaining a given effect (more than one effect may be required). For example, in the case of an adhesionpromoting coating, this material is often a copolymer, such as an acrylic, vinyl, polyester or polyurethane. In the simplest case, all the other components of this coating are essentially there to facilitate the uniform application (and subsequent adherence) of the effect polymer to the film. Consequently, the wetting, flow, drying, film formation and cure kinetics of the coating during the surface treatment process are all important factors to be considered when formulating the coating material. A typical aqueous formulation may contain a solution
PET FILM AND SHEET
or dispersion of an effect polymer, together with a wetting agent (surfactant or co-solvent), a cross-linking agent and catalyst, pH regulator, a film former (coalescent, plasticiser), defoamer, antiblock, etc. Clearly, a given ingredient may have an influence in more than one of these areas. Wetting of the PET surface (~43 dynes/cm) may be facilitated by flame or corona discharge treatment prior to coating. The cross-linker is a species that is simultaneously reactive towards the PET surface (hydroxyl and carboxyl end groups) and the effect polymer; multifunctional epoxides, aziridines, isocyanates and melamine formaldehyde resins are commonly used. PET film is commonly coated either 'in-line' or 'off-line'. In-line coating usually involves aqueous-based materials and is carried out between the forward draw and before entering the tenter, while off-line coating involves unwinding and priming the surface of preformed film reels with aqueous or solvent-based coatings. In both cases, the coating may be applied to one or both sides, and some products have different coatings applied to either side of the film. Coatings are mostly applied by offset gravure or by direct gravure coating. Coat continuity and uniformity are important to ensure that the required properties are obtained. Uniform dry coating thicknesses as low as ~10nm can be routinely achieved in-line, while off-line coatings can be 10-100 times thicker. Too much coating on the film is to be avoided in the in-line process, since the water has to be dried off in the tenter preheat section and the film will only heat up to the required temperature for the SWD when it is completely dry. Excess wet coat thickness may cause the film to be at too low a temperature when drawing starts, resulting in poor profile and possibly breakage of the film web. Applying excessive amounts of coating can also result in unacceptable film optical properties, such as coat non-uniformity, haze and yellowness. Furthermore, because the tenter process often involves recycling some film, and some of this may be coated, thick coatings may adversely effect the colour, clarity and extrusion characteristics of the recycled polymer melt. Off-line coating does not have this restriction on the chemistry and thickness of the coating; the off-line process is better suited to coating high Tg coating materials (as the coating is not drawn), and those requiring longer cure schedules. 5.4.3 Co-extrusion Co-extrusion is used to produce a film with two or more different polymer layers, so that one or both surfaces of the film have different properties to the 'core' polymer. In addition, co-extrusion allows manufacture of products with layers thinner than can be made and handled individually. Co-extrusion provides a means of flexibly configuring a wide range of film laminate structures which cost-effectively meet product requirements. An example of a co-extruded film is Mylar® 850, in the production of which a lower melting copolymer containing isophthalic acid is extruded onto a standard base film to give a film that can heat
PET PACKAGING TECHNOLOGY
seal to itself and heat seal to thermoformed APET/CPET trays and APET-coated board. It will also heat seal to various other substrates, including polyvinylidine chloride (PVDC), PVC, paper and aluminium foil, but it does not heat seal to polyolefins. The co-extruded layer is about 15% of the total structure and by tailoring the copolymer chemistry a wide heat seal range, from 140-220 C. with outstanding hot tack properties can be obtained. The copolymer, if extruded as a film itself, would not have sufficient strength and the base PET homopolymer provides the mechanical properties required. The scalable surface of the film also acts as an excellent prime for water-based lattices. This film can be exploited in various ways, for example the film can be PVDC coated from an aqueous dispersion by convenors to produce a high barrier laminating film. Further examples of co-extrusion application include the use of reclaim polymer in the centre of films, so that more expensive virgin polymer can be used sparingly to provide surface properties. The basic co-extrusion process consists of the generation of two or more melt streams and their confluence in the melt phase. The number of separate extrusion systems is determined by the number of polymer types, typically two but occasionally three and exceptionally up to ten. Each polymer type to be incorporated in the structure is separately melted, pressurised and (optionally) filtered in parallel extrusion systems before flowing into the co-extrusion hardware. The optimum method of bringing the separate melts together depends primarily on their respective flow behaviours. The melt layers must remain distinct but well bonded in the process, from the point(s) of confluence through to solidification. There are basically two hardware configurations in use for common polymers— the multimanifold die and the injector block. (Combinations of the two are also possible for complex structures.) The multimanifold die is used when the viscosities of the melts are dissimilar, or low, or where there are many streams to combine. The streams are brought together at the die, just prior to solidification, thus allowing virtually no time for the weaker melts to be distorted in the short region of laminar flow. Coextrusion profile (the relative thickness of layers across the web) is a key process requirement in many products. However, multimanifold dies are generally expensive, complex and can be difficult to incorporate in thermoviscous profile control systems. Polypropylene film processes typically utilise multimanifold dies because of the tendency of that polymer to encapsulate (that is distort the shape of) the secondary polymer in the laminar flow regions. The second option, used extensively with PET, is injector block technology. This is restricted to two or three layer applications. Injector block systems consist, in basic form, of a main melt channel with one or two side entries through which secondary melts flow. The injected melt(s) then flow side-byside with the main polymer, in the same pipe, towards the die. The mechanism is most effective when the viscosities of the melts are similar. The greater the viscosity difference the more pronounced will be the distortion of relative
PET FILM AND SHEET
profile. For many packaging applications, however, profile distortions up to 10% are acceptable, and therefore the process has a degree of robustness towards viscosity variations. The basic injector technology can be enhanced by the addition of profiling cams and fins at the point of sidestream entry, which contour the flows in a way that leads to a more uniform profile. Adjustable cams can be included, which provide for in situ optimisation. Cam design is particularly important for uniform profile. Typically, cams take the form of a rectangular slot. A particular requirement for tenter film processes is often to avoid having sticky film under tenter clips, and hence to provide web edges clear of secondary polymer. Cams can be designed which restrict the application of secondary polymer to a centre width of the film web. However, the maintenance of uniform profile in such designs is very difficult, and companies that have developed good designs are often reluctant to share them. It is generally true to say that the wider the film die, the more difficult it is to achieve good profile and clear edges. A further enhancement to injector block technology is to include melt routing flexibility through reconfigurable transition blocks/flanges. This gives the option to redirect polymer streams to any entry point of a multilayer block through a simple operator selection procedure. Co-extruded products that have low conversion efficiencies and have to include recovered scrap may present particular problems. Many packaging film applications can tolerate inclusion of reclaim in the base polymer layer, but those which cannot necessitate either scrap dumping or expensive chemical separation. 5.4.4 Fillers Fillers are added to PET for two main reasons. First, to modify surface properties: particulate fillers, such as clays and silica, typically a few microns in diameter, are added to create surface roughness during the film-drawing process. A primary function of the surface roughness is to reduce the blocking or sticking propensity of the otherwise very smooth film surfaces during winding and reel formation. The roughness also enhances dynamic handling behaviour, particularly for high speed transport and winding of very thin films. Surface optical properties can also be regulated via filler-induced surface roughness, for example to control gloss or eliminate Newton's Ring fringes between adjacent film layers. Finite element methods have been applied to enable predictive capability in the design of roughened film surfaces . Second, to modify bulk properties: although mechanical properties, such as softness, stiffness and toughness, can be addressed, it is most common for optical properties to be modified via particles. Opacity and whiteness are generated by two discrete mechanisms. Simple pigmentation (light scattering from the particle-polymer interface) can be achieved using similar titanium dioxide technology to that employed in the fibres and coatings industries. It is,
PET PACKAGING TECHNOLOGY
however, more common for the anatase crystal form to be employed, since this is a less abrasive pigment than the more strongly scattering rutile. The second mechanism involves using the additive to generate micro-voiding during the film draw. The additive can be inorganic, for example barium sulphate or calcium carbonate, or polymeric, for example, polypropylene. In this mechanism, the opacity is derived from scattering between the polymer and the void. The use of micro-voiding confers the potential advantage of a softer film of reduced density. 5.4.5 Shrinkage Standard PET film from the tenter process will shrink by 1-3% after 30 min at 150°C. For the high level of accuracy required by Membrane Touch Switch printers, 0.1-0.2% shrinkage is required. In order to meet this, the film is unwound and passed through a carefully temperature controlled oven, with almost no tension in the film. The amount of residual shrinkage in the film after this process is typically 0.1% in the MD and 0.06% in the TD. 5.4.6 Combination of effects Typically, to achieve the wide range of properties required of polyester films the effects above can be combined, as illustrated in Figure 5.15. The structure of film can be further enhanced by coating on one or both sides. This is further illustrated in Table 5.8, which outlines the key properties required for packaging and other film applications. It can be clearly seen how the combination of base film properties, fillers, coatings and co-extrusion technologies have to be used to achieve the desired properties. In the packaging market, the film is commonly laminated to such substrates as polyethylene and polypropylene. This is illustrated in Figure 5.16, showing Mylar® 813, a clear film with a pretreat coating for enhanced print adhesion, which is typically used as a part of a laminate in flexible packaging. It is usually on the outside of the structure, where the excellent print quality achieved makes products stand out on retail display. Other key properties are: aroma barrier, rigidity and robust laminate performance. Other typical applications for this product, when laminated to polyethylene or polypropylene, include: • • •
stand-up pouches for such diverse products as soups and washing liquid, which is commonly a reverse-printed duplex structure (see Figure 5.16A) beverages and pet food pouches, where a high barrier is required for shelf-life (see Figure 5.16B) and where the film is reverse-printed and adhesively laminated to aluminium foil in a triplex structure coffee and other dried product packs, where the film is a metallised duplex (see Figure 5.16C) and can be surface printed
Slippy, heat sealabie
White Slippy, heat sealable
Figure 5.15 Possible film permutations achieved through combining polymer, filler and co-extrusion technologies.
PET PACKAGING TECHNOLOGY
Table 5.8 Examples of typical film applications and the key properties required Application
Film properties required
Seal (peelable through to permanent) Wide heat seal range Barrier (oxygen and aroma) White, clear Handleability Pretreats to allow metal, ink. sealant adhesion Stiffness 12-30 urn Clear, white, matt, black Durability Adhesion with inks Silicone adhesion 23-175 urn
Imaging -montage -microfilm -digital technology media
High opacity, white through to high clarity. flatness
Antistat Handleability Dimensional stability Adhesion with inks 50-175 urn
Casting and release
Wider range of surface textures from high gloss to very matte Release coats 12-50 urn
Thin film, low shrinkage. electrical - thermomechanical properties 0.9-23 urn
Electronics -flexible printed circuits, flat flexible cable -membrane touch switch -loudspeakers
Brilliant clarity-white film Electrical properties Handleability Low shrinkage Durability Adhesion with inks 12-175|im
Coil coating/fibre reinforced plastics
Heat bondable UV stable Handleability
Electrical insulation -motors -cable
High dielectric strength Thermal endurance at elevated temperatures Dimensional stability Durability Chemical resistance 12-350 urn
PET FILM AND SHEET
Table 5.8 (continued) Application
Film properties required
Tensilised film Surface quality Dimensional stability Sublayer for magnetic coating
Medical test strip
Dimensionally stable High stiffness Inert and plasticiser free Adhesion with ink Hydrophilic surface Clear (matt or glossy), white (high opacity or translucent)
Durability Adhesion with inks Heat bondable Temperature resistance 100-350 (xm
Further examples of PET film use in packaging are: films for convenience, such as lidding, where easy peel through to permanent seal, to a variety of container types, is a key feature in ready meal applications; and films for freshness, such as in meat and cheese packaging, where barrier and clarity are the key features required for modified atmosphere packaging to achieve excellent product shelf-life.
5.5 PET sheet 5.5.1 Extrusion of PET sheet PET can be converted readily into containers suitable for a wide range of packaging applications by thermoforming of extruded sheet. The technology can be considered as comprising two process stages . In the extrusion stage, the PET pellets are melted in a continuous screw extruder and the melt passes to a sheet die—ideally using a gear pump to control flow—and then on to a chilled three-roll stack, where the sheet is quenched rapidly into an amorphous cast sheet. The next stage reheats the sheet to the required temperature using an in-line, fully integrated system or a separate machine, and the sheet is thermoformed into the finished container. Standard process conditions are used for extrusion of PET into sheet. The polymer pellets must be fully dried prior to processing, with air having a dewpoint below — 30°C. This is recommended to ensure that the polymer pellets have a moisture content of less than about 10 ppm, to minimise degradation in
Figure 5.16 Illustration of laminates in flexible packaging.
PET FILM AND SHEET
the melt due to hydrolysis. The molecular weight of the polymer should be high enough to ensure reprocessed edge and web or skeletal regrind from the sheet. All regrind should be dried before re-extrusion. Levels of regrind up to about 60% can be used and should be maintained at a consistent level for the process. PET will show a small decrease in viscosity during extrusion and a high addition of regrind will give a sheet with low viscosity. Inclusion of regrind at variable levels may influence the resin melt-out characteristics. PET pellets are plasticised using a continuous screw extruder of a suitable screw design. Melt temperatures should be 270-285°C, and should be kept as low as possible to avoid degradation and generation of acetaldehyde (AA). It may be necessary to use a metering pump to ensure a uniform delivery of polymer melt and to minimise dimensional irregularities in the sheet. Static mixers can sometimes be used to reduce variability in intrinsic viscosity resulting from inadequate mixing of virgin and regrind material. Dies for sheet are flat, using either fixed or flex-lip openings. Flex-lip gives a better range of lip openings to produce sheet of required thickness, while fixed opening dies are more limited but give better gauge and temperature control. PET melt should be cast from the die onto a three-roll stack with chilled feedwater to the rolls (see Figure 5.17). The calendering system is run with a melt bank in the nip area to produce a uniform polished sheet. Rapid quenching of the melt is essential to ensure that amorphous sheet is produced with high gloss, transparency and strength. Roll temperatures will vary between 10°C and 65°C, depending on the throughput and sheet thickness. The thickness of sheet cast will be influenced by: extruder output, die lip opening and casting roll speed. From the roll stack, the sheet can be transferred to a turret winder via edge trim slitters. Sheet can be transferred directly from the roll stack to a reheat oven and thermoformed in-line, or it can be wound and stored for forming at a later date. In direct processing, edge and web scrap is usually reground in-line and transferred back for redrying. 5.5.2
Thermoforming of PET sheet
PET can be thermoformed on most conventional equipment. The forming conditions depend on the specific container design and the degree of orientation. Low pressure containers need a shallow-to-medium draw process, while for pressure containers suitable for carbonated drinks and when good barrier properties are required, it is recommended that a deep draw process is used. The deep draw process induces a high degree of orientation into the container wall, which is essential for more demanding applications. Shallow-to-medium depth drawn containers, with stretch ratios up to about 2.5:1 in the axial direction, can be formed using vacuum (lOmbar) or with a combination of vacuum and compressed air (10 bar). Deep drawn containers require plug assist technique. The type of plug and conditions will vary depending on the sheet thickness and
Dryer Trimming station
Reheat oven Thermoforming station
Product stacking & handling
1 1 t t t \f\j\f
Regrind Figure 5.17 General in-line PHT thermotorming line.
PET FILM AND SHEET
the stretch ratio. Stretch ratios up to 3:1 and sheet thicknesses up to 1.5 mm can use a cold nylon plug or polymer-coated metal plug. Deep drawn containers require oil-heated brass plugs with a temperature between 80°C and 110°C. Sheet produced in high IV PET will require the higher plug temperature. The sheet should be heated on both sides using top and bottom heaters. For shallow transparent containers, heating from the top is sufficient. The temperature of the sheet should be reheated between 90°C and 110°C; the deeper the draw and higher the PET IV, the higher the reheat temperature required. 5.5.3 Thermoforming of CPET sheet PET can be modified with nucleating additives, including polyethylene and polypropylene polymers, such as low density polyethylene (LDPE) and linear low density polyethylene (LLDPE), which are incompatible with PET but which at low levels of addition (usually about 5%) can induce rapid crystallisation of PET during reheating and the forming process. Fast crystallising PET grades, called CPET, are specially formulated for the production of opaque containers, like ovenproof and microwaveable trays. CPET grades can be extruded on conventional sheet lines but are thermoformed into a heated mould, which heat sets the CPET container. Mould temperatures are about 160°C to optimise the crystallisation of CPET, with about 2 s contact with the hot mould, giving an overall cycle time of about 5 s. The clear sheet becomes milky white and opaque when reheated at 120-145°C, which indicates that crystallisation has occurred and it is ready to be formed. Uniform heating is critical to ensure that the finished container is uniformly crystallised. Containers that are not uniformly crystallised will tend to warp and distort when heated in an oven. Overheated sheet will produce too high a level of crystallinity and poor forming, while insufficient crystallinity will cause sticking in the mould. The ideal crystallinity range in the final container is 25-35%. Forming requires vacuum, pressure and plug assist, as well as a combination of these techniques. The containers can be cut from the sheet when it is below 65°C using heavy duty presses, matched dies with close tolerance fit, and sharp cut edges. 5.5.4 Materials Dual-ovenable plastic packaging for cooking in microwave and conventional ovens was first commercial in the mid-1980s. CPET grades are available from Eastman Chemicals, as well as a more heat-resistant PCTA copolyester, Thermx'. The other major polymer producer is M&G (ex Shell), and DuPont and Kosa produce CPET grades. The PET includes a nucleating agent, which is incorporated to promote the very fast crystallisation needed for manufacture of high temperature resistant containers. High crystallinity ensures good dimensional stability of formed trays at high temperatures when cooked in an
PET PACKAGING TECHNOLOGY
oven. Control of the level of crystallinity enables processors to produce trays which withstand temperature extremes. High crystallinity induces poor impact properties; processors compensate for this with a co-extruded sheet, nip polished during extrusion to improve impact properties. Impact modifiers and nucleating agents can be added to the PET to improve low temperature impact properties. CPET trays are designed to be used over a wide temperature band, from freezer storage (down to — 40°C) to oven cooking (at 240°C). The addition of impact modifier polymers can improve the impact strength at least twofold at ambient temperatures, and up to fivefold at freezer storage temperatures, compared to standard CPET. 5.5.5
A variation on CPET for packaging is expanded PET (EPET) for food trays, which can be deep drawn and are rigid enough for most foods, including frozen foods. An ethylene vinyl alcohol copolymer (EVOH) core layer co-extruded in the EPET structure provides barrier protection, and an adhesive layer bonds the complete structure. The expanded material achieved using a proprietary technique requires modification to extrusion equipment to ensure uniform distribution of the foamed material. Foaming can be achieved with an inert gas blowing agent. The EPET material can save up to 50% on weight compared to conventional CPET. Other techniques for extending shelf-life include the incorporation of oxygen scavenging additives. CIBA have now aquired the 'Amosorb 2000' range of inorganic absorbers developed by BP Amoco, and market the range under the trade name 'Shelfplus'. The demand for dual-ovenable packaging is growing at a fast rate and the demand for microwaveable packaging is even higher. Because the temperature requirements for microwaveable packs is not as great, the choice of suitable materials can be extended beyond PET-based structures and competition is more intense. Technological developments over recent years have included the 'Melt-toMold' system offered by Lawson Mardon Therma-Plate Corp. This process has an in-line rotary drum thermoforming process, where CPET sheet is extruded in the melt phase and fed directly onto the surface of a revolving drum, then into the thermoformer. The continuous process saves energy, the containers have better definition, and better process consistency is achieved. The technology offered includes modified polymers as part of the CPET material. The improved morphology results in smaller crystals, which can improve the gas barrier properties of CPET structures compared to conventional materials. Data on CPET trays produced by the 'Melt-to-Mold' technology claim that oxygen permeation is about five times better than that of standard co-extrusion CPET/APET structures and there is a 20% reduction in thickness. Impact resistance is also improved up to fourfold. Other advantages claimed are lower container shrinkage, improved
PET FILM AND SHEET
dimensional stability, improved heat sealing properties and double seaming integrity . Co-extruded CPET/APET with the amorphous PET as the inner layer hermetically seals to the PET film lidding material before retorting. Brown Machine offer various advanced systems designed for: quick mould change, advanced oven control, process flexibility for quick material changes, cooling programmes for faster cycle times, high speed vertical trim press for extended die life and quick and easy tool changes. 5.6
The process of making biaxially oriented polyester film is complex and requires a detailed understanding of the interrelationship between polymer properties and process to give the desired final properties in the film. The unique blend of properties of PET film makes it an extremely versatile product and the growth in the films market is predicted to be above 5% per annum. However, this masks the fact that some areas, such as packaging, industrial and electrical applications, are growing at a greater rate, whereas the growth in the more traditional markets, such as magnetic media or graphic arts materials, is more modest. Advances are continually being made in uprating the film process but, in addition, new applications for PET film in both packaging and elsewhere are continually being developed. There will be an increasing trend towards differentiation through the application of new process technologies and advances in the control of the process coupled with the combinations of base polymer, filler, coating and co-extrusion technologies. 5.7
The authors would like to thank their colleagues M. Ellam, J. Robinson, D. Wager, P. Mills, K. Looney, J. Lloyd and M. Jeffels of DuPont Teijin Films™ and P. Willcocks, S. Norval and A. Broadhurst of ICI for their contribution and comments.
References 1. Encyclopedia of Polymer Science and Engineering (ed. H.F. Mark), 2nd Edition, John Wiley and Sons, New York, Vol. 12, Polyester Films, p. 193 and references therein. 2. Ajji, A., Guevremont, J., Cole, K.C. and Dumoulin, M.M. (1996) Polymer, 37, 3707. 3. Keller, A., Lester, G.R. and Morgan, L.B. (1954) Phil. Trans. Roy. Soc. (Land.), A247, 1. 4. Hartley, F.D., Lord, F.W. and Morgan, L.B. (1954) Phil. Trans. Roy. Soc. (Land.), A247, 23. 5. Tobin, M.C. (1974) /. Polym. Sci. Polym. Phys. Ed., 12, 399. 6. Tobin, M.C. (1976) J. Polym. Sci. Polym. Phys. Ed., 14, 2253.
7. 8. 9. 10. 11. 12. 13. 14. 15. 16. 17. 18. 19. 20. 21. 22. 23. 24. 25. 26. 27. 28. 29. 30. 31. 32. 33. 34. 35. 36. 37. 38. 39. 40. 41. 42. 43. 44. 45. 46. 47. 48. 49.
PET PACKAGING TECHNOLOGY
Jog, J.P. (1995) J. Macromol. Sci. Rev. Macmmol. Chem. Phys.. C35. 531. Sheldon. R.P. (1963) Polymer. 4, 213. Zachmann, H.G. and Geumther, B. (1982) Rheol. Acta. 21, 427. Pilati, E, Toselli. M.. Messori, M.. Manzoni. C.. Turturro. A. and Gattiglia. E.G. (1997) Polymer. 38, 4469. Guemther, B. and Zachmann, H.G. (1983) Polymer, 24. 1008. Gerlach, C., Buckley, C.P. and Jones. D.P. (1998) Trans. IChemE., 76 Part A. 38. Adam, A.M., Buckley, C.P. and Jones. D.P. (2000) Polymer. 41, 771. Boyce. M.C., Socrate, S. and Liana. P.G. (2000) Polymer. 41. 2183. Lorentz, G. and Tassin, J.F. (1994) Polymer. 35. 3200. LeBourvellec. G. and Beautemps. J. (1990) J. Appl. Polym. Sci.. 39, 329. Lapersonne. P.. Bower, D.I. and Ward. I.M. (1992) Polymer. 33. 1266. Salem, D.R. (1998) Polymer. 39. 7067. Blundell, D.J.. eJ al. (1996) Polymer. 37. 3303. Mahendrasingam, A., el al (2000) Polymer. 41. 7803. Blundell. D.J., et al. (2000) Polymer. 41. 7793. Blundell, D.J., et al. (1999) Polym. Bull.. 42. 357. Ashford. E.. Bachmann, M.A., Jones. D.P. and MacKerron. D.H. (2000) Trans. IChemE.. 78 Part A, 33. Rule. R.J.. MacKerron, D.H.. Mahendrasingam. A.. Martin. C. and Nye. T.M.W. (1995) Macromolecules, 28, 8517. Biangardi. H.J. and Zachmann, H.G. (1977) Prog. Colloid Polym. Sci.. 62. 71. FaisantdeChampchesnel, J.B.. Tassin. J.F.. Bower. D.I..Ward. I.M. and Lorentz. G. (1994) Polyme r. 35, 4092. Gehrke, R., Riekel, C. and Zachmann, H.G. (1989) Polymer. 30. 1582. Moscato, M.J. and Seyler. R.J. (1994) ASTM Spec. Tech. Piibl.. STP 1249. 239. Iwakura, K.. Wang. Y.D. and Cakmak. M. (1992) Intern. Polym. Processing VII. 4. 327. Khan. M.B. and Keener, C. (1996) Polym. Eng. Sci.. 36. 1290. Yamada, T. and Nonomura, C. (1994) J. Appl. Polym. Sci.. 52. 1393. Chu. W.H. and Smith. T.L. (1973) Polym. Sci. Tech.. 1. 67. Kim. G.H.. Kang, C.-K.. Chang. C.G. and Ihm. D.W. (1997) £///: Polym. J.. 33. 1633. Jungnickel. B.-J. (1984) Makromol. Chem.. 125. 121. Heffelfinger, C.J. and Burton. R.L. (1960) J. Polym. Sci.. 47. 289. Blundell. D.J. and Pendlebury. R. (1991) The Status of X-Ray Characterisation of Crystal Orientation in Polyester Film'. ICI Company Research Report. 1C 12763. Chang. H.. Schultz. J.M. and Gohil. R.M. (1993) 7. Macromol. Sci. Phys.. B32. 99. Pendlebury. R. (1977) PhD Thesis, University of Teesside. Faisant de Champchesnel. J.B.. Bower. D.I.. Ward. I.M. and Tassin. J.F. (1993) Polymer. 34. 3763. Faisant de Champchesnel. J.B.. Tassin. J.F.. Monnerie. L.. Sergot. P. and Lorent/. G. (1997) Polymer. 38.4165. Tassin. J.F.. Vigny, M. and Veyrat. D. (1999) Macnnnolek. Chem. Macromol. Symp.. 147. 209. Kugler. J.. Gilmer. J.W.. Wiswe. D.. Zachmann. H.G.. Hahn. K. and Fischer. E. (1987) Macromolecules. 20. 1116. Greener. J.. Tsou. A.H. and Blanton. T.N. (1999) Polym. Eng. Sci.. 39. 2403. Bower. D.I.. Jarvis, D.A. and Ward. I.M. (1986) 7. Rheol.. 30. 1459. Bower. D.I.. Jarvis. D.A.. Lewis. E.L.V. and Ward. I.M. (1986) J. Polym. Sci. Polym. Pins.. 24. 1481. Gohil. R.M. and Salem. D.R. (1993) 7. Appl. Polym. Sci.. 47. 1989. Gohil, R.M. (1994) J. Appl. Polym. Sci.. 52. 925. Okazaki, I. and Wunderlich. B. (1996) 7. Polym. Sci. Polym. Phys.. 34. 2941. Wunderlich. B. (1976) Macmmolecular Phvsics. Vol. 2. Academic Press. New York.
PET FILM AND SHEET
50. 51. 52. 53. 54. 55. 56. 57. 58. 59. 60. 61.
Greener, J., O'Reilly, J.M. and Contestable, B.A. (1997) Polym. Mat. Sci. Eng., 76, 266. Wilson, M.P.W. (1974) Polymer, 15, 277. Shin, W.K. (1994) Polym. Eng. Sci., 34, 1121. Watenabe, H., Asai, T. and Ouchi, I. (1980) Proc. Jpn. Congr. Mater. Res., 23, 282. Haworth, B., Dong, Z.H. and Davidson, P. (1993) Polym. Int., 32, 325. Gohil, R.M. (1993) J. Appl. Polym. Sci., 48, 1635. Gohil, R.M. (1993) J. Appl. Polym. Sci., 48, 1649. Varma, P., Lofgren, E.A. and Jabarin, S.A. (1998) Polym. Eng. Sci., 38, 245. Tsou, A.M. and Tirrell, M. ANTEC '93, p. 1730. Morel, J.F., Phung, N.D. and Joly, J.C. (1980) IEEE Tram. Electr. Insul., 15, 335. MacDonald, W.A. (1995) Trends Polym. Sci. ,3,212. Mills, P.J. (1997) Structure and Properties of Oriented Polymers (ed. I. M. Ward), 2nd Edition. Chapman & Hall, London, chapter 9. 62. Gerlach, C.G.F., Dunne, F.P.E., Jones, D.P., Mills, P.D.A. and Zahlan, N. (1996) /. Strain Anal.. 31/1, 65. 63. 'Melinar' PET 14: Sheet Extrusion and Thermoforming. 1CI. 64. Freundlich, R. and Johnson, D.C. (1992) New CPET containers at Therma-Plate. Therma-Plate Corp. FoodPlas, Orlando, Florida, USA.
Injection and co-injection preform technologies Paul Swenson
6.1 Multilayer characteristics Production of multilayer co-injection preforms is the most economical way to achieve enhanced properties in a rigid PET container. In the second half of the year 2000, the commercial introduction of several new oxygen barrierscavenger materials improved multilayer 02 performance to 62 times that of a monolayer PET bottle. This performance is a full order of magnitude better than was possible with barrier-only materials during the 1990s. Barrier-only materials, such as ethylene vinyl alcohol (EVOH) and polyamide (PA)-MXD6, in a multilayer PET container had provided only 2-4 times the OT performance of monolayer PET and, at that level of barrier improvement, large scale conversions of juices, beer and other oxygen-sensitive products did not make economic sense. Now, however, with the shelf-life extension provided by the 62 times enhancement conversion makes sense from the point of view of package cost, downstream supply line savings and consumer preference. Two of the new barrier-scavengers were developed by material suppliers for general sale to all converters and three were developed by large converters for proprietary in-house use. A joint venture between Darex and Evalca (Kuraray) introduced an EVOH-based barrier-scavenger. Honeywell, formerly Allied Signal, developed a barrier-scavenger family of materials based on PA-6. The three converters with proprietary materials, Crown Cork & Seal, SchmalbachLubeca and Continental PET Technologies, based their new barrier-scavenger on PA-MXD6. This exemplary shift in materials performance has almost coincided with the announcement of major developments in co-injection machinery and technology. Kortec, Inc., the supplier of the only co-injection machinery that operates at monolayer cycle times, has licensed certain multilayer technology from Pechiney. These two important advances—in materials and in converting machinery—will lead the next wave of conversions from glass to PET. Multilayer co-injection is the process by which one or more interior layers of material are totally encapsulated by outer virgin PET layers. It is the only technology able to provide any combination of clarity, gas-barrier, gasscavenger and recycled PET (RPET) in a single process carried out in the same cycle time as monolayer PET molding (see Figure 6.1 for materials and layer
INJECTION AND CO-INJECTION PREFORM TECHNOLOGIES
Figure 6.1 Wall sections of a multilayer container: A) three-layer wall with centered core; B) four-layer wall of barrier and recycled polyethylene terephthalate (RPET) with barrier near contents; C) four-layer wall with barrier towards outside; D) five-layer wall.
construction). Other technologies require either a second process on a separate machine (internal or external coatings, as shown in Figure 6.2) or a second injection cycle on the same machine (inject-over-inject, as shown in Figure 6.3). The net result is that a multilayer container is at least 20% less expensive than a coated or inject-over-inject container. Multilayer co-injection not only produces the least expensive high-barrier container it also produces the best-performing container. Unlike multilayer containers, coated containers do not have gas-scavenging properties and, compared to multilayer containers, coated containers have either lower gas-barrier properties or have an unattractive tint or texture imparted to the container by the coating. Multilayer co-injection technology, being simply a variant of injection molding technology, is also easier to introduce into an existing molding plant.
PET PACKAGING TECHNOLOGY
Figure 6.2 Wall sections of a coated container: A) internal coating: B) external coating.
Figure 6.3 Preform cross-section made by inject-over-inject process.
Currently employed personnel already have the basic knowledge to enable them to learn multilayer co-injection, and co-injection machinery fits directly into existing preform handling and subsequent blow molding processes. Multilayer co-injection has the advantage that the container properties can be changed by selection of the type and volume of each material injected into the preform. One of several commercially available materials having the clarity of PET could be used to provide both gas-barrier and gas-scavenger properties. One of a larger number of clear materials could be selected to provide a barrieronly property to the container. A single molding plant, or even a single machine, can easily produce containers for a variety of different applications requiring widely different properties by a simple change of material selection and volume.
INJECTION AND CO-INJECTION PREFORM TECHNOLOGIES
6.2 Applications Multilayer co-injection applications are characterized by the primary enhancement relative to monolayer PET needed for the use of the container. Performance-driven applications are those that require an increase in the gasbarrier or gas-scavenging properties relative to PET. Containers using RPET are considered to be economics-driven or legislative-driven applications. 6.2.7 Performance-driven applications The most basic performance enhancement is to increase the gas-barrier property relative to PET. Small CSD (carbonated soft drinks) containers typically require a shelf-life increase by a factor of two to four times that of a similarly sized monolayer PET container. Barrier materials, EVOH or PA-MXD6, are traditionally used to block the CO2 loss through the sidewall of the container. The thickness of the barrier layer is controlled to produce the desired shelflife. Another gas barrier application is food containers for tomato products or green teas, which require a twofold or threefold improvement of the C>2 barrier of PET to prevent oxygen ingress into the container contents. The enhanced barrier performance of the multilayer container will reduce the Oz ingress or CC>2 egress to extend the shelf-life of the packaged product. The shelf-life will expire when oxidation-induced flavor changes in the product exceed an acceptable threshold or when the CO2 level in the product drops below its acceptable level. A higher level of performance enhancement is achieved by co-injecting a material that has both gas-barrier and oxygen-scavenging properties. The barrier property of the material will reduce the permeation of both CO2 and Oo, while the scavenging ability of the material will maintain the C>2 in the container at nearly zero during the life of the scavenger. Beer and small fruit juice are products that have stimulated the development of these combination barrier/scavenger materials, which have 62 times the 02 performance of monolayer PET. 6.2.2 Economics- or legislative-driven applications The use of RPET in a container is driven by the economic goal of using a material that is less costly than virgin PET or, perhaps conversely, is required by governmental mandate regardless of the cost. Multilayer co-injection can be used to incorporate up to 40% of the preform weight as an interior layer of RPET that is totally encapsulated by the virgin PET outer layer. Since the RPET does not contact either the contents or the consumer, a non-food-contact grade material can be used. The biggest impediment to the wide scale use of bottle-to-bottle RPET is the inability to secure consistent sources of RPET except within the few countries mandating such use. RPET in the form of flake, amorphous or crystallized pellets can be used in a multilayer container.
PET PACKAGING TECHNOLOGY
Flake RPET requires special drying equipment and in-line melt filtration in the co-injection machine to remove containments. Amorphous pelletized RPET also uses special drying equipment. Crystallized RPET pellets are dried in the same manner as virgin PET. If either of the pelletized forms of RPET is melt filtered during pelletization, added melt filtration is not required during the co-injection process. 6.2.3 Combination applications Combination applications are those that combine the performance capabilities of a barrier or barrier-scavenger with the economic benefit of RPET or preform lightweighting. In an RPET application, virgin PET totally encapsulates a layer of RPET and a layer of barrier or barrier-scavenger. The lower cost of the noncontact RPET will usually offset the cost of the barrier enhancing material in order to satisfy either a cost- or legislation-mandated goal. Small CSD containers, below 500ml, may weigh the same as a 500ml container because the shelf-life requirements of these containers can only be met by a thick sidewall to prevent CC»2 loss. A multilayer 23 g container with a CC*2 barrier layer will have more than twice the shelf-life of a 29 g monolayer PET container. The 20% reduction in container weight provides a multilayer container with a 20 week shelf-life at the same cost as a monolayer container with a 10 week shelf-life. The economic advantages of the barrier-enhanced lightweight container lie in improved product quality and extended distribution flexibility. 6.3
Closure vs bottle permeation
To create a barrier-enhanced container it is necessary to rethink the relative permeation through the closure as compared to that through the bottle itself. Table 6.1 lists C>2 and CO^ permeation rates for typical 28 mm closures with standard liners and with Ch scavenger liners. Also listed are typical permeation Table 6.1 Oxygen and carbon dioxide permeation of different 500 ml containers and closures
Monolayer bottle Bottle with barrier EVOH-F101 Bottle with barrier-scavenger Closure with standard liner Closure with OT scavenger-liner
Oi ingress (ml/day)
CO2 egress (ml/day)
0.025 0.006 0.0004 0.0025 0.0002
1.60 0.50 0.50 0.20 0.20
Abbreviation: EVOH. ethylene vinyl alcohol polymer.
INJECTION AND CO-INJECTION PREFORM TECHNOLOGIES
rates for monolayer PET, barrier-enhanced multilayer and barrier-scavengerenhanced multilayer 500 ml containers. Similarly sized bottles and closures can be designed and manufactured to have permeation rates different from the listed values of these hypothetical ones but the table shows significant performance differences between monolayer and multilayer packages. A typical monolayer PET bottle has 4 times and 62 times the C>2 permeation rate of the barrierenhanced and barrier-scavenger-enhanced multilayer bottle, respectively. The enhanced-bottle COa permeation rate is less than 25% the rate of the monolayer bottle. Note that the presence of the C>2 scavenger has little effect on the CO2 performance of the base barrier material. These significant reductions in the permeation rate of the enhanced bottle make the closure permeation rate a significant factor in overall package permeation. A closure with standard liner may allow 9% and 17% of the respective 62 and CC>2 permeation of the hypothetical monolayer package, but because the permeation of the enhanced bottle is so low, the closure will be responsible for nearly 30% and 45% of the respective C>2 and CO2 permeation of the hypothetical barrier-enhanced multilayer package. The standard closure allows nearly 86% of the C>2 permeation of the barrier-scavenger-enhanced package. These large 'leaks' indicate the need to use C>2 scavenger liners to maintain the desired package performance of an enhanced bottle. Table 6.2 lists the C>2 and CO2 permeation rates of four different 500 ml bottle and closure combinations. It is clearly shown that the use of an (>2 scavenger in both the bottle and the closure will provide the extremely low permeation rate required by highly oxygen-sensitive foods or beverages. At the listed permeation rate of 0.0006 ml O2/day, the total oxygen ingress over 300 days—less than 0.2 parts per million (ppm) of the container contents—makes the scavengerenhanced package suitable for beer applications. This package provides 45 times the performance of a standard closure and monolayer PET bottle. For allowable oxygen thresholds near 5 ppm, the barrier bottle and scavenger closure provides 37% longer shelf-life than the barrier bottle with a standard closure, and one of these combinations would normally be suitable for juice and other food products.
Table 6.2 Total oxygen and carbon dioxide permeation of different 500 ml container and closure combinations
Monolayer bottle + standard closure Barrier bottle + standard closure Barrier bottle + scavenger closure Scavenger bottle + scavenger closure
O? ingress (ml/day)
CO2 egress (ml/day)
0.0275 0.0085 0.0062 0.0006
1.90 0.70 0.70 0.70
PET PACKAGING TECHNOLOGY
As discussed in the previous section, the overall package performance is a combination of the closure and the container and the only way to achieve the most economical overall performance is by engineering both the closure and container as an overall system. The ability to engineer a wide range of properties is one of the key advantages of multilayer technology. The primary variables are the properties of the materials (gas permeation rates for C>2 and CC>2, and C>2 scavenger capacity), and the amount and placement of these properties in the preform and container. 6.4.1 Barrier properties The barrier properties of a barrier material (or the barrier component of a barrier scavenger) are dependent on the relative humidity (RH) of the material experienced during its shelf-life. Figure 6.4 shows the humidity relationship of O2 permeability of EVOH-F101 and PA-MXD6. The effect of RH on CO2 permeability is similar to the oxygen relationship. In a beverage container, the
40 60 Relative humidity (%)
Figure 6.4 Coefficient of permeability of oxygen v.v relative humidity for PA-MXD6 and EVOH-FIO! Abbreviations: PA. polyamide: EVOH. ethylene vinyl alcohol.
INJECTION AND CO-INJECTION PREFORM TECHNOLOGIES
Table 6.3 Enhancing-layer relative humidity and resulting coefficient of permeability in different wail structures Coefficient of permeability (cm3 • mm/M 2 • day • atm) EVOH-F101 wan structure (see Fig. 6.1) 1A IB 1C ID
Layer relative humidity 70% 80% 90% 1/2 at 90% 1/2 at 70%
0.010 0.018 0.070
0.08 0.13 0.24
0.040 0.046 0.070
0.310 0.360 0.550
Abbreviations: EVOH, ethylene vinyl alcohol polymer; PA, polyamide.
RH across the container wall changes linearly from 100% RH at the inside surface of the wall to ambient humidity at the outside surface of the wall— assumed to be 60% RH for the purposes of engineering most containers. The radial placement of the barrier layer in the preform wall dictates the average RH of the barrier layer and, therefore, the effective permeation coefficient. Table 6.3 shows how the position of the barrier in the cross-section of the container wall affects the average RH of the barrier layer and the permeability for EVOH and PA-MXD6. Note that the O2 permeability of EVOH is less than 40% that of MXD6 at 80% RH but is equal to that of MXD6 at 90% RH. For the container performance shown in the remaining tables and figures, the position of the barrier layer is assumed to be as shown in Figure 6.1 A. Interestingly, for MXD6, the performance of the five-layer wall shown in Figure 6. ID provides less barrier effect than the three-layer wall shown in Figure 6.1 A. This is because the effective permeability of the sum of the two barrier layers (RH 90% and RH 70%) is about 13% higher than the permeability of a central layer at RH 80%. 6.4.2 Oxygen barrier The oxygen ingress of typical 500 ml containers is shown in Figure 6.5. The PETonly container has a relatively high permeation rate, reaching 1 ppm within about 16 days. The MXD6 barrier at 5% of container weight allows O2 permeation at a rate which reaches 1 ppm in about 30 days, nearly 2 times the PET-only time. The container with 5% EVOH-F101 barrier reaches 1 ppm in about 62 days, more than 4 times the PET-only time. A greater thickness of EVOH can be used to further extend the time to reach 1 ppm, but applications needing more enhancement than 5% EVOH-F101 typically use O2 barrier-scavenger rather than thicker barrier-only to extend the product shelf-life.
PET PACKAGING TECHNOLOGY
45 60 75 Time (days)
Figure 6.5 Oxygen ingress vs time for 500 ml containers enhanced with PA-MXD6 and EVOH-F101. Abbreviations: PA. polyamide: EVOH, ethylene vinyl alcohol.
Different foods and beverages have different sensitivity to oxygen ingress, and this sensitivity must be matched by the container and closure permeation rate to keep the total below the threshold level for the desired shelf-life of the package. Barrier-only containers are ideal for applications that allow oxygen ingress of 5-10ppm. If the allowable ingress is less than 5ppm, an oxygen barrier-scavenger is the preferred material (see Section 6.4.4). 6.4.3 Carbon dioxide barrier The carbon dioxide egress from several different 500 ml containers is presented in Figure 6.6. Acceptable shelf-life is often defined as the time at which the volume of CC>2 remaining reaches some percentage of the volume when the package is initially filled. The egress rate is affected by the type of barrier material, the thickness of barrier layer in the container sidewall and the distribution of the layer in the container. The difference in COo permeability between PA-MXD6 and
INJECTION AND CO-INJECTION PREFORM TECHNOLOGIES
90 120 150 180 210 Time (days)
Figure 6.6 Carbon dioxide egress vs time for 500 ml containers enhanced with PA-MXD6 and EVOHF101. Abbreviations: PA, polyamide; EVOH, ethylene vinyl alcohol.
EVOH-F101 is clearly shown at the barrier layer RH = 80% used in this example. The relative differences decrease when the barrier RH approaches 90% (see Figure 6.4 showing 62 relationships). The five-layer container with 6% volume of MXD6 will have an average barrier thickness of 4% in the container sidewall. Therefore, it has a shorter CO2 shelf-life than the 5% volume of the three-layer container having an average of 7% thickness in the sidewall and nearly zero in the thick finish and base. 6.4.4 Scavenger property The addition of an C>2 scavenger property to a barrier material completely changes the total package 02, as shown in Figure 6.7. By chemically binding O2, the scavenger maintains the C>2 level close to the amount that was initially entrained in the contents during the filling process. The addition of a scavenger extends the glass-like 02 level to a period exceeding 300 days for the 5 % barrier-scavenger volumes shown in Figure 6.7. A thicker or thinner barrier-scavenger layer will, respectively, increase or decrease the glass-like life. When the scavenger is completely bound with C>2, the permeation rate is similar to the 'barrier' rate of the base material.
PET PACKAGING TECHNOLOGY
30 60 90 120 150 180 210 240 270 300 330 360 Time (days)
Figure 6.7 Total package oxygen ingress vs time for 500 ml containers and closures enhanced with barrier or barrier-scavenger materials.
6.5 Wall structure The scavenging property of commercial scavengers is fairly independent of RH in the 70-90% range that typically occurs in container walls. This fact, coupled with the humidity dependence of the barrier property, leads to the concept that the optimal placement of the layer within the cross-section of the container wall is different for different classes of application. Figure 6.8 shows various container wall sections that maximize the container performance by the optimal placement of the barrier or barrier-scavenger layer. Figure 6.8A is recommended for most applications requiring a combination of OT scavenger and C(>> barrier. The central placement provides lower CO> permeability than placement closer to the inside wall and the scavenger layer is protected by the thickness of the outer PET layer equal to nearly half the container wall. In the wall shown in Figure 6.8B, the barrier-scavenger layer is biased toward the inside of the container, and while the thicker outside PET layer provides maximum protection of the scavenger property, the higher RH reduces the CC>2 barrier effect of the layer. Figure 6.8C shows placement of a barrier-only material layer closer to the outside wall. The CC>2 and Oz permeability are both lower because the RH at that position is lower than in the central position. While the lower RH enhances
INJECTION AND CO-INJECTION PREFORM TECHNOLOGIES
Figure 6,8 Wall sections of multilayer containers: A) with centered layer; B) with bias-inside layer; C) bias-outside layer; D) recycled polyethylene terephthalate (RPET) and biased-inside layer; E) RPET and bias-outside layer; F) centered RPET layer.
the barrier property, this bias to the outside is not recommended for an C>2 scavenging layer because the thinner outer PET wall leads to quicker saturation of the scavenger capacity. Figure 6.8D and 6.8E show four-layer structures of RPET along with either barrier or barrier-scavenger layer. For a barrier-scavenger layer, the structure shown in Figure 6.8D is recommended if the decrease in CC>2 barrier caused by the higher RH location does not make the CO2 shelf-life too short. The thickness of the RPET and outer PET layer protects the scavenging capacity of the barrierscavenger layer, and the closer proximity to the container slightly reduces the amount of C>2 desorbed into the contents from the inner PET wall. Compared to the structure shown in Figure 6.8A, the reduction in desorbed oxygen will be approximately 0.08 ppm for a typical 500 ml container. Figure 6.8E may be used to maximize the CC>2 and 62 barrier effect by placing the layer in a lower RH position. Figure 6.8F shows the wall section of a PET/RPET container. 6.6
Preform and bottle design
Apart from the position and thickness of the core layer, the design of a multilayer preform and container is no different from that of a monolayer PET container. The mechanical properties, such as top load and vacuum test, are not affected
PET PACKAGING TECHNOLOGY
by the presence of the small thickness of a barrier layer or the layer thickness of a RPET layer with intrinsic viscosity (IV) similar to the virgin PET skin. Impact failure in the gate area will be unchanged from monolayer impact tests if the barrier or RPET layer does not extend completely into the preform base (see Figure 6.9A). The design of the external dimensions of the multilayer preform is the same as that of monolayer PET. The relative thickness of the core layer in the
Figure 6.9 Layer distribution in preforms and blown container: A) preform with 'controlled fill' layer distribution; B) preform with complete fill distribution: C) container blown from preform (A).
INJECTION AND CO-INJECTION PREFORM TECHNOLOGIES
container follows the relative thickness as molded in the preform. For barrier and barrier-scavenger applications, the design of the core layer thickness and position should be such as to maximize the core thickness in that portion of the preform wall which forms the sidewall of the container. 6.6.1 Permeation through finish, sidewall and base Figure 6.9A and 6.9C show the ideal distribution of a barrier or barrier-scavenger layer in a preform and subsequent container. The tip of the preform below line 'A' corresponds to the thick amorphous portion of the base in the container. Although the preform tip and finish are a significant part of the preform weight, they form a very small portion of the surface area of the container. The small surface area in combination with the 5-10 times greater thickness than the container sidewall means that no barrier enhancement is needed in those areas of the container. In fact, any barrier material molded in those portions of the preform only increases the cost of the container without improving its performance. Table 6.4 presents data for the same CC>2 permeation rate from 500 ml containers with different MXD6 barrier layer distributions. To obtain the same permeation rate in the blown container, the total volume of MXD6 barrier material must be greater in the preform shown in Figure 6.9B than in the controlled distribution of the preform shown in Figure 6.9A, because in both cases virtually all of the permeation occurs though the thin sidewall rather than through the thick finish and base. The data show that in the structure of either bottle, the proportion of permeation through the finish and base is less than their corresponding proportion of the total surface area. Thus, there is no benefit to enhancing the barrier of the finish and base unless the permeation of the sidewall is much less than the permeation of the finish and base on a per unit area basis. It is evident that the barrier molded into the finish and base shown in Figure 6.9B does not effectively reduce the permeation rate through those portions but simply
Table 6.4 Percentage of permeation, surface area and container weight for the finish, sidewall and base portions of 500 ml containers of different structures Permeation (%)
Fig. 6.9A Finish Sidewall1 line A irrier volume o 10%CO 2 loss (including closure loss) Weeks to 10% CO2 loss (excluding closure loss)
2.4 96.4 1.2
Fig. 6.9B 1.3 98.2 0.5
Surface area (%)
4.8 93.4 1.8
16.2 74.0 9.8
PET PACKAGING TECHNOLOGY
increases the MXD6 volume in the container by 20% (from 5.0% to 6.0% of the preform weight). 6.6.2
The concept of 'controlled fill' has been developed because the overall performance of the container is improved more by enhancing the thin sidewall (92-95% of container surface area) than by enhancing the thick finish and base (both of which total about 5-8% of the container surface area). This general rule holds true until the container barrier performance exceeds more than 15 times PET. The optimal 'controlled fill' location of the leading edge of the core layer is just above the neck support ring, as shown in Figure 6.9A, and the optimal location of the trailing edge of the core layer is just below the intersection of the preform body and spherical tip, shown as line 'A' in Figure 6.9A. These limits ensure that the enhancing layer provides coverage of the container sidewall and thin portion of the base (shown outside of line 'A' in Figure 6.9C) and extends partially into the thick portion of the finish and amorphous portion of the base. The core layer position in the preform can be described in terms of coverage along the axial length of the preform, 'controlled fill' as shown in Figure 6.9A and 'complete fill' as shown in Figure 6.9B, and separately in terms of the placement between the inside and outside surfaces of the preform wall, 'centered', 'bias-inside', 'bias-outside' and 'five-layer', as shown in Figures 6.8A, B and C and 6. ID respectively. Multilayer co-injection technology capable of 'controlled fill' typically places the core layer 'centered' within the preform wall. However, one company, Kortec, has also developed the ability to place it 'biased-inside' or 'biased-outside' as well as the standard 'centered'. The multilayer technology that can produce a 'complete fill' preform places the layer 'biased-inside' or 'five-layer'. Table 6.5 lists different preform structures and the corresponding core layer volumes needed to produce the same container performance as a baseline structure 'A' of 'controlled fill' with the core layer 'centered' in the wall. The data were generated using MXD6 as a barrier layer and as the base component for the barrier-scavenger layer. Similar results occur for an EVOH or PA-6 barrier and barrier-scavenger material. Structure 'A', a bottle made from a 'controlled fill' and 'centered' preform, has the optimal overall OT and CC>2 enhancement because the enhancing layer is concentrated in the thin sidewall of the container. For the bias-inside structure of container 'B', a scavenger layer requires less volume but a barrier layer requires more volume to equal the performance of container 'A'. Conversely, for the bias-outside structure of container *C\ a scavenger layer requires more volume and a barrier layer requires less volume to duplicate the performance of the 'A' container.
Table 6.5 The enhancing-layer volumes used to maintain the same permeation rate for different layer distributions in 500 ml containers Structure
Cb scavenge! (%)
O2 Barrier (%)
O2 Desorption (ppm)
C02 Barrier (%)
Controlled fill Figure 6.9A & 6.9C Controlled fill Figure 6.9A & 6.9C Controlled fill Figure 6.9A & 6.9C
Centered Figure 6.8A RH = 80%
Optimize overall enhancement by maximizing protection in thin sidewall
Bias-inside Figure 6.8B & 6.8D RH = 90% Bias-outside Figure 6.8C & 6.8E RH = 70%
Higher RH decreases barrier properties
Lower RH improves barrier properties
Complete fill Figure 6.9B
20% of core layer is wasted in thick finish and base
Complete fill Figure 6.9B
Complete fill Figure 6.9B
Centered Figure 6.8A RH = 80% Bias-inside Figure 6.8B & 6.8D RH = 80% Bias-outside Figure 6.8C & 6.8E
Complete fill Figure 6.9B
Higher RH decreases barrier properties, and 20% of core layer is wasted in finish and base Benefit of lower RH is wasted in thick finish and base Split RH decreases barrier property, and 20% of core layer is wasted in finish
5-layer Figure 6. 1 D >/2atRH = 90% >/2 at RH = 70%
Abbreviations: RH, relative humidity; ppm, parts per million.
PET PACKAGING TECHNOLOGY
All of the structures using 'complete fill' require a greater volume of enhancing layer than the corresponding 'controlled fill' structures. For example, while a 'bias-inside' scavenger layer of container 'E' requires less volume than the 'centered' layer of container 'D', it requires 20% more volume (6% vs 5%) than the corresponding 'controlled fill' container 'B'. 6.7
Headspace oxygen absorption
Oxygen enters a container by entrainment during the filling process or by permeation through the container or closure. Any of this C>2 in excess of the amount absorbed by the contents remains in the container headspace. While the amount of headspace C>2 in a multilayer package with a properly applied closure is extremely small, for highly oxygen-sensitive foods or beverages, this O2 could be enough in some instances to produce oxidized flavors. The question then becomes, can this C>2 be absorbed by a scavenger layer in the container or by a scavenger liner of the closure before it reacts with the package contents. To be absorbed by the scavenging components of the closure or container, the C>2 must permeate through the contacting surface of the closure or container; the contacting surface of the container being the inside wall of the finish and headspace portion of the neck. The thickness of the inner PET layer in the finish is at least five times greater than in the neck, so that scavenging of headspace (>2, if any, will occur primarily through the thinner neck sidewall. However, the partial pressure of O?, even if equivalent to as much as 1 part per million (ppm) of the container contents, is so low that the driving force to cause permeation through the PET layer into the scavenging layer of the container is only 1/50 of that driving (>> into the container from the atmosphere. The active components in the closure scavenger liner are also below the contact surface of the liner, and the lack of driving force makes the permeation rate from the headspace to the liner effectively zero. The net result is that the reaction rate of OT with the contents will most likely absorb the headspace OT far faster than it could possibly be absorbed by either the closure or container scavenger components. 6.8
Oxygen desorption from PET
A portion of the small volume of oxygen that is absorbed into the PET wall of the container prior to filling will desorb into the contents after filling. Under normal atmospheric conditions, each gram of oxygen-saturated PET will contain 0.008 ml of oxygen if no oxygen scavenger is present in the container structure. Figure 6.10A and B show a uniform concentration of oxygen across the wall section of a monolayer wall and barrier layer wall, respectively, before filling the container. After filling with a low O? product, such as beer or fruit juices.
INJECTION AND CO-INJECTTON PREFORM TECHNOLOGIES
Figure 6.10 Oxygen concentration in container wall before and after filling: A) PET-only wall before filling; B) barrier-enhanced wall before filling; C) barrier-scavenger enhanced wall before filling; D) PET-only wall after filling; E) barrier enhanced wall after filling; F) barrier-scavenger enhanced wall after filling.
the soluble oxygen in the wall will desorb from the PET into the contents. For a monolayer wall, the concentration gradient will be as shown in Figure 6.10D, reflecting the fact that half the oxygen originally in the wall has desorbed out of the wall. The concentration of oxygen in the inner wall of Figure 6.10E is nearly zero because it is easier for C>2 to permeate through the inner PET layer than it is to permeate through the barrier layer. Approximately 50% of the original oxygen will have desorbed into the contents, and although the amount of desorption is similar to the monolayer wall, the concentration gradient after filling is different. The placement of a scavenger layer in the wall produces an 02 concentration gradient across the wall even before the container is filled. As shown in Figure 6. IOC, the concentration is zero at the scavenger/PET interface. Figure 6.1 OF depicts the concentration gradient after the oxygen has desorbed from the PET. In a scavenger structure, approximately 25% of the oxygen in the inside PET wall at the time of filling migrates into the scavenger layer. The remaining 75% desorbs into the contents. Table 6.6 lists the amount of oxygen desorbed from the walls of different container structures. Scavenger-enhanced containers desorb less oxygen than containers enhanced with only a barrier layer. As expressed in terms of ppm of the contents, the amount of desorbed O2 is only significant if the contents have a shelf-life 62 threshold of less than 5 ppm. If the threshold is less than 3 ppm, the amount desorbed by a barrier-only container (0.37 ppm) will begin
PET PACKAGING TECHNOLOGY Table 6.6 Oxygen desorbed from PET into contents for different 500 ml container structures Structure
Oxygen desorbed (O? ppm in contents)
Center barrier Center scavenger Offset scavenger-inside
6.8A 6.8A 6.8B
0.37 0.18 0.10
to have a significant effect on shelf-life. The difference between the center and the bias-inside scavenger layer is a relatively small portion (0.08 ppm) of the threshold of even the most sensitive food or beverage product.
Beer is probably the most oxygen-sensitive beverage that is packaged in plastic. The total package C>2 threshold is typically in the 1-2 ppm range, and some beers are even below 1 ppm. Thus, a beer package requires the use of scavenger components in both the closure and the container. Table 6.2 shows a total package O2 permeation rate of 0.0006 ml/day. This rate will allow 0.09 ppm (>2 ingress over a 150 day life. If this permeated oxygen is added to the oxygen desorbed from the PET in a container with a central barrier-scavenger, the total O? ingress will be less than 0.3 ppm (see Figure 6.7). Oxygen ingress is only part of the permeation design for a beer container. Carbon dioxide egress defines the requirements of the barrier component of the barrier-scavenger. When using any of the commercially available materials, the thickness of the barrier-scavenger layer is dictated by the requirement to slow CO? egress rather than by the capacity of the Oo scavenging component. For example, the thickness that would provide 150 days of CO2 life has enough oxygen scavenging capacity to prevent O? ingress for more than 300 days. The placement of the barrier-scavenger layer in the wall must balance several factors: oxygen desorption, CO^ ingress vs relative humidity of the barrier layer and cost. Scavenger layers are effective when located in the center of the wall or when biased toward the inside wall surface of the container. However, the higher RH of a layer closer to the inside of the container increases the CO2 permeability of the barrier layer by 50%. For the preform shown in Figure 6.9A, Table 6.7 shows the changes in O2 desorption and CO2 shelf-life caused by the barrier position in the container wall. This position change will decrease the CO2 shelf-life by 14%, or conversely, require a 50% increase (from 5% to 7.5%) in barrier-scavenger volume to maintain the same CO? life as does a centrally placed layer.
INJECTION AND CO-INJECTION PREFORM TECHNOLOGIES
Table 6.7 Oxygen desorption, oxygen permeation and carbon dioxide shelf-life for 500ml containers with different wall structures and layer volumes Barrier scavenger position
Layer volume (%)
Desorbed 03 (ppm)
O? permeation (ml/day)
CO2 life (weeks)
5.0 5.0 7.5
0.18 0.10 0.10
0.0006 0.0006 0.0006
20.9 18.0 20.9
Center of wall Bias-inside Bias-inside
The bias-inside scavenger layer halves the already low C>2 desorption, from 0.18 ppm to 0.10 ppm, but requires a thicker layer to meet the CC>2 shelf-life requirements. The cost of the layer thickness increase to achieve 0.08 ppm desorption decrease adds about 3% to the price of a barrier-scavenger-enhanced bottle. Thus, the ideal structure to optimize the C>2 and CO2 performance for a product such as beer is the central barrier-scavenger layer shown in Figure 6.8A. For a typical scavenger-lined closure and 500ml beer bottle with 5% volume of barrier-scavenger centrally placed in the wall, the total package oxygen is plotted in Figure 6.11. The initial oxygen level is the sum of the C>2 entrained in 1 T-
90 120 Time (days)
Figure 6.11 Total package oxygen vs time for 500 ml barrier-scavenger enhanced container.
PET PACKAGING TECHNOLOGY
the beer at the time of filling (typically 0.20 ppm) and the 02 desorbed from the PET (0.18 ppm). The graph shows the desorption taking place in the first week after filling. For purposes of comparison, the CCh shelf-life expiration time is shown at 150 days. If a 'complete fill' with 'bias-inside' layer is used to distribute the barrierscavenger in the preform, the desorbed C>2 is reduced to 0.10 ppm, but the core volume must be increased to 9.0% of the preform to achieve the same COo shelf-life. A thicker barrier layer is required by the humidity affect of the 'biasinside' position, and the extra core volume in the finish and base does not extend the CC>2 shelf-life. The additional core volume increases the price of the bottle by about 6%, and while it does decrease the C>2 desorption by 0.08 ppm (from 0.18 ppm to 0.10 ppm), it does not improve either the COi shelf-life or the O2 ingress rate after desorption. 6.10
Small juice containers
Fruit juices typically have oxygen thresholds in the range of 2-10 ppm. To achieve a desired shelf-life for juices at the lower end of the range (< 5 ppm), an oxygen barrier-scavenger core layer is usually used in bottle sizes of 500 ml or smaller. At the higher end of the allowable oxygen threshold, a barrier-only core layer usually provides sufficient shelf-life. For example, the 500 ml container shown in Figure 6.5 using 5% volume of EVOH-F101 has less than 3 ppm O2 ingress at 180 days. That same container with a barrier-scavenger layer is suitable for the most sensitive juice product, and will have less than 1 ppm ingress over the same time period, as illustrated in Figure 6.7. Because juices require only oxygen protection, it is worthwhile to consider whether 'bias-inside' or 'bias-outside' placement of the enhancing layer will improve the economics of package performance. The most economical combination of layer material and preform wall structure is 3-4% volume of a 'centered' barrier-scavenger. This combination will be less expensive, yet give a longer shelf-life, than as much as 5% EVOH barrier 'biased-outside' to maximize its barrier property. Since 3% is the lower limit of core layer volume in a multilayer preform, there is usually no advantage to a 'bias-inside' placement of the scavenger except for shelf-life requirements that approach one year duration. 6.11
Small CSD containers
Small containers for carbonated soft drinks have not been widely used because their CO2 shelf-life has been too short for the capabilities of even the best soft drink distribution systems. Monolayer PET packages as small as 400 ml have been made with the same preforms normally used on 600 ml containers in order
INJECTION AND CO-INJECTION PREFORM TECHNOLOGIES
EVOH-F101 (4%) 23 g
15 30 45 60 75 90 105 120 135 150
Time (days) Figure 6.12 Carbon dioxide egress vs time for 400 ml carbonated soft drink (CSD) containers weighing 23 g and 29 g. Abbreviations: PET, polyethylene terephthalate; EVOH, ethylene vinyl alcohol.
to produce a thicker PET sidewall that compensates for the adversely increasing surface area-to-volume ratio of the smaller package. The heavier walled container typically has a marginally acceptable shelf-life and is relatively expensive because of the extra PET weight and longer cycle times for injection molding. Multilayer preforms with a CC>2 barrier layer can provide in excess of 20 weeks shelf-life while reducing preform weights by 6g. Figure 6.12 shows the CO2 barrier performance of a 400 ml container made from a standard heavy preform, 29 g, and the corresponding performance of a 23 g preform with and without barrier enhancement. Enhancement with MXD6 extends the shelf-life to 15 weeks from the 10 week shelf-life of the heavyweight PET monolayer container. The higher barrier properties of an EVOH layer extend the shelflife to more than 20 weeks. When using multilayer technology that can run at monolayer cycle times, the cost of the enhanced container can actually be less than the cost of the heavyweight monolayer container, while doubling its shelflife. The resulting economic benefits of longer shelf-life on bottling distribution efficiencies flow to the bottom line of the bottlers. 6.12
Core layer volumes
The performance of every multilayer container can be optimized to provide the most economical package to meet the performance demanded by its specific
PET PACKAGING TECHNOLOGY
Table 6.8 Typical volumes of enhancing layers for different applications Enhancing-layer volume (ide
1 tr& cond
•*——.—•— 2 45-75 W/m 2K
Heat transfer coefficients:
2-4 W/m 2K
Figure 8.21 Impact of various factors on preform reheating: thermal balance for the preform wall. Variables: q, heat flow; r. radial axis; /. longitudinal axis. Subscripts: rad, radiation; conv. convection; cond. conduction; tr. transmission.
TWO-STAGE INJECTION STRETCH BLOW MOULDING
Figure 8.22 Lamp and preform configuration in a reheating oven.
in that section but also because there is little (second lamp) or no (first lamp) neighbour-lamp impact to get the heat flow to high levels. This makes it difficult to apply much heat in this section of the preform. Heat is required in this section of the preform to start the stretch blow process and predetermines the overall material distribution in the bottle. The middle lamps are usually moved a little further away from the preform (larger distance to the surface) to ensure that they can be operated at high power with good heat penetration into the preform wall (wave length). This is because the close array of lamps cause heating overlap effects from the individual lamps, which result in high heat flows to the middle section of the preform. Here, the effect of surface cooling on the outside of the preform wall is most important. The top lamps can return to a reduced distance from the preform surface; ideally they are adjustable in height position and proximity with flexibility that makes the end-cap of the preforms easier to reheat. While the middle lamps typically have a distance of 15-20 mm, depending on the length of the preform, the lower-level lamps are at the low end of this range. The upper lamps, with the target heating area in the end-cap, can be at the high end of the range. The geometrical arrangement of the lamps relative to the surface of the preforms allows pre-profiling of the heat along the preform length, while the power of the heater lamps gives the additional variable of adjusting the final heat profile. Ideally, as mentioned above, the lamps should be operated in a power range that gives the maximum lamp temperature allowing the best possible heat penetration. A typical temperature profile along the preform axis is shown in
PET PACKAGING TECHNOLOGY
Length axis (mm)
Figure 8.23 Temperature profile along the preform axis.
Figure 8.23, indicating that the higher temperature is necessary between the support ring level and the body of the preform (i.e. in the tapered section). This section is first pre-stretched and subsequently blow-expanded to form the base bubble, which then propagates from the neck of the preform over the whole length into the final container. Heating and equilibration times may have a considerable impact on the effectiveness of the reheating process. While it is not necessarily advantageous to have long heating times—since this adds to the complexity caused by the influence of heat conduction within the preform wall—there is a relationship between the wall thickness to be reheated and the time needed to reach the required temperature range. Practical experience shows that times between 15 and 25 s are appropriate to reheat preforms to their required temperature range and accomplish the profiling during this time period. Good results have been achieved, in conventional high-performance heating systems, with equilibration times of 40-60% of the heating times. These equilibration times can be split between two heating sections and prior to stretch blowing. However, most machines do not accommodate this favourable feature. The typical effect of having an equilibration period following a heating period is shown in Figure 8.24. It is obvious that the temperature level on the inside wall of the preform lags behind that on the outside during the heating phase, although it recovers and exceeds the level of the outside temperature during the equilibration period. The length of the equilibration period will determine the eventual difference between the inside and outside temperatures of the preform wall. Key factors affecting the gradient of the cooling during equilibration time are the temperature of the
TWO-STAGE INJECTION STRETCH BLOW MOULDING
Figure 8.24 Time v,v T inside/T outside (Ti/To) for heating and equilibration.
environment and heat transfer coefficient assumed for the surface of the preform. It must be supposed that in preform sections with uniform wall thickness this effect will also be uniform over the length of the preform. This assumption may not be true because of variation in lamp radiation temperature (i.e. aging of lamps), outside cooling effects during reheating (forced air convection or sudden changes in room temperature) and the potential conductive heat input from thicker sections at the end of the cylindrical (equal wall thickness) portion of a preform. 188.8.131.52 Stretch blow moulding Stretch blow moulding is carried out in four subsequent phases, which occur in the blow mould once a reheated (and temperature equilibrated) preform has been delivered to the blowing stations. These four key phases are: • •
axial pre-stretching pre-blowing and bubble propagation up to typically 90-95% of the final shape of the container • final blowing to the residual shape of the container • cooling of the stretch blown container in the closed mould These four phases are shown in Figure 8.25. The axial pre-stretching (steps 2 and 3) overlap with the start of pre-blowing (step 4) in a way that will help to determine the final material distribution in the container. The longer the pre-stretching occurs, the more material will be transferred to the base end of the container. The earlier the pre-blowing starts, the more material will be expanded early enough to be pressed to the chilled mould wail which prohibits any further material distribution, thus keeping it in that very section. The propagation of the bubble proceeds so that the material makes contact with the wall in the shoulder, body and base section of the container mould (steps 5—8). The high-pressure final blow is applied (step 9) to shape the ultimate contour of the container,
PET PACKAGING TECHNOLOGY
Figure 8.25 Steps I-10 in the stretch blow-moulding process.
which is then frozen through contact cooling (step 10) on the wall of the watercooled mould (ideally 4-12°C). Eventually, the pressure is released from the container mould when the container can maintain its shape and dimensions without any impact on the desired properties. This requirement determines the so-called mould-close-time that, for a standard container, is typically in the range 1.8-2.3 s. The most critical section of the container to cool down is the base section, since the wall thickness of the base remains relatively high. Having been heated to the deformation temperature in order to allow the forming of the base shape, it now needs all this heat removing to maintain base dimensional stability. This time is broken down into the phases displayed in Figure 8.26. The cooling time is required mostly from a physical point of view so that a process optimization often starts with a time for pre-stretch (0.1-0.15 s) and pre-blow (0.3-0.6 s). Depending on the container being blown and the available exhaust
Figure 8.26 Mould close time breakdown.
TWO-STAGE INJECTION STRETCH BLOW MOULDING
Figure 8.27 Pressure curve.
section of a blow system the exhaust time of the high-pressure blow air takes a relatively fixed amount of time (0.2-0.5 s), leaving a total of 1.2-1.5 s for the final blow and cooling. Blow channel cross-sections and valve configuration then determine how the pressure (which has built up during the final blow stage) will be released. This can be achieved very quickly, leaving most of the time for cooling, or slightly more slowly which can cost about 25% of the cooling effect in the mould. A typical pressure curve is shown in Figure 8.27. Pre-blow pressures are usually set in the range of 5-15 bar, while final blow pressures are operated above 35 to a maximum of 40 bar (limited through readily available compressors). Pre-stretching speeds can range 0.5-1.5 m/s; it may sometimes be necessary to adjust the speed of the stretch rod independently from any other process parameter. This will assist control of material distribution during the blowing process and will allow the stretch rod to advance at maximum speed to the correct position within the preform before actually commencing the stretch. It is obvious that heavier preform/bottle combinations will require a longer period of reheating as well as stretch blowing, especially when additional processes are added, for example thermal treatments such as heat-setting. Very light preform/bottle combinations do not cause the opposite effect to any considerable extent since timing is already squeezed to a minimum for most standard containers within the limits cited above. Speciality containers designed with rectangular or other fancy features in the base, shoulder or other sections will require the whole process to be sequenced from the other end. This means stretching the end portion of the preform first and blowing the bottle starting from the base. It requires skill in temperature profiling and process control but may at times lead to good results with very fast blowing processes, almost omitting the pre-blow stage; however, these
PET PACKAGING TECHNOLOGY
are complex process conditions that standard commercial equipment does not usually allow. 184.108.40.206 Technologies for thermally stable containers Thermal treatment of PET has an impact on the properties of the material. The aim is always to increase the thermal stability of the package and its performance relative to heat exposure. Once a container is blown under the standard stretch blow moulding process, any kind of thermal treatment could be carried out in the blow mould or in any other device that will maintain the shape of the container. If this cannot be accomplished, any treatment above the glass transition temperature will release part of the orientation that has been induced during the stretch blow moulding process and the container will lose its shape. The temperature under which the thermal treatment is carried out determines the level of change in properties of the container. There are four different levels of thermal treatment, as summarized in Table 8.9. These different technologies overlap. Most of the treatment requirements are defined by the filling process of a container subsequent to the blowing process. It is imperative to know the exact filling temperature the container will have to stand and for how long, and under which conditions the container will then be chilled down to room or storage temperature. PET has little thermal stability above the glass transition temperature. Thermal relaxation and pre-shrinkage. Thermal relaxation is carried out in warm moulds (30-70°C) and is a process that pre-shrinks the container when it is being produced. Machine speed and container cost are only marginally Table 8.9 Thermal treatment: methods to thermally stabilize PET bottles
Typical bottle weight 1 .5 Itr Filling temperature Duration to quench ( * ) Output range Mould temperature
Heat set one mould
Heatset dual mould
< 1 min
bphV -1500 station C
mould only post cooling internal air internal gas/ internal water air cooling spray cooling cooling
Add'l technique Crystallinity
( * ) with less than 2 1.33). PVC has a similar density to PET (> 1.33) and will remain in the same fraction. Complete separation of all PVC materials before grinding and washing is essential for good quality. Heavily printed label sections and metallic/metalised materials can also appear in this fraction. Hydrocyclones are much faster, more efficient and easier to adjust for quality than the older settling tank systems, and are a major component of modern plastic recycling plants. 220.127.116.11 Final sorting This is an optional stage designed to reject discoloured, degraded or nonconforming species. This equipment is expensive to install but essential for high quality R-PET. Excessive black specks from degraded adhesive or dirt can reduce yields significantly. Sorting is usually based on photometric selection according to optical reflection, colour, shape and size. Once the non-conforming flakes are identified, a jet of compressed air removes them. The actual set-up of the selection is critical; if it is too sensitive, the yields of the main product will fall as more good product is rejected with the impurities. 18.104.22.168 Melt filtration, repelletisation This is an optional stage, often combined with solid state polymerisation (SSP) to produce the highest quality product. Here, non-melting particles are removed and pellet uniformity is achieved, which is essential for good drying and uniform processing. Feedstock from selected used PET containers is treated by this type of technology and the R-PET used in an identical fashion to virgin material. Recyclers will eliminate as many of the stages as possible to reduce costs and at the same time provide the product quality assurance needed by the end user. The product achieved in stage 20 is relatively pure, clean flake and is suitable for the majority of R-PET end-use applications (e.g. fibre and sheet). The end uses here are only limited by molecular weight and high purity constraints. Strapping tape is one end use that demands a relatively high molecular weight (IV usually > 0.80). This is achieved by SSP of either the washed flake or repelletised chip at about 220°C, under vacuum or an atmosphere of inert gas, for up to 10 h (stage 29). If flake is used for this additional process, it is important that the chip is of regular size to ensure uniform molecular weight distribution, an essential condition for homogenous melting during subsequent reprocessing. If repelletised chip is used, then the final product is of almost the same consistency as virgin and can be blended and used together with virgin without any major difficulties.
PET PACKAGING TECHNOLOGY
For further detail on types of equipment available for cleaning PET, the reader should contact specialist suppliers . The reader can also consult a comprehensive review of the recycling and recovery of all plastics . 11.6.4 R-PET and food-contact quality Health and safety of the consumer is the prime concern in considering the reuse and recycling of any materials in food-contact applications. In this context, RPET has to comply with all the rules and regulations that apply to virgin PET. One particular property of PET, when compared to other plastics, is its low diffusion coefficient. This is a factor of 100 lower than some other materials, which means it is more difficult for contaminants to diffuse into or out of PET [ 18]. There is no specific EU legislation that covers recycled plastics; most regulations neither preclude nor allow such use in food contact applications. However, there are exceptions and some national regulations expressly forbid such applications. Research work to define safe boundaries and possible limitations of use can be consulted . EU legislation covering the recycling of packaging materials has provided incentives to look at all potential outlets for R-PET. As food contact applications are the largest market, this area has received much attention. Some manufacturers of recycling equipment now offer plant that is said to be capable of purifying R-PET to a standard which allows it to comply with the current regulations. One such construction, the Erema 'two-step process' (illustrated in Figure 11.4), claims to be capable of raising the molecular weight sufficiently in the first section to produce R-PET polymer to reuse for manufacture of bottles. The final purification is also claimed to be of satisfactory quality for food contact applications . A number of other inventions seeking similar purity without resorting to the more certain but costlier solvolysis techniques can be studied in the relatively recent patent literature. The references here are not comprehensive; the reader can use them as a good initial source of information and they also provide other 'prior art' references. Starting with washed, clean flake followed by a degassing technique in the solid phase and subsequent melt extrusion/vacuum venting, produces a high purity R-PET [21 ]; spiking techniques with contaminants, such as toluene, benzophenone, metal arsenates and chloroform, are used to show the effectiveness of the cleaning. A similar technique with two independent extruders was previously patented . Washed, clean R-PET is further decontaminated by leaching with solvents, such as acetone and ethyl acetate, which dissolve in and swell the PET and are easily removed afterwards . Preextraction of R-PET flake with methyl ethyl ketone, tetrahydrofuran (THF) or dioxane is claimed to remove PVC and PS, in addition to other impurities. The extracted R-PET is then dissolved in ethyl carbonate or dimethyl phthalate before recovery by precipitation using cool solvent . Steam 'stripping' of
a = Conveyor belt b = Rotary tools e = Vacuum cutter compacter/driver h = Extruder i = Screen changer
c = Transfer screw f = Extruder intake
d = Vacuum slide valve g = Double venting
Figure 11.4 Erema 'two-step process' plant for high purification of recycled PET. Figure redrawn from Erema publications .
PET PACKAGING TECHNOLOGY
prewashed R-PET flake at 150-190°C is claimed to achieve high purity , as is nitrogen purging at 218°C using washed flake of specified particle size . Treatment of washed PET flake, reclaimed from used bottles, with a calculated amount of 50% sodium hydroxide solution to react with about 3-10% of the PET, at temperatures just below melting (ca 250CC), partially saponifies the PET and is claimed to strip free the contaminated surface layer. This process is the technological basis of new plant commissioned in Switzerland in 2000 . 11.6.5 Recycling of PET by chemical methods— 'solvolysis' Solvolytic methods are much more complicated than straightforward washing processes and are more energy intensive. They also need specialist plant and are therefore more costly, especially if performed on a small scale (i.e. below 20-30 K tonnes per annum). However, they can utilise lower quality feedstock as the processes allow additional purification to be performed. PET can be recycled by breaking down the polymer chains by treatment with chemicals, such as: alcohols, e.g. methanol (methanolysis, producing dimethyl terephthalate [DMT] monomer); ethylene glycol (glycolysis, producing bis[hydroxyethyl]terephthalate [BHET] monomer); acids (hydrolysis); or alkalis (saponification). These treatments effectively depolymerise the PET. reform the partially esterified monomers and, finally, the intermediates of terephthalic acid (TA) and ethylene glycol (EG). However, the two major processes that have been used commercially are glycolysis and methanolysis. Polyesterification is an equilibrium reaction and the depolymerisation is carried out with an excess of the solvent to force the reaction backwards and regenerate the intermediates (see Figure 11.5). Selection of the most appropriate technique is dependent upon the quality of the available feedstock and the quality of the products required. Glycolysis is a compromise between simple washing and reprocessing of the clean flake by melt extrusion and complete recovery of the intermediates by methanolysis and hydrolysis procedures. To be economically attractive, depolymerisation facilities should achieve a minimum economy of scale dependent upon the cost and purity of the feedstock.
HO-CH,-CH. OCCO-CH,-CH. OH
-HO-CH2-CH2-OH fEG' PET polymer
^^ R = CH3 = DMT for methanolysis R = HO-CH2-CH2-0 = BHET for glycotys.s R = H = TA for hydrolysis
Figure 11.5 Depolymerisation reactions of PET. Abbreviations: PET. polyethylene terephthalate: EG. ethylene glycol; DMT. dimethyl terephthalate: BHET. bis (hydroxyethyl) terephthalate: TA. terephthalic acid.
ENVIRONMENTAL AND RECYCLING CONSIDERATIONS
Using post-consumer recovered PET containers as a source, the expected economical plant size will exceed 15,000 tonnes per annum, with plant sizes in the region of 40,000-50,000 annual tonnes more advantageous. Finding reliable and continual sources of feedstock to supply plants of this size has not been sustainable so far but with the increasing volumes of PET bottles collected by the national recovery associations this limitation may soon be overcome. It is possible to convert PET into alternative intermediate compounds, known as polyols, by breaking down the chains with polyglycols and ethylene oxide treatment. These compounds are available for conversion into polyurethane and polyisocyanurate foams and resins. This topic has also been the subject of research trials but as yet no widespread commercial development . 22.214.171.124 Glycolysis[29,3\] Glycolysis involves treating the PET with excess of ethylene glycol, driving the reaction backwards and forming BHET with smaller quantities of oligomers (n — 3-6). BHET is the intermediate formed by the reaction of TA with EG in the direct esterification process. This reaction is normally effected under pressure, at temperatures preferably about 210-220°C, to achieve a fast enough reaction rate; an ester-interchange catalyst (e.g. zinc acetate) can be used to speed up the process. At room temperature, BHET is a waxy solid of relatively high melting point, which cannot be purified by distillation (unlike DMT). BHET is not isolated as a generic product and is part of the dynamics of the conventional esterification process. Purification is normally effected by melt filtration under pressure to remove physical impurities, preceded (or followed) by possible treatment with carbon, which by selective adsorption removes chemical impurities that lead to poor colour and oxidative degradation. The filtration processes can be very cumbersome if significant quantities of fine pigments or colours, like titania, are to be removed. In glycolytic processes, nonpigment colours that are intentionally added to PET or copolymer constituents are not generally removed. Acid-based modifiers, such as isophthalic acid (IPA), will also remain and react again in the process. Heating ethylene glycol at high temperatures also forms higher glycols, such as diethylene glycol (DEG), as byproducts. This component will also polymerise and has the effect of reducing the melting point of the resultant PET; it therefore needs to be kept well under control. Catalysts (e.g. sodium acetate trihydrate) can be used to suppress DEG formation . The process is therefore preferably carried out with recovered material of known history and high quality. Feedstock will usually be well washed and cleaned before use. It is normally integrated well into conventional plant operations and nearly always used as a careful blend with mainstream BHET, usually less than 25% concentration. The risk of contamination of mainstream operations is high and careful attention to the quality of the recovered feedstock is vital. To place the risk in context, modern direct esterification plants produce
PET PACKAGING TECHNOLOGY
ca 250,000 tonnes per year in continuous steady-state operation; any disruption will cause a major disturbance. Glycolysis polymer is nearly always inferior in colour and physical properties when compared to virgin and the end-use outlets are carefully selected . Glycolysis has some significant advantages over either methanolysis or hydrolysis, primarily because BHET may be used as a raw material for either a DMT-based or a TPA-based PET production process without major modification of the production facility. Another significant advantage provided by the glycolysis technique is that the removal of glycol from the depolymerisation solvent is not necessary. Glycolysis principles have been utilized to generate polyester diol precursors for manufacture of polyurethanes (PU) or polyisocyanurates. The mixture obtained from boiling PET with glycol at 200°C is esterified with adipic acid (220° C) and forms a product suitable for manufacture of polyurethane foam insulation [29, 31]. Scrap PET can be treated with diethylene glycol to form a low molecular weight modified aromatic polyol, which is further reacted with an aliphatic polyol (ethoxylated methyl glycoside) to form another suitable precursor (see  for useful references to prior art). Figure 11.6 illustrates some examples of the depolymerisation of PET by the glycolysis and methanolysis routes. 126.96.36.199 Methanolysis Treatment of PET with methanol, again under pressure and at temperatures around 200°C, reverses the polymerisation in a similar manner to glycolysis but the intermediate produced is dimethyl terephthalate (DMT) along with ethylene glycol. The reaction uses a transesterification catalyst, usually the acetate of cobalt, magnesium, manganese or zinc; this intermediate is very well characterised and a commercially traded product with defined properties. DMT is purified by distillation, a process that yields high purity, especially free from physical contaminants. In this respect, it is much easier to purify than BHET and can generally accept an input specification of lower physical quality. However, organic impurities leading to poor colour may still persist and complete removal is not always possible. The product is usually isolated prior to reuse, and can be subject to final analysis followed by appropriate blending before reuse. DMT derived from methanolysis of post-consumer recovered containers generally has a product quality identical to that of DMT from virgin routes and is used for all DMT applications. Development of the process has concentrated on increasing the yields of DMT, which means moving the reaction away from the equilibrium condition reducing the formation of oligomers and BHET. One improvement describes dissolution of the PET in oligomers of EG and TA or DMT; super-heated methanol is then passed through the solution. The EG and DMT are recovered overhead . In a further refinement, the process is adjusted to produce 'half-esters'
Used PET bottles
Kecoverea cleaned PET (R-PET)
1r Treat with excess methanol at 200°C, high pressure
DMT Carbon treat, filter distillation to purify (or crystallisation)
Y Methanol and ethylene glycol recovery
Production of PET polymer
BHET Carbon treat, pressure filtration to purify
\r Treat with ex cess ethylene glyc olor 180 ;?20°C, high p •essure
J BHET Blending operations
PET bottles Figure 11,6 Examples of glycolysis and methanoiysis routes to depolymerisation of PET. Abbreviations: DMT. dimethyl terephthalate: BHET, bis (hydroxycthyl) terephthalate.
PET PACKAGING TECHNOLOGY
(esters of TA with methanol and EG). The advantage of this development is that these half-esters have the potential to be used in either DMT or TA based polymerisation processes without additional purification. This should reduce the number of stages, use less equipment and consume less energy than previous methanolysis type processes (see , which includes a good review of earlier processes). Both glycolysis and methanolysis use materials that are well established within the PET manufacturing process flowsheets, and their impact on product and process quality is very well understood. Ethylene glycol and methanol are easily recovered and reused within the process, with little solid or other waste. Economics are also very well understood; plant design and achievement of throughputs can be forecast with high accuracy. 188.8.131.52 Hydrolysis Hydrolysis of PET is conducted by treating the PET with water, mineral acids or caustic soda (see Figure 11.7). The TA obtained is referred to as 'crude' and is then subject to purification by crystallisation, from solvents like acetic acid, to achieve standards equivalent to available commercial grades of TA. Like the other depolymerisation processes, it is also possible to treat with activated carbon to remove the organic impurities. The economics of these processes are highly dependent on scale, degree of purification required and utilisation of the by-products. Chemical purity of the TA is only one aspect of its acceptability; modern direct esterification technology demands TA that forms 'pre-mixtures' with EG and resultant viscosities that allow rapid transfer by pumping methods. Similarly, dispersion rates of the TA within the glycol to form 'slurries' are dependent upon the particle size and shape. The glycol segment is purified by distillation. The TA product is not easy to purify to a standard normally acceptable for direct esterification but this can be done. Multiple recrystallisations of TA improve purity but at extra cost. Following these processes, uses must be found for neutralisation residues, such as sodium sulphate. Hydrolytic breakdown of PET into its prime intermediates followed by repolymerisation is likely to be more expensive than either glycolysis or methanolysis, as it involves additional processing stages. However, it allows purification of both intermediates to levels equivalent to that of virgin products. Although these processes work technically, satisfactory commercial processes are not operating at present. Older technology describes the use of concentrated sulphuric acid (11 acid:2 water) at room temperature to achieve hydrolysis within minutes. The resultant crude TA is precipitated by dilution, filtered, and dissolved in alkali to effect further purification . Recent developments have used solid sodium hydroxide to initiate and speed up the reaction, driving off glycol and then diluting with water. This allows operation at atmospheric pressures. Purification can be effected by extracting impurities with butanol
Hydrolysis with water 220°C/sodium acetate catalyst, 4h
Hydrolysis with mineral acid Sulphuric acid 60-90°C, atmospheric pressure, within minutes
Recovered cleaned PET (R-PET)
Hydrolysis with caustic (2) Sodium hydroxide/1 00°C, atmospheric pressure, less than 1 h (also + 50% solution stoichiometric ratio 200-300°C)
Hydrolysis with caustic (1 ) 8-10%solution/200°C, 15-20Atms, over 4 h
Neutralise with mineral acid to release the solid TA Terephthalic acid and ethylene glycol Purification Figure 11.7 Examples of hydrolytic routes for depolymerisation of PET. Abbreviation: TA, terephthalic acid.
PET PACKAGING TECHNOLOGY
before passing the solution down a column of activated charcoal to remove the remaining impurities. The technology is known as the RECOPET process . A similar technique uses a strong caustic solution (ca 50%) to form a slurry of disodium terephthalate, which is heated to 300 C to drive off the glycol and destroy other organic contaminants. The resultant mobile slurry is then diluted with water, and further purified by centrifugation and filtration before recovering the TA by neutralisation with mineral acid. The high temperatures used suggest that the process could be used for highly contaminated PET wastes. This technology is known as the 'UNPET' process . In another variation, relatively clean PET bottle scrap is first treated with boiling EG using a countercurrent flow apparatus. The PET is rapidly glycolysed to a brittle composition of BHET and oligomers. This brittle flake is then crushed and separated from other coarse impurities, such as PVC. It is further purified by settling methods before hydrolysis to crude TA. The process, which claimed to use relatively crude PET bottle scrap, was known as the 'RENEW process [38 J. Methods of recovering TA by hydrolysis techniques nearly always fail on the issue of repurification of the TA. The PET waste arises from many sources and contains variable quantities of impurities, which pass into the crude product. Attempting to match virgin quality is very difficult without excessive quality control procedures, which are complex and costly. Improvements to the process technology are still being attempted. PET waste is first hydrolysed with an excess of pure water at ca 250'C/autoclave, and the crude TA is then hydrogenated at 280CC using a palladium/carbon catalyst. However, viable and competitive commercial processes are some way off (for a good description of the prior art see ).
Environmental benefits of recycling
Recycling is assumed to deliver environmental benefits in terms of material savings. The appropriate technique for measuring these savings is termed 'life cycle assessment' (LCA). LCA is a technique that catalogues all the environmental aspects associated with a product or, more specifically, the processes used to produce the product or provide the service. The catalogue (inventory) is then used to assess the impact of those aspects on the environment. The procedure is similar to a financial audit but examines the environmental viability of a process. An LCA is useful because it collects all available environmental factors from the time resources are extracted from nature to the time when the resources are returned back to nature, a so called 'cradle to grave' process. For example, total energy consumed and emissions generated to air, water and earth during product manufacture, use and disposal. The EU Packaging and Packaging Waste Directive, 94/62/EC, refers to the use of LCA techniques for use in examining achievements towards the
ENVIRONMENTAL AND RECYCLING CONSIDERATIONS
environmental targets set in the directive with the clear intention of determining a programme of regulation. Following from these initiatives, an LCA international standard ISO 14040 , now exists which defines how LCAs should be completed, verified and used. In many instances, the environmental benefits are immediately obvious with limited analysis; for example, in the case of aluminium recycling the whole process of recovery and recycling uses about 10% of the energy used to extract virgin aluminium from its ores. A simple energy analysis suffices if the major judgement criteria are energy consumption and emissions to air/water/land— most emissions arise from burning of fuels and extraction of ores. In other cases, the savings are not always so clearly delineated and careful assessment of a wider range of parameters is necessary. 11.7.1 General principles of recycling (adapted from Boustead [40J) There are essentially two types of recycling: 'closed loop' recycling classifies those processes which recover and reprocess material and feed it back into the same production system, and 'open loop' recycling classifies processes which recover and reprocess material then feed it to a different production process. PET 'bottle-to-bottle' recycling is an example of closed loop recycling; and using recycled PET from used bottles to manufacture fibres, rigid sheet, film or engineering PET plastics are examples of open loop recycling. Closed loop recycling is probably the simplest form. It is illustrated schematically in Figure 11.8, which shows a simple linear production sequence consisting of three unit operations, labelled: Production (1), Use (2) and Disposal (3). A recycling loop (4) is included, in which some of the waste materials are extracted from the system, reprocessed and fed back into the same production sequence to displace virgin raw materials. Materialflows. Assume that all of the operations operate without loss of material and that the consumer is located somewhere in operation 2. The saving in raw materials due to recycling can be calculated. Assume also that/is the fraction of the waste leaving operation 2 that is reprocessed and returned to the main production sequence. If the recycling loop was absent (i.e. / — 0), then normal operations would see a mass flow (m) moving through the sequence. With the recycling loop in place, the consumer in operation 2 will still see a product of mass, m, flowing past. However, the raw materials input to operation 1 has been reduced from m to m(\ — /) and the solid waste entering operation 3 has also been reduced from m to m(\ — /). Therefore, as a consequence of introducing the recycling loop, both the demand for raw materials and the solid waste generated have been reduced. Even if an allowance is made for material loss in all of the operations, the same general conclusion will apply.
Recycle process loop (4)
Figure 11.8 Simple production sequence when a closed recycling loop is included. For explanation see Section I 1.7.1.
ENVIRONMENTAL AND RECYCLING CONSIDERATIONS
An alternative way of viewing this effect is to suppose that a single mass, m, is fed into operation 1 in Figure 11.8 and then monitor the quantity of product that will pass the consumer as some fraction of this initial mass is repeatedly recycled. On the first pass, the product mass will be m. After the first recycle, the mass will be mf. At the second recycle it will be m/ 2 and so on. Thus, after an infinite number of recycles, the consumer will have experienced a total mass, M, of product passing through, where:
M = m + mf + mf2 + w/ 3 + mf4 + and summing this series gives: M = m/(l - /)
Thus, if there is no recycling,/will be zero and M = m. However, say 50% of the materials leaving operation 2 is recycled, then / — 0.5 and M = 2, so that for an input of 1 kg of material, the consumer will experience 2 kg of product. Similarly, with 90% recycling, / = 0.9 and M = 10, so that an input of 1 kg of raw material will lead to the passage of 10kg of product. In all of these cases, the amount of solid waste generated will remain at 1 kg, irrespective of the mass of product passing the consumer. Thus, if the aim of recycling is to minimise consumption of raw materials and generation of solid waste, then the goal should be to try and achieve the highest recycling rate possible. Energy flows. The energy needed to drive the systems shown in Figure 11.8 presents a more complicated picture than the raw materials flows. To evaluate these energies, suppose that the energy requirement per unit output for each of the unit operations 1 to 4 is: E\, £2, £3 and £4, respectively; thus, E\ is the energy required by operation 1 to give an output of 1 kg from operation 1, and so on. For the system of Figure 11.8 where no recycling occurs (i.e. / = 0), the system energy, Es, is given by: Es — m • E\ + m • £2 + w • £3 = m(E\ + £2 + £3)
The system energy with recycling will be E^ where: E; = (1 - /)mE| + mE2 + (I - ,/)m£ 3 + /m£ 4 and this rearranges to: E( = m(El + E2 + £3) + fm(E4 - E} - £3)
Using equation (1), this can be rewritten as: E; = Es + /HI (£4 - El ~ £ 3 )
PET PACKAGING TECHNOLOGY
If the energy change introduced as a result of incorporating the recycling loop is written as A£ s , where: then, from Equation (3): A£s = /m(£, + £ 3 - £ 4 )
If the righthand side of this equation is positive, then there will be energy savings. However, if the term is negative, then the recycling loop will have incurred a net expenditure of additional energy. The critical condition, which determines whether energy will be saved or lost in recycling, is the value of £4 relative to the sum of £"1 and £3. Note that that this general conclusion does not change if there are material losses from the recycling loop as would occur in a real recycling operation. For the recycling of post-consumer waste, operation 1 in Figure 1 1 .8 will represent all processes starting with the extraction of raw materials from the earth through to the production and delivery of a material at the converter. Operation 3 will represent all materials handling operations that occur after the consumer has finished with the product at the end of its useful life, and in most systems represents the collection and disposal of waste. In general, the energy associated with operation 3 will be small compared with the energy associated with operation 1 . Consequently, provided that the materials can be collected. reprocessed and delivered to the converter with an energy requirement less than that needed to produce virgin materials via operation 1 , then an energy saving will occur. One important consequence flows from this conclusion. As the production of virgin materials is made increasingly more energy efficient by improved manufacturing techniques, the scope for energy saving by recycling is gradually diminished because the parameter E\ in Equation (4) is decreased relative to £4. Conversely, when recycling is made more energy efficient, as for example through improved waste collection, larger amounts of material can be recycled without loss of energy. 11.7.2 Application of the general principles to the recovery and recycling of PET bottles To simplify the illustration, only the energy parameter is discussed in the following section and emissions to the environment are not included. However this does not mean that these factors should be ignored; other assessments of the viability of recycling processes may rank emissions higher than energy consumption —for example, global warming gases may take priority. Figure 11.9 illustrates typical PET-user chains through extraction of oil. manufacture of products (i.e. bottles, fibre or engineering plastics), through the
Figure 11.9 Typical PET material user chains with material recycling loop and route to energy recovery. Abbreviations: PTA, pure terephthalic acid; EG, ethylene glycol; PET, polyethylene terephthalate; DMT, dimethyl terephthalate.
PET PACKAGING TECHNOLOGY
use operation and eventually to final disposal. Also included are a recycling loop, and an indication that the used products can be a possible energy source. Considering recycling of PET bottles, the recycling loop collects the used bottles, progresses them through the sequence of sorting, followed by washing and cleaning to a usable flake before returning the recovered PET back into the user chain immediately prior to the manufacture of more bottles. The lighter grey block delineates the boundary of this process. The recycling loop also illustrates the additional or alternative step of recovery by solvolytic processes; in this case the PET is broken down into its intermediates before returning into the user chain prior to manufacture of the PET polymer. This additional step is delineated by the extension of the boundary, including the darker grey area. The three basic operations of production, use and disposal are easily discerned. The closed loop example would be the 'bottle-to-bottle' sequence and the open loop example the use of R-PET in the other sequences for fibre and engineering plastics manufacture. It can also be seen from Figure 11.9 that the recycling loop is split into three main operations: collection, sorting and delivery to the recycler, washing and cleaning of the flake, and the more complex solvolytic recovery process. It is possible that used bottles can be fed directly into the solvolytic processes without prior cleaning. However, this is not usual at the present stage of developments and some prior washing is assumed. 184.108.40.206 Potential energy savings Before one can consider the reprocessing options, it is appropriate to look at what potential energy savings are possible. In principle, collection, reprocessing and reintroduction of recycled PET material will directly displace virgin materials from the consumption chain. It is this displacement value that is the driving force for recycling operations. In Figure 11.9 the chain from oil to PET polymer is represented by only three stages. In actual fact, there are about 13-14 stages. The full sequence of operations outlined in Figure 11.10 consumes a total of 77 MJ for every kg of bottle-grade PET produced [41 ]. This total is made up of 39 MJ as 'feedstock' and 38 MJ as fuels consumed to drive the process. The feedstock is the organic equivalent to the inorganic glass in bottles or the aluminium metal in cans and is carried through the recycling process as material equivalent before re-entering the user chain again as regenerated PET polymer. Put another way, 38 MJ of fuels are consumed to deliver 1 kg of virgin polymer to the bottle preparation process. Any recovery and recycling operations that deliver R-PET back to the bottle production process should, therefore, consume less than 38 MJ if savings are to be achieved. It should be noted that these values will continue to fall as manufacturing technology improves. In the early 1980s, intermediates plants usually had operating capacities of 100,000-150,000 tonnes per annum. Such plants, installed today, will have operating capacities of > 250,000 tonnes per annum Similar changes
ENVIRONMENTAL AND RECYCLING CONSIDERATIONS
Oil refining I
Oil production & delivery
naptha Natural gas production & delivery
I DMT production & purification
Solid state polymerisation Crystalline PET Figure 11.10 Full sequence of operations to produce virgin PET polymer. Abbreviations: DMT, dimethyl terephlhalate; TA, terephthalic acid; PTA, pure terephthalic acid; BHET, bis(hydroxyethyl) terephthalate.
are noted with polymerisation capacity; > 150,000 tonnes per annum units are in operation today, an advance on older 50,000 tonnes per annum capacity plants. These unit size changes and technology improvements increase efficiencies enormously, especially energy utilisation. It is these factors that have allowed the price of PET to remain virtually unchanged over the last 15-20 years and reduced the energy consumption to the low figures we see today. Some historical total energy consumption figures for manufacture of PET are presented in Table 11.6. It should also be noted that the figure of 77 MJ/kg represents an average value and in reality there will be a range dependent on a number of factors. Plant size, occupational capacity and efficiencies are factors that are well understood. What is not well understood are the other influencing factors related to use of oil or gas as the principal raw material and the national power supply systems in the country of manufacture. For example, if gas is used as primary feedstock to make the PET polymer, the overall energy contributions will be higher than if oil was used, simply because gas has a higher calorific value. One kilogram of carbon from methane will require a feedstock energy of 72 MJ compared to 1 kg of carbon from oil of feedstock energy 59 MJ (i.e. pentane as an example of naphtha). Similar but smaller differences are seen if all the electrical power is derived from
PET PACKAGING TECHNOLOGY Table 11.6 Total energy values for manufacture of PET polymer Reference Boustead - 1982  Franklin Associates - 1980  Boustead - 1989, 1993  Franklin Associates - 1992  BUWAL 132 - 1990 [45 ] APME- 1995  APME-2000
Energy (MJ/kg) 150 123-127 128-135 89 ca 70 84 77
hydro-power compared to power generated from relatively inefficient coal fuels. It is beyond the scope of this article to describe these differences in detail and the reader should refer to the methodology used in compiling the APME eco-profile reports for a more thorough discourse of the subject . 220.127.116.11 Fuels and feedstocks In the above theoretical analysis, materials flows have been illustrated separately from energy flows and the final consequences of recycling are shown to be different for these two different parameters. In general, recycling will always result in a reduction in consumption of raw materials and generation of solid waste per unit product at the consumer. For energy, however, there is no guarantee that savings will occur when recycling is practised. The energy changes resulting from recycling are governed by a number of different parameters and only when certain well-defined conditions are satisfied will energy savings occur. For products manufactured from inorganic materials, raw materials consumption is invariably kept separate from the consumption of fuels. The units in which they are measured are different and there is therefore no temptation to try and combine the two. For polymers, and other materials based on combustible feedstocks, such as wood products, the raw materials input, measured as the feedstock energy, can be measured in mass terms but is often expressed in the same units as the fuel energy. Consequently, there is frequently the desire to combine the two contributions into a single parameter for simplicity. This, however, should be avoided. The effect of recycling on feedstock energy follows the treatment given earlier for materials flows, whereas the treatment for fuel energy follows that given for energy and, as noted earlier, they are different. Only if the material is ultimately thrown away as waste, without energy recovery, is it meaningful to add together fuel and feedstock energies as a description of the total energy resource that must be extracted from the earth. It is also important to distinguish between two different types of recycling processes for plastics: mechanical recycling and energy recovery. Mechanical recycling is the recovery of plastics for further use as materials. This form of
ENVIRONMENTAL AND RECYCLING CONSIDERATIONS
recycling is available to all other materials. The environmental benefits arise from the ability to spread the initial material production energy over several uses (shown in the earlier analysis as mass flows through the consumer). Energy recovery is the recovery of the feedstock energy (or a proportion of it) for use as a fuel. In other words, it is the conversion of feedstock to fuel. This option is available to relatively few materials; plastics and wood products are the most obvious examples. These two recovery options are complementary; they are not mutually exclusive. Consequently, recycling should not be regarded as a choice between mechanical recycling or energy recovery, since both are possible for the same material. 18.104.22.168 Collection of bottles Obviously, before we can reprocess we need a supply of collected bottles. The energy associated with collection is very often accounted for in a social context and as part of the duty carried out by local authorities in connection with waste disposal operations. This figure can be extremely variable; however, if recycling is being operated with the intention to save overall resource, then energy expended on collection must be factored into the calculations. One source of information on energy consumed during collection comes from a study from the Netherlands on plastic waste management options . Five different collection models were studied, consuming 3-4 MJ/kg for collection, some pretreatment separation and delivery to the processing plant. These models are noted as: • • • • •
collect integral with MSW and ship to MSW combustion plant kerbside separate collection of 100% of plastics as part of MSW scheme and transport to separation plant kerbside collection of 95.9% plastics as in 2; collect 4.1% separately as bottles kerbside collection of plastics/metals/drinks cartons (PMD) kerbside collection of 54% of all plastics and 46% with MSW; delivery to feedstock recycling
Note: the lowest energy option is not to collect, separate, measure the yields and deliver to the recyclers but to collect and deliver straight to an energy recovery facility fca 1.5 MJ/kg). This latter figure could be a realistic representation of a very basic minimum figure, which could be achieved if all that was needed was to collect and prepare 100% PET bottles then delivery to a processing site. These figures are probably representative of the better-developed schemes. There are schemes at earlier stages of development that reflect higher energy figures. Certainly, those with a higher proportion of drop-off collection points and rural areas would expect to consume more energy.
Studies executed for APME  indicate collection energies from 0.2 to 1.2MJ/kg for systems covering collection with MSW to separate green bin collection of all plastic bottles. Rural area collections can be up to 5-6 times more energy intensive. Other data  suggest collection energy figures of up to 15 MJ/kg (including sorting) and also give some indication that volumes from urban collections can be up to seven times more effective in yield when compared to collections from rural areas. These figures suggest that sensible collection schemes for recyclables should be developed, which are not too ambitious. Simply setting goals of 80-90% recovery when the best available information says less than half of this is achievable is guaranteed to fail. To obtain the correct balance demands careful analysis before compiling a programme. Figure 11.11, which illustrates the general case of total system energy, shows how the balance will change as a programme becomes more successful and recovery of the last remaining material shifts the efficiency of the exercise. Trying to recover the last 5% when the recovery rate is already 95% would require that every last container, including those taken away by overseas holidaymakers, be recovered. Clearly this is impractical but it underlines the fact that at very high recovery rates, the recovery energy would certainly be increasing steeply. As a consequence, the actual relationship between total system energy and recycled fraction is most likely to be a curve, such as that shown schematically. Application of Pareto analysis to target the major effects is recommended and a careful audit of environmental cost, in addition to the normal economic cost, carried out on a regular basis.
0% Recycled fraction
Figure 11.11 System energy as a function of recycled fraction when all of the energy terms are constant.
ENVIRONMENTAL AND RECYCLING CONSIDERATIONS
It is clear (from Figure 11.11) that if the overall recycling process is not to use more energy than the process without recycling, then the recycled fraction should not increase above f\. It can also be deduced that if the recycling target is to actually save energy, then recycling should be practised only until the total energy curve reaches the minimum of Figure 11.11; that is, until the recycling fraction reaches fa. The importance of this is that recycling targets or collection targets should not be set arbitrarily. If energy savings are a target for any recycling process, then the primary aim should be either to establish the form of the curve in Figure 11.11 so that the limits f\ and fa can be determined or to establish the condition set by Equation (4), so that energy is not wasted. 22.214.171.124 Reprocessing of the collected bottles Depending on the type of recycling process used, the reprocessed bottles could be introduced back into the chain either as a clean washed polymer flake, as partly polymerised PET (BHET from glycolysis) or as the recovered intermediates, DMT (from methanolysis), PTA and EG (from hydrolytic processes). Reprocessing of the collected containers can be carried out in several ways, but the procedures illustrated in Table 11.7 usually follow the delivery of bottles to the processing plant. For the purposes of this discussion, only the methods of recovery back to a reusable polymer are considered. Associated with the description 'a collected PET bottle' are labels, caps, residues from the contents and other soil depending on method of collection and storage. This associated detritus can amount to 50% of the total weight. As bottles are engineered lighter, this ratio generally increases. Separation and preparation before final reprocessing can make very variable demands on energy input. This is particularly so with methanolysis and glycolysis. Some hydrolytic processes claim an advantage by being able to use highly contaminated feedstock needing a minimum of pretreatment. Good quality used PET bottle input is essential for efficient reprocessing. There is also another option, which should not be ignored for lower quality materials unsuitable for mechanical recycling. PET has an intrinsic energy value equivalent to that of soft coal (i.e. 23 MJ/kg) or approximately half that of fuel oils. Hydrocarbon fuel oils have values of ca 40-45 MJ/kg. PET does burn in a clean manner and can be used as an effective fuel substitute. If energy recovery
Table 11.7 Energy consumption for PET recovery processes Method of recovery Reprocessing to clean PET flake Hydrolytic processes to PET Methanolysis/glycolysis to PET
Approximate energy consumption (MJ/kg)
6-15 20-30 24-38
[42-451  [43, 44. 50]
PET PACKAGING TECHNOLOGY
Table 11.8 Summary of potential energy savings (MJ/kg) from recycling of PET
Washing to flake Hydrolysis Glycolysis/ methanolysis Energy
Energy for reprocessing
Energy for total 'waste management'
Potential savings— from displacement of virgin PET